#------------------------------------------------------------------------------
#$Date: 2025-07-06 16:07:54 +0300 (Sun, 06 Jul 2025) $
#$Revision: 300450 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/13/43/7134380.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7134380
loop_
_publ_author_name
'Guo, Haiyang'
'He, Donglin'
'Long, De-Liang'
'Cronin, Leroy'
_publ_section_title
;
 Robotic exploration of amino-acid functionalised molybdenum blue
 polyoxometalate nanoclusters
;
_journal_issue                   39
_journal_name_full               'Chemical Communications'
_journal_page_first              7121
_journal_page_last               7124
_journal_paper_doi               10.1039/D5CC00703H
_journal_volume                  61
_journal_year                    2025
_chemical_formula_sum            'C126 H1332 Mo308 N14 Na12 O1519'
_chemical_formula_weight         57181.38
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2019/3
_audit_update_record
;
2025-01-29 deposited with the CCDC.	2025-04-04 downloaded from the CCDC.
;
_cell_angle_alpha                93.9010(10)
_cell_angle_beta                 94.7110(10)
_cell_angle_gamma                95.1660(10)
_cell_formula_units_Z            1
_cell_length_a                   30.4172(2)
_cell_length_b                   34.0113(2)
_cell_length_c                   46.8336(2)
_cell_measurement_reflns_used    446824
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      25.28
_cell_measurement_theta_min      2.30
_cell_volume                     47951.8(5)
_computing_cell_refinement       'CrysAlisPro 1.171.41.111a (Rigaku OD, 2021)'
_computing_data_collection       'CrysAlisPro 1.171.41.111a (Rigaku OD, 2021)'
_computing_data_reduction        'CrysAlisPro 1.171.41.111a (Rigaku OD, 2021)'
_computing_molecular_graphics    Diamond3
_computing_publication_material  WinGX
_computing_structure_refinement  'SHELXL-2019/2 (Sheldrick, 2019)'
_computing_structure_solution    'SHELXT-2019/2 (Sheldrick, 2019)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            'HyPix-Arc 150'
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy R, HyPix-Arc 150'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0661
_diffrn_reflns_av_unetI/netI     0.0307
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       40
_diffrn_reflns_limit_k_min       -40
_diffrn_reflns_limit_l_max       55
_diffrn_reflns_limit_l_min       -55
_diffrn_reflns_number            1816573
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.068
_diffrn_reflns_theta_max         25.068
_diffrn_reflns_theta_min         2.200
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'Mova (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    2.038
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.691
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.67a (Rigaku Oxford Diffraction, 2022)
Numerical absorption correction based on gaussian integration over
a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'Dark blue'
_exptl_crystal_density_diffrn    1.980
_exptl_crystal_density_method    none
_exptl_crystal_description       block
_exptl_crystal_F_000             27406
_exptl_crystal_size_max          0.136
_exptl_crystal_size_mid          0.105
_exptl_crystal_size_min          0.020
_refine_diff_density_max         2.10
_refine_diff_density_min         -1.89
_refine_diff_density_rms         0.15
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     6438
_refine_ls_number_reflns         169615
_refine_ls_number_restraints     310
_refine_ls_restrained_S_all      1.031
_refine_ls_R_factor_all          0.0722
_refine_ls_R_factor_gt           0.0509
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0837P)²+263.5025P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1427
_refine_ls_wR_factor_ref         0.1578
_reflns_Friedel_coverage         0.000
_reflns_number_gt                127073
_reflns_number_total             169615
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d5cc00703h2.cif
_cod_data_source_block           ghy025_sq
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'direct methods' was
changed to 'direct'.

data item '_atom_sites_solution_secondary' value 'diffmap' was
changed to 'difmap'.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 

 Adding full bibliography for 7134378--7134381.cif.
;
_cod_database_code               7134380
_shelx_shelxl_version_number     2019/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.769
_shelx_estimated_absorpt_t_max   0.960
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1A Mo 0.20329(2) 0.80183(2) 0.90848(2) 0.03985(16) Uani 1 1 d . . . . .
Mo1B Mo 0.61949(3) 0.82931(2) 0.84369(2) 0.04361(17) Uani 1 1 d . . . . .
Mo1C Mo 0.76432(2) 0.60417(2) 0.76346(2) 0.04641(17) Uani 1 1 d . . . . .
Mo1D Mo 0.41189(3) 0.89043(2) 0.98748(2) 0.04109(16) Uani 1 1 d . . . . .
Mo1E Mo 0.22128(3) 0.89471(2) 1.01460(2) 0.04155(16) Uani 1 1 d . . . . .
Mo1F Mo 0.19450(3) 0.79126(2) 1.10578(2) 0.04340(16) Uani 1 1 d . . . . .
Mo1G Mo 0.84218(2) 0.77755(2) 0.87006(2) 0.04139(16) Uani 1 1 d . . . . .
Mo1H Mo 0.58517(3) 0.89301(2) 0.92683(2) 0.04458(17) Uani 1 1 d . . . . .
Mo1I Mo 0.15627(3) 0.57998(2) 0.33893(2) 0.04377(17) Uani 1 1 d . . . . .
Mo1J Mo 0.42997(3) 0.80276(2) 0.67456(2) 0.04342(17) Uani 1 1 d . . . . .
Mo1K Mo 0.27043(3) 0.83601(2) 0.96876(2) 0.04455(17) Uani 1 1 d . . . . .
Mo1L Mo 0.34752(2) 0.84374(2) 0.70120(2) 0.04067(16) Uani 1 1 d . . . . .
Mo1M Mo 0.14840(3) 0.73863(2) 0.94759(2) 0.04244(16) Uani 1 1 d . . . . .
Mo1N Mo -0.12496(3) 1.34019(2) 0.68874(2) 0.04279(17) Uani 1 1 d . . . . .
Mo1O Mo 0.31649(2) 0.93086(2) 0.72484(2) 0.04399(17) Uani 1 1 d . . . . .
Mo1P Mo 0.29166(2) 0.80239(2) 0.87096(2) 0.04274(16) Uani 1 1 d . . . . .
Mo1Q Mo 0.14622(2) 0.73652(2) 1.04555(2) 0.04304(16) Uani 1 1 d . . . . .
Mo1R Mo 0.06281(3) 0.39761(2) 1.01090(2) 0.04802(19) Uani 1 1 d . . . . .
Mo1S Mo 0.51561(3) 0.70034(2) 0.78257(2) 0.05140(19) Uani 1 1 d . . . . .
Mo1T Mo -0.00944(3) 0.54611(2) 0.33760(2) 0.04717(18) Uani 1 1 d . . . . .
Mo1U Mo -0.03456(3) 1.30060(2) 0.71412(2) 0.04605(18) Uani 1 1 d . . . . .
Mo1V Mo 0.10962(3) 1.42947(2) 0.70460(2) 0.04782(18) Uani 1 1 d . . . . .
Mo1W Mo 0.21443(3) 1.37981(2) 0.73241(2) 0.05095(19) Uani 1 1 d . . . . .
Mo1X Mo 0.34352(3) 0.64531(2) 0.56244(2) 0.04877(19) Uani 1 1 d . . . . .
Mo1Y Mo 0.43327(3) 0.86661(2) 0.55633(2) 0.04975(18) Uani 1 1 d . . . . .
Mo1Z Mo 0.49065(3) 0.94701(2) 0.67237(2) 0.04552(17) Uani 1 1 d . . . . .
Mo2A Mo 0.40745(3) 0.68592(2) 0.51546(2) 0.04989(19) Uani 1 1 d . . . . .
Mo2B Mo 0.48586(2) 0.85184(2) 0.62747(2) 0.04595(17) Uani 1 1 d . . . . .
Mo2C Mo 0.34406(3) 0.74459(2) 0.55959(2) 0.04989(18) Uani 1 1 d . . . . .
Mo2D Mo 0.41765(3) 0.78205(3) 0.51477(2) 0.05095(19) Uani 1 1 d . . . . .
Mo2E Mo 0.17510(3) 0.59243(2) 0.49891(2) 0.04955(19) Uani 1 1 d . . . . .
Mo2F Mo 0.43813(3) 1.14373(2) 0.73679(2) 0.05236(19) Uani 1 1 d . . . . .
Mo2G Mo 0.28168(3) 0.58733(2) 0.50023(2) 0.04918(19) Uani 1 1 d . . . . .
Mo2H Mo 0.47761(3) 1.04199(2) 0.71184(2) 0.04814(18) Uani 1 1 d . . . . .
Mo2I Mo 0.39531(3) 0.89255(3) 0.64865(2) 0.05158(19) Uani 1 1 d . . . . .
Mo2J Mo 0.06750(4) 0.50644(2) 1.01073(2) 0.0634(3) Uani 1 1 d . . . . .
Mo2K Mo 0.06222(3) 0.62410(2) 0.36274(2) 0.0533(2) Uani 1 1 d . . . . .
Mo2L Mo 0.27021(3) 0.83086(3) 1.06583(2) 0.0564(2) Uani 1 1 d . . . . .
Mo2M Mo 0.46013(3) 0.76251(2) 0.57780(2) 0.04809(18) Uani 1 1 d . . . . .
Mo2N Mo 0.30634(3) 0.77219(3) 0.65148(2) 0.05224(19) Uani 1 1 d . . . . .
Mo2O Mo 0.21701(3) 1.17749(2) 0.78577(2) 0.0546(2) Uani 1 1 d . . . . .
Mo2P Mo 0.25420(3) 1.08985(2) 0.76996(2) 0.0571(2) Uani 1 1 d . . . . .
Mo2Q Mo 0.11241(3) 1.32492(2) 0.70574(2) 0.0553(2) Uani 1 1 d . . . . .
Mo2R Mo 0.23844(3) 0.84214(3) 0.69187(2) 0.0546(2) Uani 1 1 d . . . . .
Mo2S Mo 0.82014(3) 0.75464(3) 0.93520(2) 0.0579(2) Uani 1 1 d . . . . .
Mo2T Mo 0.33683(3) 0.63684(2) 0.45319(2) 0.05130(19) Uani 1 1 d . . . . .
Mo2U Mo 0.30199(3) 1.31223(2) 0.74122(2) 0.0550(2) Uani 1 1 d . . . . .
Mo2V Mo 0.32484(3) 1.18907(2) 0.79372(2) 0.0526(2) Uani 1 1 d . . . . .
Mo2W Mo 0.22889(3) 0.65102(2) 0.45409(2) 0.05268(19) Uani 1 1 d . . . . .
Mo2X Mo 0.21771(3) 0.70982(2) 0.88663(2) 0.0603(2) Uani 1 1 d . . . . .
Mo2Y Mo 0.20844(3) 0.68648(2) 0.36146(2) 0.0561(2) Uani 1 1 d . . . . .
Mo2Z Mo 0.36350(3) 1.05901(3) 0.71170(2) 0.0551(2) Uani 1 1 d . . . . .
Mo3A Mo 0.34771(3) 0.74522(3) 0.45889(2) 0.0619(2) Uani 1 1 d . . . . .
Mo3B Mo -0.08542(3) 0.60337(3) 0.37611(2) 0.0633(2) Uani 1 1 d . . . . .
Mo3C Mo 0.43856(4) 1.02098(3) 0.63139(2) 0.0644(3) Uani 1 1 d . . . . .
Mo3D Mo 0.37932(4) 0.85512(3) 0.48031(2) 0.0761(3) Uani 1 1 d . . . . .
Mo3E Mo 0.29317(3) 0.76509(4) 1.12698(2) 0.0805(3) Uani 1 1 d . . . . .
Mo3F Mo 0.24932(4) 1.31581(3) 0.66836(2) 0.0673(3) Uani 1 1 d . . . . .
Mo3G Mo 0.19522(3) 0.91474(3) 0.74289(2) 0.0631(2) Uani 1 1 d . . . . .
Mo3H Mo 0.09941(3) 0.63649(3) 0.53242(2) 0.0662(3) Uani 0.95 1 d . . P . .
Mo3I Mo 0.71650(4) 0.38919(4) 0.77770(3) 0.0604(3) Uani 0.85 1 d . U P A 1
Mo3J Mo 0.37351(4) 1.18154(3) 0.67109(2) 0.0706(3) Uani 1 1 d . . . . .
Mo3K Mo 0.13314(3) 1.11071(3) 0.76529(3) 0.0860(4) Uani 1 1 d . . . . .
Mo3L Mo 0.18490(5) 0.74160(4) 0.66462(3) 0.0652(3) Uani 0.9 1 d . U P B 1
Mo3M Mo 0.39740(3) 0.69834(3) 0.79639(3) 0.0782(3) Uani 1 1 d . . . . .
Mo3N Mo 0.07961(3) 0.56424(3) 0.94770(2) 0.0425(2) Uani 0.8 1 d . . P E .
Mo3O Mo -0.06956(3) 1.19273(3) 0.72976(2) 0.0696(3) Uani 1 1 d . . . . .
Mo3P Mo 0.18132(4) 1.34098(4) 0.60062(2) 0.0781(3) Uani 0.95 1 d . . P . .
Mo3Q Mo 0.30107(5) 0.70047(3) 0.83444(4) 0.1148(6) Uani 1 1 d . . . . .
Mo3R Mo 0.75222(5) 0.82599(6) 0.97118(2) 0.0949(5) Uani 0.9 1 d . U P C 1
Mo3S Mo 0.43283(5) 0.95499(3) 0.50890(2) 0.0689(3) Uani 0.85 1 d . U P D 1
Mo3T Mo 0.38862(7) 1.11307(5) 0.60530(3) 0.0950(5) Uani 0.9 1 d . U P D 1
Mo3U Mo 0.65502(7) 0.86545(8) 0.99237(4) 0.0979(8) Uani 0.8 1 d . U P C 1
Mo3V Mo 0.25774(4) 0.79114(3) 0.34827(2) 0.0852(3) Uani 1 1 d . . . . .
Mo3W Mo 0.13749(5) 0.67217(5) 0.60791(3) 0.0893(5) Uani 0.9 1 d . U P B 1
Mo3X Mo 0.13040(7) 0.63526(5) 0.90576(4) 0.0568(4) Uani 0.65 1 d . U P E 1
Mo3Y Mo -0.01498(4) 0.60608(5) 0.50050(2) 0.0943(4) Uani 0.9 1 d . . P H .
Mo3Z Mo 0.02663(4) 1.14799(3) 0.75262(4) 0.1167(6) Uani 1 1 d . . . . .
Mo4A Mo 0.34206(2) 0.90265(2) 0.86499(2) 0.03299(14) Uani 1 1 d . . . . .
Mo4B Mo -0.00389(2) 0.53806(2) 1.12931(2) 0.03153(13) Uani 1 1 d . . . . .
Mo4C Mo 0.98695(2) 0.56116(2) 0.84776(2) 0.03249(14) Uani 1 1 d . . . . .
Mo4D Mo 0.03611(2) 0.71688(2) 1.04599(2) 0.03449(14) Uani 1 1 d . . . . .
Mo4E Mo 0.82857(2) 0.44881(2) 0.80267(2) 0.03665(15) Uani 1 1 d . . . . .
Mo4F Mo -0.04950(2) 0.53950(2) 0.91826(2) 0.03407(14) Uani 1 1 d . . . . .
Mo4G Mo 0.06679(2) 0.67865(2) 1.14856(2) 0.03478(14) Uani 1 1 d . . . . .
Mo4H Mo 0.83198(2) 0.53325(2) 0.77098(2) 0.03617(15) Uani 1 1 d . . . . .
Mo4I Mo 0.56301(2) 0.79128(2) 0.78055(2) 0.03668(15) Uani 1 1 d . . . . .
Mo4J Mo 0.47198(2) 0.79555(2) 0.81502(2) 0.03446(14) Uani 1 1 d . . . . .
Mo4K Mo 0.06510(2) 0.61812(2) 1.02246(2) 0.03856(15) Uani 1 1 d . . . . .
Mo4L Mo 0.71371(2) 0.88438(2) 0.83448(2) 0.04040(16) Uani 1 1 d . . . . .
Mo4M Mo 0.08864(2) 0.76410(2) 1.10556(2) 0.03692(15) Uani 1 1 d . . . . .
Mo4N Mo 0.08835(2) 0.79085(2) 1.00078(2) 0.03718(15) Uani 1 1 d . . . . .
Mo4O Mo 0.49070(2) 0.92297(2) 0.94684(2) 0.03564(14) Uani 1 1 d . . . . .
Mo4P Mo 0.89346(2) 0.61553(2) 0.76709(2) 0.03625(15) Uani 1 1 d . . . . .
Mo4Q Mo 0.43286(3) 0.86384(2) 0.89179(2) 0.04013(16) Uani 1 1 d . . . . .
Mo4R Mo 0.65840(2) 0.84061(2) 0.77447(2) 0.03845(15) Uani 1 1 d . . . . .
Mo4S Mo 0.09844(2) 0.59292(2) 1.11999(2) 0.03901(15) Uani 1 1 d . . . . .
Mo4T Mo 0.87925(2) 0.57785(2) 0.83507(2) 0.04032(16) Uani 1 1 d . . . . .
Mo4U Mo 0.14396(2) 0.84124(2) 1.05838(2) 0.03993(16) Uani 1 1 d . . . . .
Mo4V Mo 0.15725(2) 0.85342(2) 0.95719(2) 0.03912(15) Uani 1 1 d . . . . .
Mo4W Mo 0.63708(2) 0.72621(2) 0.77127(2) 0.04458(17) Uani 1 1 d . . . . .
Mo4X Mo 0.24721(2) 0.89327(2) 0.90919(2) 0.03695(15) Uani 1 1 d . . . . .
Mo4Y Mo 0.88997(2) 0.69695(2) 0.88709(2) 0.03967(16) Uani 1 1 d . . . . .
Mo4Z Mo 0.82724(2) 0.70003(2) 0.75810(2) 0.04030(16) Uani 1 1 d . . . . .
Mo10 Mo 0.61082(2) 0.92608(2) 0.85706(2) 0.03668(15) Uani 1 1 d . . . . .
Mo11 Mo 0.43653(2) 0.90302(2) 0.72229(2) 0.03948(16) Uani 1 1 d . . . . .
Mo12 Mo 0.80609(2) 0.82658(2) 0.81676(2) 0.04069(16) Uani 1 1 d . . . . .
Mo13 Mo -0.04891(3) 1.41189(2) 0.71126(2) 0.04073(16) Uani 1 1 d . . . . .
Mo14 Mo 0.41149(3) 0.99847(2) 0.75590(2) 0.04308(17) Uani 1 1 d . . . . .
Mo15 Mo 0.74624(2) 0.77558(2) 0.76119(2) 0.04006(16) Uani 1 1 d . . . . .
Mo16 Mo 0.05038(3) 1.37667(2) 0.74771(2) 0.04280(16) Uani 1 1 d . . . . .
Mo17 Mo 0.89066(2) 0.74611(2) 0.81448(2) 0.03961(16) Uani 1 1 d . . . . .
Mo18 Mo 0.30767(2) 0.93230(2) 0.96868(2) 0.03864(15) Uani 1 1 d . . . . .
Mo19 Mo 0.77466(2) 0.72344(2) 0.81715(2) 0.04296(16) Uani 1 1 d . . . . .
Mo20 Mo 0.09269(3) 0.53801(2) 0.38556(2) 0.04674(18) Uani 1 1 d . . . . .
Mo21 Mo 0.75444(3) 0.82158(3) 0.88917(2) 0.0515(2) Uani 1 1 d . . . . .
Mo22 Mo 0.24485(3) 1.27268(2) 0.79191(2) 0.05136(19) Uani 1 1 d . . . . .
Mo23 Mo 0.15050(3) 1.33061(2) 0.77540(2) 0.04747(18) Uani 1 1 d . . . . .
Mo24 Mo 0.37504(3) 1.09557(2) 0.78083(2) 0.04769(18) Uani 1 1 d . . . . .
Mo25 Mo 0.25186(3) 0.60099(2) 0.39328(2) 0.04829(18) Uani 1 1 d . . . . .
Mo26 Mo 0.39325(3) 0.71870(2) 0.62159(2) 0.04657(18) Uani 1 1 d . . . . .
Mo27 Mo 0.19216(3) 0.54894(2) 0.43710(2) 0.04801(18) Uani 1 1 d . . . . .
Mo28 Mo 0.72721(3) 0.49752(2) 0.77104(2) 0.0542(2) Uani 1 1 d . . . . .
Mo29 Mo 0.18284(3) 0.71163(2) 1.14298(2) 0.04698(17) Uani 1 1 d . . . . .
Mo30 Mo 0.17626(3) 1.38339(2) 0.66563(2) 0.0544(2) Uani 1 1 d . . . . .
Mo31 Mo 0.53393(3) 0.86795(3) 0.99556(2) 0.0563(2) Uani 1 1 d . . . . .
Mo32 Mo 0.12768(3) 1.22267(2) 0.76635(2) 0.0574(2) Uani 1 1 d . . . . .
Mo33 Mo 0.22359(3) 0.65033(3) 0.55500(2) 0.0557(2) Uani 1 1 d . . . . .
Mo34 Mo 0.37756(3) 1.23255(2) 0.74272(2) 0.0560(2) Uani 1 1 d . . . . .
Mo35 Mo 0.43625(3) 1.10599(2) 0.67077(2) 0.0549(2) Uani 1 1 d . . . . .
Mo36 Mo 0.08275(3) 0.59031(3) 0.45535(2) 0.0563(2) Uani 1 1 d . . . . .
Mo37 Mo 0.26675(3) 1.21480(3) 0.72946(2) 0.0597(2) Uani 1 1 d . . . . .
Mo38 Mo 0.14121(3) 0.75723(2) 0.32124(2) 0.0613(2) Uani 1 1 d . . . . .
Mo39 Mo 0.90384(5) 0.69490(4) 0.96984(3) 0.0523(3) Uani 0.87 1 d . U P F 1
Mo40 Mo 0.3958(5) 0.8347(3) 1.10404(14) 0.120(2) Uani 0.376(15) 1 d D U P G 1
Mo41 Mo 0.70799(5) 0.29867(6) 0.81206(4) 0.0987(6) Uani 0.85 1 d . U P A 1
Mo42 Mo 0.15928(4) 1.00828(3) 0.76283(4) 0.1255(6) Uani 1 1 d . . . . .
Mo43 Mo -0.11231(5) 0.61265(6) 0.45468(3) 0.0887(4) Uani 0.85 1 d . U P H 1
Mo44 Mo 0.42864(5) 1.04324(3) 0.55243(2) 0.0732(3) Uani 0.9 1 d . . P D 1
Mo45 Mo 0.34012(4) 0.82397(3) 0.40438(2) 0.0895(4) Uani 1 1 d . . . . .
Mo46 Mo 0.64875(6) 0.55734(5) 0.73161(4) 0.0631(4) Uani 0.7 1 d . U P I 1
Mo47 Mo 0.57206(5) 0.62930(5) 0.73782(4) 0.0636(4) Uani 0.7 1 d . U P I 1
Mo48 Mo 0.28432(8) 1.29139(6) 0.59292(4) 0.1026(7) Uani 0.8 1 d . U P D 1
Mo51 Mo 0.44503(2) 0.89761(2) 0.82699(2) 0.03121(13) Uani 1 1 d . . . . .
Mo52 Mo 0.02595(2) 0.55058(2) 1.06511(2) 0.03074(13) Uani 1 1 d . . . . .
Mo53 Mo 0.93940(2) 0.41606(2) 0.81538(2) 0.03218(14) Uani 1 1 d . . . . .
Mo54 Mo 0.93359(2) 0.51445(2) 0.78806(2) 0.03266(14) Uani 1 1 d . . . . .
Mo55 Mo 0.55173(2) 0.88402(2) 0.79794(2) 0.03364(14) Uani 1 1 d . . . . .
Mo56 Mo 0.50385(2) 0.95044(2) 0.88190(2) 0.03279(14) Uani 1 1 d . . . . .
Mo57 Mo 0.39783(2) 0.95380(2) 0.92244(2) 0.03382(14) Uani 1 1 d . . . . .
Mo58 Mo 0.00317(2) 0.63652(2) 1.09078(2) 0.03209(14) Uani 1 1 d . . . . .
Mo59 Mo 0.94893(2) 0.65789(2) 0.82777(2) 0.03582(14) Uani 1 1 d . . . . .
Mo60 Mo 0.35462(17) 1.21321(10) 0.59500(5) 0.1021(16) Uani 0.760(9) 1 d . U . D
1
Mo61 Mo 0.4674(3) 0.8609(3) 1.05758(14) 0.0587(14) Uani 0.5 1 d D U P G 1
M3I Mo 0.7080(4) 0.3983(4) 0.7942(4) 0.074(3) Uani 0.1 1 d . U P A 2
M3L Mo 0.1823(6) 0.7571(5) 0.6542(3) 0.088(4) Uani 0.1 1 d . U P B 2
M3R Mo 0.7280(5) 0.8008(5) 0.9641(3) 0.083(3) Uani 0.1 1 d . U P C 2
M3S Mo 0.3917(5) 0.9493(3) 0.5135(3) 0.089(3) Uani 0.1 1 d . U P D 2
M3T Mo 0.4186(5) 1.1265(4) 0.6074(3) 0.072(3) Uani 0.1 1 d . U P D 2
M3U Mo 0.6419(4) 0.8440(2) 0.9891(2) 0.062(2) Uani 0.15 1 d . U P C 2
M3W Mo 0.1364(3) 0.6936(3) 0.59705(16) 0.0675(19) Uani 0.15 1 d . U P B 2
M3X Mo 0.1470(2) 0.6264(2) 0.91481(14) 0.0594(15) Uani 0.2 1 d . U P E 2
M39 Mo 0.8827(3) 0.6836(3) 0.9672(2) 0.066(2) Uani 0.15 1 d . U P F 2
M40 Mo 0.38466(10) 0.8188(3) 1.09992(14) 0.1021(19) Uani 0.524(15) 1 d . U P G 2
M41 Mo 0.7060(2) 0.3159(2) 0.82813(17) 0.0592(17) Uani 0.15 1 d . U P A 2
M43 Mo -0.1032(5) 0.6435(5) 0.4517(2) 0.084(3) Uani 0.1 1 d . U P H 2
M44 Mo 0.3826(14) 1.0269(12) 0.5534(8) 0.126(11) Uiso 0.05 1 d . . P D 2
M46 Mo 0.6415(4) 0.5521(3) 0.7459(2) 0.091(3) Uani 0.15 1 d . U P I 2
M47 Mo 0.5714(3) 0.6183(3) 0.7520(2) 0.086(3) Uani 0.15 1 d . U P I 2
M48 Mo 0.2599(4) 1.2712(4) 0.5934(2) 0.097(3) Uani 0.15 1 d . U P D 2
M60 Mo 0.3251(7) 1.1968(4) 0.5929(2) 0.093(3) Uani 0.160(8) 1 d . U . D 2
M61 Mo 0.4691(8) 0.8640(6) 1.0634(4) 0.053(3) Uani 0.2 1 d . U P G 2
O1 O 0.46432(16) 0.94751(14) 0.84906(10) 0.0338(11) Uani 1 1 d . . . . .
O2 O 0.94552(17) 0.51269(15) 0.75377(11) 0.0386(12) Uani 1 1 d . . . . .
O3 O 0.40152(17) 0.88662(14) 0.85578(10) 0.0346(11) Uani 1 1 d . . . . .
O4 O 0.89479(16) 0.56160(15) 0.78497(10) 0.0348(11) Uani 1 1 d . . . . .
O5 O 0.00368(17) 0.57254(15) 1.16243(10) 0.0363(12) Uani 1 1 d . . . . .
O6 O 0.08312(16) 0.64395(14) 1.10646(10) 0.0334(11) Uani 1 1 d . . . . .
O7 O 0.94542(16) 0.60270(14) 0.84024(10) 0.0340(11) Uani 1 1 d . . . . .
O8 O 0.91468(15) 0.53182(14) 0.83665(10) 0.0325(11) Uani 1 1 d . . . . .
O9 O 0.50052(17) 0.90094(14) 0.81094(11) 0.0357(11) Uani 1 1 d . . . . .
O10 O 0.01033(17) 0.65894(14) 1.12844(10) 0.0366(12) Uani 1 1 d . . . . .
O11 O 0.94799(16) 0.46666(15) 0.80016(11) 0.0353(11) Uani 1 1 d . . . . .
O12 O 0.42665(18) 0.92664(15) 0.95410(10) 0.0382(12) Uani 1 1 d . . . . .
O13 O 0.02154(16) 0.51199(14) 1.09605(10) 0.0333(11) Uani 1 1 d . . . . .
O14 O 0.51071(18) 0.75972(15) 0.79317(11) 0.0418(13) Uani 1 1 d . . . . .
O15 O 0.04340(18) 0.75969(15) 1.07620(11) 0.0393(12) Uani 1 1 d . . . . .
O16 O -0.00261(16) 0.49098(14) 1.14617(10) 0.0344(11) Uani 1 1 d . . . . .
O17 O 0.87721(17) 0.62745(15) 0.81738(11) 0.0376(12) Uani 1 1 d . . . . .
O18 O 0.95184(19) 0.38357(15) 0.78917(11) 0.0433(13) Uani 1 1 d . . . . .
O19 O 0.83685(18) 0.77598(15) 0.82473(12) 0.0422(13) Uani 1 1 d . . . . .
O20 O 0.09410(16) 0.56587(14) 1.08605(10) 0.0303(10) Uani 1 1 d . . . . .
O21 O 0.38042(17) 0.88320(14) 0.90598(10) 0.0358(11) Uani 1 1 d . . . . .
O22 O 0.1574(2) 1.38979(17) 0.70768(13) 0.0504(14) Uani 1 1 d . . . . .
O23 O 0.59993(17) 0.84542(15) 0.79338(11) 0.0380(12) Uani 1 1 d . . . . .
O24 O 0.13387(18) 0.79129(15) 1.08071(11) 0.0392(12) Uani 1 1 d . . . . .
O25 O 0.64054(19) 0.85859(17) 0.74344(12) 0.0489(14) Uani 1 1 d . . . . .
O26 O 0.69289(18) 0.73820(15) 0.75987(11) 0.0404(12) Uani 1 1 d . . . . .
O27 O 0.54539(19) 0.89931(16) 0.95993(11) 0.0453(13) Uani 1 1 d . . . . .
O28 O 0.41972(19) 0.81549(15) 0.88174(11) 0.0446(13) Uani 1 1 d . . . . .
O29 O 0.01855(16) 0.58209(14) 1.10409(10) 0.0326(11) Uani 1 1 d . . . . .
O30 O 0.41001(17) 0.91189(15) 0.80121(11) 0.0387(12) Uani 1 1 d . . . . .
O31 O 0.09219(18) 0.82770(15) 1.03457(11) 0.0416(13) Uani 1 1 d . . . . .
O32 O 0.67290(18) 0.82359(15) 0.82382(11) 0.0403(12) Uani 1 1 d . . . . .
O33 O 0.05350(17) 0.55937(14) 1.02852(10) 0.0335(11) Uani 1 1 d . . . . .
O34 O 0.83148(17) 0.59109(15) 0.76606(11) 0.0385(12) Uani 1 1 d . . . . .
O35 O 0.79589(18) 0.81212(15) 0.77770(12) 0.0425(13) Uani 1 1 d . . . . .
O36 O 0.45481(17) 0.93455(14) 0.90860(10) 0.0334(11) Uani 1 1 d . . . . .
O37 O 0.98122(16) 0.54676(14) 0.80663(10) 0.0336(11) Uani 1 1 d . . . . .
O38 O 0.29327(17) 0.90865(14) 0.88760(11) 0.0369(12) Uani 1 1 d . . . . .
O39 O -0.05132(17) 0.62478(16) 1.08496(11) 0.0419(13) Uani 1 1 d . . . . .
O40 O 0.48200(19) 0.82608(17) 0.66270(12) 0.0479(14) Uani 1 1 d . . . . .
O41 O 0.82715(17) 0.69636(15) 0.80805(11) 0.0370(12) Uani 1 1 d . . . . .
O42 O 0.86992(17) 0.49287(14) 0.78661(10) 0.0351(11) Uani 1 1 d . . . . .
O43 O 0.74790(17) 0.77208(15) 0.81078(11) 0.0391(12) Uani 1 1 d . . . . .
O44 O 0.79251(17) 0.48783(16) 0.78169(11) 0.0415(12) Uani 1 1 d . . . . .
O45 O 0.0490(2) 0.69413(16) 1.17975(11) 0.0442(13) Uani 1 1 d . . . . .
O46 O -0.10089(19) 1.39734(15) 0.67978(11) 0.0434(13) Uani 1 1 d . . . . .
O47 O 0.30188(17) 0.87055(15) 0.94352(11) 0.0379(12) Uani 1 1 d . . . . .
O48 O 0.50742(18) 0.99896(15) 0.89262(12) 0.0417(13) Uani 1 1 d . . . . .
O49 O 0.18004(19) 0.89748(16) 0.98147(12) 0.0469(14) Uani 1 1 d . . . . .
O50 O 0.55508(17) 0.94505(14) 0.86446(11) 0.0366(12) Uani 1 1 d . . . . .
O51 O 0.3104(2) 0.82070(17) 0.99149(12) 0.0494(14) Uani 1 1 d . . . . .
O52 O 0.1230(2) 0.53631(16) 0.35087(11) 0.0465(14) Uani 1 1 d . . . . .
O53 O 0.78747(17) 0.73123(16) 0.85489(11) 0.0408(12) Uani 1 1 d . . . . .
O54 O 0.92656(17) 0.70478(15) 0.81500(12) 0.0411(12) Uani 1 1 d . . . . .
O55 O 0.65395(17) 0.88635(14) 0.84862(12) 0.0394(12) Uani 1 1 d . . . . .
O56 O 0.86639(18) 0.58677(17) 0.86880(12) 0.0440(13) Uani 1 1 d . . . . .
O57 O 0.87132(18) 0.74113(16) 0.77546(12) 0.0432(13) Uani 1 1 d . . . . .
O58 O -0.05795(17) 0.53968(15) 1.11864(11) 0.0387(12) Uani 1 1 d . . . . .
O59 O 0.21717(18) 0.83288(15) 0.98887(11) 0.0383(12) Uani 1 1 d . . . . .
O60 O 0.73255(19) 0.68784(16) 0.81363(12) 0.0452(13) Uani 1 1 d . . . . .
O61 O -0.00880(18) 0.72946(16) 1.02719(11) 0.0429(13) Uani 1 1 d . . . . .
O62 O 0.1946(2) 1.23135(17) 0.78262(13) 0.0538(15) Uani 1 1 d . . . . .
O63 O 0.27020(19) 0.89343(15) 0.98852(11) 0.0413(13) Uani 1 1 d . . . . .
O64 O 0.44140(19) 0.79625(16) 0.76714(11) 0.0448(13) Uani 1 1 d . . . . .
O65 O 0.00328(19) 1.40433(15) 0.73253(11) 0.0441(13) Uani 1 1 d . . . . .
O66 O 0.83017(16) 0.55292(15) 0.81701(10) 0.0350(11) Uani 1 1 d . . . . .
O67 O 0.15715(18) 0.78521(15) 1.02553(11) 0.0406(12) Uani 1 1 d . . . . .
O68 O 0.52274(16) 0.82864(14) 0.79703(10) 0.0344(11) Uani 1 1 d . . . . .
O69 O 0.58799(18) 0.78704(15) 0.82626(11) 0.0400(12) Uani 1 1 d . . . . .
O70 O 0.7630(2) 0.61064(19) 0.79916(15) 0.0615(17) Uani 1 1 d . . . . .
O71 O 0.45144(19) 0.87297(16) 0.74792(11) 0.0446(13) Uani 1 1 d . . . . .
O72 O 0.000000 0.500000 1.000000 0.049(2) Uani 1 2 d S . P . .
O73 O 1.03520(18) 0.58880(16) 0.85047(12) 0.0427(13) Uani 1 1 d . . . . .
O74 O 0.37166(17) 0.95129(14) 0.88510(10) 0.0351(11) Uani 1 1 d . . . . .
O75 O 0.6313(2) 0.81625(17) 0.87707(12) 0.0508(15) Uani 1 1 d . . . . .
O76 O 0.92256(17) 0.37680(14) 0.84367(10) 0.0349(11) Uani 1 1 d . . . . .
O77 O 0.41379(18) 0.85689(16) 0.69215(11) 0.0426(13) Uani 1 1 d . . . . .
O78 O 0.59242(16) 0.92356(14) 0.81635(11) 0.0348(11) Uani 1 1 d . . . . .
O79 O 0.02895(16) 0.60851(14) 1.05858(10) 0.0329(11) Uani 1 1 d . . . . .
O80 O 0.48147(17) 0.88117(14) 0.86902(10) 0.0347(11) Uani 1 1 d . . . . .
O81 O 0.94622(17) 0.63629(15) 0.78830(11) 0.0381(12) Uani 1 1 d . . . . .
O82 O 0.21186(17) 0.85597(15) 0.93364(10) 0.0373(12) Uani 1 1 d . . . . .
O83 O 0.3575(2) 0.69759(17) 0.58511(11) 0.0465(14) Uani 1 1 d . . . . .
O84 O 0.78065(18) 0.73123(16) 0.77331(11) 0.0416(13) Uani 1 1 d . . . . .
O85 O 0.1671(2) 1.31697(17) 0.72817(13) 0.0521(15) Uani 1 1 d . . . . .
O86 O 0.46640(17) 0.86404(14) 0.92446(10) 0.0358(11) Uani 1 1 d . . . . .
O87 O 0.15317(17) 0.59931(16) 1.12948(11) 0.0423(13) Uani 1 1 d . . . . .
O88 O 0.32262(19) 0.90563(17) 0.76976(11) 0.0458(13) Uani 1 1 d . . . . .
O89 O 0.1841(2) 0.74516(16) 0.91222(12) 0.0477(14) Uani 1 1 d . . . . .
O90 O 0.06628(18) 0.72449(15) 1.12667(11) 0.0396(12) Uani 1 1 d . . . . .
O91 O 0.76927(18) 0.54439(16) 0.76229(12) 0.0461(13) Uani 1 1 d . . . . .
O92 O 0.25921(19) 0.93231(15) 0.93938(11) 0.0423(13) Uani 1 1 d . . . . .
O93 O 0.2239(2) 1.18098(17) 0.73912(14) 0.0554(16) Uani 1 1 d . . . . .
O94 O 0.2281(2) 0.94273(16) 1.02632(13) 0.0560(16) Uani 1 1 d . . . . .
O95 O 0.32008(18) 0.84622(15) 0.85852(11) 0.0394(12) Uani 1 1 d . . . . .
O96 O 0.13098(19) 0.69128(15) 1.15516(11) 0.0426(13) Uani 1 1 d . . . . .
O97 O 0.61438(18) 0.91038(15) 0.89667(11) 0.0411(13) Uani 1 1 d . . . . .
O98 O 0.87066(18) 0.66287(15) 0.75997(11) 0.0406(12) Uani 1 1 d . . . . .
O99 O 0.54835(18) 0.89547(15) 0.76352(11) 0.0417(13) Uani 1 1 d . . . . .
O100 O 0.44155(16) 0.83966(14) 0.81809(10) 0.0349(11) Uani 1 1 d . . . . .
O101 O 0.1964(2) 0.61688(16) 0.42249(11) 0.0458(13) Uani 1 1 d . . . . .
O102 O 0.43522(18) 0.95138(16) 0.74180(11) 0.0432(13) Uani 1 1 d . . . . .
O103 O 0.4462(2) 0.78499(18) 0.70566(12) 0.0529(15) Uani 1 1 d . . . . .
O104 O 0.53213(17) 0.92616(15) 0.91533(11) 0.0381(12) Uani 1 1 d . . . . .
O105 O 0.46522(19) 1.02904(16) 0.74840(12) 0.0462(13) Uani 1 1 d . . . . .
O106 O 0.62657(17) 0.78672(15) 0.77315(11) 0.0384(12) Uani 1 1 d . . . . .
O107 O 0.41636(19) 0.93399(16) 0.67863(11) 0.0458(13) Uani 1 1 d . . . . .
O108 O 0.29603(18) 0.87251(17) 0.71153(12) 0.0455(13) Uani 1 1 d . . . . .
O109 O 0.57268(17) 0.86419(14) 0.84624(10) 0.0356(11) Uani 1 1 d . . . . .
O110 O -0.10175(18) 0.52457(17) 0.90504(12) 0.0461(13) Uani 1 1 d . . . . .
O111 O 0.1720(2) 0.54712(18) 0.51142(12) 0.0599(17) Uani 1 1 d . . . . .
O112 O 0.2727(2) 1.15011(17) 0.78431(13) 0.0517(15) Uani 1 1 d . . . . .
O113 O 0.84270(19) 0.52000(16) 0.73711(11) 0.0446(13) Uani 1 1 d . . . . .
O114 O 0.10498(17) 0.71245(14) 1.07045(10) 0.0360(11) Uani 1 1 d . . . . .
O115 O 0.1880(2) 0.82824(18) 1.13008(12) 0.0570(16) Uani 1 1 d . . . . .
O116 O 0.1162(2) 0.60376(16) 0.37901(11) 0.0484(14) Uani 1 1 d . . . . .
O117 O 0.0708(2) 0.56042(18) 0.42143(12) 0.0538(15) Uani 1 1 d . . . . .
O118 O 0.1388(2) 1.2199(2) 0.73133(15) 0.0667(19) Uani 1 1 d . . . . .
O119 O 0.04702(17) 0.49995(14) 1.05072(10) 0.0348(11) Uani 1 1 d . . . . .
O120 O 0.4316(2) 1.11872(16) 0.77034(13) 0.0497(14) Uani 1 1 d . . . . .
O121 O 0.49986(19) 0.79709(15) 0.84797(11) 0.0431(13) Uani 1 1 d . . . . .
O122 O 0.92916(17) 0.67311(15) 0.86538(11) 0.0389(12) Uani 1 1 d . . . . .
O123 O 0.73093(18) 0.86196(16) 0.87080(12) 0.0460(14) Uani 1 1 d . . . . .
O124 O 0.83059(18) 0.47077(17) 0.83622(11) 0.0447(13) Uani 1 1 d . . . . .
O125 O 0.07530(16) 0.55076(14) 1.14233(10) 0.0314(11) Uani 1 1 d . . . . .
O126 O 0.34750(18) 0.95029(14) 0.94155(11) 0.0383(12) Uani 1 1 d . . . . .
O127 O 0.70848(18) 0.81698(15) 0.76564(11) 0.0412(12) Uani 1 1 d . . . . .
O128 O 0.3926(2) 1.07897(18) 0.81242(13) 0.0549(16) Uani 1 1 d . . . . .
O129 O 0.1930(2) 0.73653(18) 0.97102(13) 0.0553(15) Uani 1 1 d . . . . .
O130 O 0.0487(2) 1.38408(18) 0.78345(12) 0.0533(15) Uani 1 1 d . . . . .
O131 O 0.57058(18) 0.73453(16) 0.77273(13) 0.0471(14) Uani 1 1 d . . . . .
O132 O 0.87530(17) 0.41838(15) 0.80584(11) 0.0374(12) Uani 1 1 d . . . . .
O133 O 0.4199(2) 0.99805(17) 0.79174(12) 0.0505(15) Uani 1 1 d . . . . .
O134 O 0.84300(19) 0.66742(16) 0.87720(14) 0.0513(15) Uani 1 1 d . . . . .
O135 O 0.25597(18) 0.79473(15) 0.94344(11) 0.0416(13) Uani 1 1 d . . . . .
O136 O 0.11815(17) 0.83104(15) 0.98079(11) 0.0384(12) Uani 1 1 d . . . . .
O137 O 0.4410(2) 1.09049(16) 0.71333(13) 0.0493(14) Uani 1 1 d . . . . .
O138 O 0.1002(2) 1.34207(16) 0.74791(12) 0.0476(14) Uani 1 1 d . . . . .
O139 O 0.85839(18) 0.74447(16) 0.90197(11) 0.0448(14) Uani 1 1 d . . . . .
O140 O -0.02841(17) 0.54283(15) 1.05402(11) 0.0388(12) Uani 1 1 d . . . . .
O141 O 0.48848(18) 0.91371(16) 0.70452(11) 0.0433(13) Uani 1 1 d . . . . .
O142 O 0.4916(2) 0.99324(17) 0.69818(12) 0.0507(14) Uani 1 1 d . . . . .
O143 O 0.0784(2) 0.80528(15) 1.12442(11) 0.0464(14) Uani 1 1 d . . . . .
O144 O -0.02783(17) 0.56480(14) 0.88809(10) 0.0352(11) Uani 1 1 d . . . . .
O145 O 0.91071(18) 0.60051(16) 0.73557(11) 0.0441(13) Uani 1 1 d . . . . .
O146 O 0.3624(2) 1.11032(17) 0.73281(13) 0.0511(15) Uani 1 1 d . . . . .
O147 O 0.1993(2) 1.11968(18) 0.77725(16) 0.0639(18) Uani 1 1 d . . . . .
O148 O 0.0632(2) 0.34975(17) 1.02987(12) 0.0571(17) Uani 1 1 d . . . . .
O149 O 0.20268(18) 0.90809(17) 0.89087(12) 0.0482(14) Uani 1 1 d . . . . .
O150 O 0.9267(2) 0.78579(17) 0.81669(14) 0.0535(15) Uani 1 1 d . . . . .
O151 O 0.35762(19) 0.81974(16) 0.73080(11) 0.0455(13) Uani 1 1 d . . . . .
O152 O 0.1857(2) 0.68047(18) 1.11310(14) 0.0590(17) Uani 1 1 d . . . . .
O153 O -0.1011(2) 1.28964(16) 0.69917(11) 0.0476(14) Uani 1 1 d . . . . .
O154 O 0.39570(19) 0.85000(16) 0.96547(13) 0.0492(14) Uani 1 1 d . . . . .
O155 O 0.08321(18) 0.74561(15) 1.02625(11) 0.0398(12) Uani 1 1 d . . . . .
O156 O 0.64598(19) 0.96710(16) 0.85950(13) 0.0502(14) Uani 1 1 d . . . . .
O157 O 0.04877(18) 0.66901(15) 1.02293(10) 0.0379(12) Uani 1 1 d . . . . .
O158 O 0.3990(2) 0.67637(18) 0.63709(12) 0.0571(16) Uani 1 1 d . . . . .
O159 O 0.6190(2) 0.7359(2) 0.72340(14) 0.076(2) Uani 1 1 d . . . . .
O160 O 0.4183(2) 0.73678(18) 0.54294(11) 0.0490(14) Uani 1 1 d . . . . .
O161 O 0.35916(19) 0.91258(15) 0.98981(11) 0.0432(13) Uani 1 1 d . . . . .
O162 O 0.1636(2) 0.81293(19) 0.88423(12) 0.0520(15) Uani 1 1 d . . . . .
O163 O 0.8057(2) 0.78958(19) 0.90232(12) 0.0540(16) Uani 1 1 d . . . . .
O164 O 0.79822(18) 0.81475(15) 0.85709(11) 0.0418(13) Uani 1 1 d . . . . .
O165 O 0.3684(2) 0.6185(2) 0.42917(13) 0.0658(18) Uani 1 1 d . . . . .
O166 O 0.1979(2) 0.50511(18) 0.45103(13) 0.0586(16) Uani 1 1 d . . . . .
O167 O 0.25058(17) 0.83779(15) 0.89326(11) 0.0382(12) Uani 1 1 d . . . . .
O168 O 0.01205(17) 0.68199(14) 1.07257(10) 0.0358(11) Uani 1 1 d . . . . .
O169 O 0.36428(18) 0.80059(16) 0.67402(10) 0.0422(13) Uani 1 1 d . . . . .
O170 O 0.1149(2) 0.62521(17) 1.04128(16) 0.0598(17) Uani 1 1 d . . . . .
O171 O 0.4459(2) 0.72160(18) 0.60063(12) 0.0534(16) Uani 1 1 d . . . . .
O172 O 0.16302(18) 0.79869(15) 0.94044(11) 0.0388(12) Uani 1 1 d . . . . .
O173 O 0.2046(2) 1.30981(17) 0.78742(13) 0.0542(15) Uani 1 1 d . . . . .
O174 O 0.7564(2) 0.77452(18) 0.72690(13) 0.0535(15) Uani 1 1 d . . . . .
O175 O 0.4198(3) 0.6865(2) 0.8346(2) 0.095(3) Uani 1 1 d . . . . .
O176 O 0.68663(18) 0.88525(15) 0.79551(12) 0.0424(13) Uani 1 1 d . . . . .
O177 O 0.3212(2) 1.25801(17) 0.73496(13) 0.0528(15) Uani 1 1 d . . . . .
O178 O 0.0695(2) 1.36415(15) 0.70154(11) 0.0454(13) Uani 1 1 d . . . . .
O179 O 0.0874(2) 0.66695(16) 0.34952(11) 0.0487(14) Uani 1 1 d . . . . .
O180 O 0.2445(2) 0.65266(18) 0.37824(12) 0.0540(15) Uani 1 1 d . . . . .
O181 O 0.20306(19) 0.82746(15) 1.07413(11) 0.0440(13) Uani 1 1 d . . . . .
O182 O 0.03498(18) 0.79186(17) 0.98949(12) 0.0466(14) Uani 1 1 d . . . . .
O183 O 0.78216(18) 0.65483(16) 0.75498(12) 0.0437(13) Uani 1 1 d . . . . .
O184 O 0.2782(2) 0.63101(18) 0.42969(12) 0.0537(15) Uani 1 1 d . . . . .
O185 O 0.08025(17) 0.52703(15) 0.97913(11) 0.0403(12) Uani 1 1 d . . . . .
O186 O 0.4137(2) 1.18939(18) 0.74677(14) 0.0588(16) Uani 1 1 d . . . . .
O187 O 0.41721(18) 1.00145(15) 0.92910(11) 0.0418(13) Uani 1 1 d . . . . .
O188 O 0.50541(19) 0.96908(16) 0.96076(12) 0.0445(13) Uani 1 1 d . . . . .
O189 O 0.17359(19) 0.87360(15) 1.03454(11) 0.0427(13) Uani 1 1 d . . . . .
O190 O 0.15722(19) 0.69970(16) 1.02224(12) 0.0469(14) Uani 1 1 d . . . . .
O191 O 0.40068(19) 1.01471(16) 0.70894(12) 0.0457(13) Uani 1 1 d . . . . .
O192 O 0.0074(2) 0.39468(17) 1.00026(13) 0.0584(17) Uani 1 1 d . . . . .
O193 O 0.4230(2) 0.75819(17) 0.64893(11) 0.0490(14) Uani 1 1 d . . . . .
O194 O 0.78080(18) 0.41551(17) 0.80002(12) 0.0476(14) Uani 1 1 d . . . . .
O195 O 0.3111(2) 1.07865(17) 0.77748(13) 0.0540(16) Uani 1 1 d . . . . .
O196 O 0.76301(17) 0.86127(15) 0.81949(12) 0.0418(13) Uani 1 1 d . . . . .
O197 O 0.9507(2) 0.7443(2) 0.89598(18) 0.074(2) Uani 1 1 d . . . . .
O198 O 0.1689(2) 0.63857(16) 0.33934(11) 0.0454(13) Uani 1 1 d . . . . .
O199 O -0.0545(2) 0.57680(17) 0.94463(11) 0.0515(15) Uani 1 1 d . . . . .
O200 O 0.07356(19) 0.45558(16) 1.00619(11) 0.0445(13) Uani 1 1 d . . . . .
O201 O 0.2377(2) 1.42623(18) 0.73443(15) 0.0621(17) Uani 1 1 d . . . . .
O202 O 0.1241(2) 0.87317(17) 0.93258(12) 0.0492(14) Uani 1 1 d . . . . .
O203 O 0.34455(19) 0.87659(17) 0.66177(11) 0.0459(14) Uani 1 1 d . . . . .
O204 O 0.46611(19) 0.87330(18) 0.59122(12) 0.0487(14) Uani 1 1 d . . . . .
O205 O -0.0809(2) 1.42899(16) 0.73592(12) 0.0471(14) Uani 1 1 d . . . . .
O206 O 0.37025(18) 0.89742(16) 0.72027(10) 0.0404(12) Uani 1 1 d . . . . .
O207 O 0.3640(2) 1.22841(18) 0.78223(14) 0.0592(16) Uani 1 1 d . . . . .
O208 O 0.0255(2) 0.55406(18) 0.93684(14) 0.0582(16) Uani 1 1 d . . . . .
O209 O -0.1506(2) 1.35254(17) 0.71788(11) 0.0492(14) Uani 1 1 d . . . . .
O210 O 0.6481(2) 0.72561(18) 0.80714(13) 0.0548(15) Uani 1 1 d . . . . .
O211 O 0.2814(2) 0.65007(18) 0.56938(12) 0.0519(15) Uani 1 1 d . . . . .
O212 O -0.06423(19) 1.35369(15) 0.70948(10) 0.0408(12) Uani 1 1 d . . . . .
O213 O -0.0352(2) 1.25086(17) 0.72201(14) 0.0579(16) Uani 1 1 d . . . . .
O214 O 0.1285(2) 0.5189(2) 1.02950(15) 0.0666(18) Uani 1 1 d . . . . .
O215 O 0.2244(2) 0.6995(2) 1.16738(17) 0.075(2) Uani 1 1 d . . . . .
O216 O 0.1750(2) 0.56224(18) 0.30850(11) 0.0499(15) Uani 1 1 d . . . . .
O217 O 0.3355(2) 0.69678(17) 0.53262(11) 0.0465(14) Uani 1 1 d . . . . .
O218 O 0.1451(2) 1.47016(18) 0.71044(15) 0.0618(17) Uani 1 1 d . . . . .
O219 O 0.2386(2) 0.8149(2) 0.83502(12) 0.0590(17) Uani 1 1 d . . . . .
O220 O 0.0855(3) 0.3832(2) 0.98053(14) 0.077(2) Uani 1 1 d . . . . .
O221 O 0.10772(18) 0.75216(16) 0.97232(11) 0.0421(13) Uani 1 1 d . . . . .
O222 O 0.1336(2) 1.32843(17) 0.67173(12) 0.0508(15) Uani 1 1 d . . . . .
O223 O 0.3900(2) 0.73150(18) 0.49365(11) 0.0494(14) Uani 1 1 d . . . . .
O224 O 0.38590(19) 0.76923(17) 0.59106(11) 0.0450(13) Uani 1 1 d . . . . .
O225 O 0.2409(2) 1.26427(17) 0.73974(13) 0.0519(15) Uani 1 1 d . . . . .
O226 O 0.5440(2) 0.94528(19) 0.66638(14) 0.0583(16) Uani 1 1 d . . . . .
O227 O 0.46441(19) 0.89987(17) 0.64687(12) 0.0473(14) Uani 1 1 d . . . . .
O228 O 0.8255(2) 0.71261(17) 0.72452(12) 0.0518(15) Uani 1 1 d . . . . .
O229 O 0.3259(2) 0.79666(17) 0.90113(13) 0.0523(15) Uani 1 1 d . . . . .
O230 O 0.3373(2) 0.73378(17) 0.63552(12) 0.0507(14) Uani 1 1 d . . . . .
O231 O 0.2263(2) 0.75616(19) 1.13085(13) 0.0567(16) Uani 1 1 d . . . . .
O232 O 0.2944(2) 1.30198(18) 0.78063(14) 0.0584(16) Uani 1 1 d . . . . .
O233 O 0.3116(2) 1.03824(19) 0.70894(13) 0.0564(16) Uani 1 1 d . . . . .
O234 O 0.2983(2) 0.5885(2) 0.37931(13) 0.0593(17) Uani 1 1 d . . . . .
O235 O 0.0155(2) 0.61113(16) 0.33131(11) 0.0468(14) Uani 1 1 d . . . . .
O236 O 0.2593(2) 0.8001(2) 1.10128(13) 0.0605(17) Uani 1 1 d . . . . .
O237 O 0.32575(17) 0.92078(15) 0.83399(11) 0.0393(12) Uani 1 1 d . . . . .
O238 O 0.41013(19) 0.84063(17) 0.63337(11) 0.0459(14) Uani 1 1 d . . . . .
O239 O 0.2205(2) 1.35943(17) 0.69223(13) 0.0541(15) Uani 1 1 d . . . . .
O240 O 0.54650(19) 0.80107(17) 0.74675(11) 0.0464(14) Uani 1 1 d . . . . .
O241 O 0.3012(2) 0.97411(16) 0.98841(12) 0.0500(15) Uani 1 1 d . . . . .
O242 O 0.2401(2) 0.55532(18) 0.41493(12) 0.0538(15) Uani 1 1 d . . . . .
O243 O 0.82936(19) 0.42623(16) 0.75360(10) 0.0445(13) Uani 1 1 d . . . . .
O244 O 0.1488(2) 1.3791(2) 0.62558(14) 0.0646(18) Uani 1 1 d . . . . .
O245 O 0.2629(2) 0.93687(18) 0.73347(14) 0.0574(16) Uani 1 1 d . . . . .
O246 O 0.43174(18) 0.75530(15) 0.81466(11) 0.0405(12) Uani 1 1 d . . . . .
O247 O 0.1284(2) 0.87319(17) 1.08365(12) 0.0539(16) Uani 1 1 d . . . . .
O248 O -0.0285(2) 1.45684(15) 0.69391(11) 0.0458(13) Uani 1 1 d . . . . .
O249 O 0.35278(19) 0.78037(17) 0.53428(12) 0.0478(14) Uani 1 1 d . . . . .
O250 O 0.29272(19) 0.81217(17) 0.68402(11) 0.0475(14) Uani 1 1 d . . . . .
O251 O 0.3999(2) 0.65390(17) 0.54533(12) 0.0525(15) Uani 1 1 d . . . . .
O252 O 0.2049(2) 0.58007(16) 0.36535(11) 0.0486(14) Uani 1 1 d . . . . .
O253 O 0.2606(2) 1.35128(17) 0.74381(14) 0.0549(16) Uani 1 1 d . . . . .
O254 O 0.73230(19) 0.93202(16) 0.84128(14) 0.0534(15) Uani 1 1 d . . . . .
O255 O 0.2094(2) 1.27861(19) 0.67303(15) 0.0687(19) Uani 1 1 d . . . . .
O256 O 0.2252(2) 0.58403(17) 0.47168(11) 0.0494(14) Uani 1 1 d . . . . .
O257 O 0.5401(2) 0.86569(19) 0.62994(14) 0.0570(16) Uani 1 1 d . . . . .
O258 O 0.7766(3) 0.5921(2) 0.71554(13) 0.071(2) Uani 1 1 d . . . . .
O259 O 0.0441(2) 0.56375(16) 0.36451(12) 0.0498(14) Uani 1 1 d . . . . .
O260 O 0.7185(2) 0.78217(18) 0.87493(14) 0.0545(15) Uani 1 1 d . . . . .
O261 O 0.0584(2) 1.44834(16) 0.68939(12) 0.0498(14) Uani 1 1 d . . . . .
O262 O 0.47816(18) 0.89296(15) 0.98105(11) 0.0418(13) Uani 1 1 d . . . . .
O263 O 0.2708(2) 1.21957(17) 0.78264(13) 0.0528(15) Uani 1 1 d . . . . .
O264 O 0.2543(2) 1.0986(2) 0.73465(15) 0.0703(19) Uani 1 1 d . . . . .
O265 O 0.2293(2) 0.69707(18) 0.44327(13) 0.0550(15) Uani 1 1 d . . . . .
O266 O 0.3168(2) 1.18550(16) 0.74147(13) 0.0503(14) Uani 1 1 d . . . . .
O267 O 0.4607(2) 0.6830(2) 0.50993(13) 0.0615(17) Uani 1 1 d . . . . .
O268 O 0.4563(2) 1.05144(17) 0.67189(12) 0.0516(15) Uani 1 1 d . . . . .
O269 O 0.14927(18) 0.75302(15) 1.12075(11) 0.0405(12) Uani 1 1 d . . . . .
O270 O 0.7322(3) 0.3444(3) 0.7966(2) 0.098(3) Uani 1 1 d . U . . .
O271 O 0.2939(2) 0.75177(18) 0.56988(13) 0.0537(15) Uani 1 1 d . . . . .
O272 O 0.87988(17) 0.73659(15) 0.85489(11) 0.0389(12) Uani 1 1 d . . . . .
O273 O 0.3010(2) 0.76288(18) 0.84716(14) 0.0617(18) Uani 1 1 d . . . . .
O274 O 0.2027(2) 0.7978(2) 0.68097(14) 0.0664(19) Uani 1 1 d . . . . .
O275 O 0.2343(2) 0.61044(17) 0.52075(11) 0.0497(14) Uani 1 1 d . . . . .
O276 O 0.1229(2) 1.27539(16) 0.77218(12) 0.0511(15) Uani 1 1 d . . . . .
O277 O 0.1481(2) 0.53633(17) 0.40754(11) 0.0491(14) Uani 1 1 d . . . . .
O278 O 0.19343(19) 0.74344(16) 1.07030(11) 0.0434(13) Uani 1 1 d . . . . .
O279 O 0.2808(2) 0.65260(17) 0.48191(11) 0.0483(14) Uani 1 1 d . . . . .
O280 O 0.1115(2) 0.60131(19) 0.49700(12) 0.0556(16) Uani 1 1 d . . . . .
O281 O 0.5068(2) 0.7498(2) 0.56492(13) 0.0588(17) Uani 1 1 d . . . . .
O282 O 0.2553(2) 1.2738(2) 0.82768(14) 0.0657(18) Uani 1 1 d . . . . .
O283 O 0.0822(2) 1.28080(18) 0.70261(14) 0.0600(17) Uani 1 1 d . . . . .
O284 O 0.88436(19) 0.81400(17) 0.87601(14) 0.0531(15) Uani 1 1 d . . . . .
O285 O 0.5272(2) 1.06849(19) 0.71746(14) 0.0611(17) Uani 1 1 d . . . . .
O286 O -0.0126(2) 1.30074(19) 0.68208(13) 0.0599(17) Uani 1 1 d . . . . .
O287 O 0.3586(2) 0.61504(18) 0.58744(12) 0.0604(17) Uani 1 1 d . . . . .
O288 O 0.8559(3) 0.7292(2) 0.95768(14) 0.073(2) Uani 1 1 d . . . . .
O289 O 0.3806(2) 1.04806(17) 0.75440(12) 0.0495(14) Uani 1 1 d . . . . .
O290 O 0.7516(3) 0.4712(2) 0.72744(15) 0.073(2) Uani 1 1 d . . . . .
O291 O 0.3595(2) 1.14786(18) 0.79091(13) 0.0547(16) Uani 1 1 d . . . . .
O292 O 0.8750(3) 0.8065(3) 0.94567(18) 0.102(3) Uani 1 1 d . . . . .
O293 O 0.85298(19) 0.85690(17) 0.81859(14) 0.0533(15) Uani 1 1 d . . . . .
O294 O 0.1333(2) 1.34891(19) 0.80605(13) 0.0590(17) Uani 1 1 d . . . . .
O295 O 0.3058(2) 0.8042(2) 0.62537(13) 0.0672(19) Uani 1 1 d . . . . .
O296 O 0.2771(2) 0.53955(18) 0.50697(13) 0.0598(17) Uani 1 1 d . . . . .
O297 O 0.2608(2) 0.87031(17) 1.04216(12) 0.0483(14) Uani 1 1 d . . . . .
O298 O 0.4406(2) 0.95023(18) 1.01248(13) 0.0593(17) Uani 1 1 d . . . . .
O299 O 0.1746(3) 0.7608(2) 1.17916(13) 0.072(2) Uani 1 1 d . . . . .
O300 O 0.1728(3) 0.6927(2) 0.38727(13) 0.069(2) Uani 1 1 d . . . . .
O301 O 1.00388(17) 0.66986(16) 0.83352(13) 0.0463(14) Uani 1 1 d . . . . .
O302 O 0.1468(2) 0.57293(17) 0.45960(12) 0.0495(14) Uani 1 1 d . . . . .
O303 O 0.1322(3) 0.68949(19) 0.93578(15) 0.069(2) Uani 1 1 d . . . . .
O304 O 0.1846(2) 1.37788(17) 0.76530(13) 0.0536(15) Uani 1 1 d . . . . .
O305 O -0.0439(2) 0.57006(18) 0.36691(13) 0.0572(16) Uani 1 1 d . . . . .
O306 O 0.3510(2) 1.3385(2) 0.74561(17) 0.072(2) Uani 1 1 d . . . . .
O307 O 0.2068(2) 0.8721(2) 0.71359(16) 0.074(2) Uani 1 1 d . . . . .
O308 O 0.0993(2) 0.6352(2) 0.44361(14) 0.0651(18) Uani 1 1 d . . . . .
O309 O 0.5589(2) 0.84958(18) 0.91173(14) 0.0589(16) Uani 1 1 d . . . . .
O310 O 0.3028(2) 0.7487(2) 0.47800(15) 0.0668(18) Uani 1 1 d . . . . .
O311 O 0.2382(2) 0.76921(16) 0.88374(13) 0.0505(15) Uani 1 1 d . . . . .
O312 O -0.0654(2) 1.30771(17) 0.75765(12) 0.0508(14) Uani 1 1 d . . . . .
O313 O 0.0692(2) 0.49126(18) 0.38300(13) 0.0580(16) Uani 1 1 d . . . . .
O314 O 0.3706(2) 1.07588(18) 0.67719(12) 0.0523(15) Uani 1 1 d . . . . .
O315 O 0.4414(2) 0.80541(18) 0.55407(11) 0.0498(14) Uani 1 1 d . . . . .
O316 O 0.2271(3) 0.69072(19) 0.53575(15) 0.0698(19) Uani 1 1 d . . . . .
O317 O 0.4873(3) 1.1280(2) 0.67058(17) 0.077(2) Uani 1 1 d . . . . .
O318 O 0.7092(2) 0.5953(2) 0.7503(2) 0.082(2) Uani 1 1 d . . . . .
O319 O 0.1765(3) 0.7494(2) 0.27994(14) 0.072(2) Uani 1 1 d . . . . .
O320 O 0.3261(2) 1.2000(2) 0.82902(14) 0.0662(19) Uani 1 1 d . . . . .
O321 O 0.3511(2) 0.71778(19) 0.81583(19) 0.081(2) Uani 1 1 d . . . . .
O322 O 0.3189(2) 0.58866(18) 0.47061(12) 0.0552(16) Uani 1 1 d . . . . .
O323 O 0.4690(2) 0.97920(18) 0.64217(12) 0.0548(16) Uani 1 1 d . . . . .
O324 O 0.4171(2) 1.15015(17) 0.69618(13) 0.0557(16) Uani 1 1 d . . . . .
O325 O 0.09214(19) 1.42122(16) 0.74109(12) 0.0457(13) Uani 1 1 d . . . . .
O326 O 0.3866(2) 1.0044(2) 0.63903(15) 0.0670(18) Uani 1 1 d . . . . .
O327 O 0.2616(2) 1.21010(19) 0.69387(14) 0.0648(18) Uani 1 1 d . . . . .
O328 O 0.4377(3) 0.9132(2) 0.54232(14) 0.070(2) Uani 1 1 d . . . . .
O329 O 0.2574(3) 1.0890(2) 0.81949(17) 0.090(3) Uani 1 1 d . . . . .
O330 O 0.1640(2) 0.62577(18) 0.53364(12) 0.0562(16) Uani 1 1 d . . . . .
O331 O 0.3810(2) 0.8610(2) 0.56660(14) 0.0625(17) Uani 1 1 d . . . . .
O332 O 0.3153(3) 0.7334(2) 0.68958(15) 0.079(2) Uani 1 1 d . . . . .
O333 O 0.0106(2) 1.32766(16) 0.73778(12) 0.0460(13) Uani 1 1 d . . . . .
O334 O 0.35296(19) 0.96956(16) 0.74700(12) 0.0450(13) Uani 1 1 d . . . . .
O335 O 0.2159(3) 0.5886(2) 0.57480(14) 0.077(2) Uani 1 1 d . . . . .
O336 O 0.3271(2) 1.1514(2) 0.67614(16) 0.0706(19) Uani 1 1 d . . . . .
O337 O 0.4923(2) 1.15762(19) 0.73912(16) 0.0691(19) Uani 1 1 d . . . . .
O338 O 0.3838(2) 0.7950(2) 0.47887(13) 0.0645(18) Uani 1 1 d . . . . .
O339 O 0.2884(2) 1.30983(19) 0.69949(15) 0.0637(18) Uani 1 1 d . . . . .
O340 O 0.7166(3) 0.5165(2) 0.80319(18) 0.083(2) Uani 1 1 d . . . . .
O341 O -0.1669(2) 1.29509(17) 0.67163(13) 0.0571(16) Uani 1 1 d . . . . .
O342 O 0.8896(3) 0.6965(2) 1.00417(15) 0.077(2) Uani 1 1 d . . . . .
O343 O 0.6219(2) 0.67709(18) 0.75931(18) 0.075(2) Uani 1 1 d . . . . .
O344 O 0.2488(3) 0.6709(3) 0.32336(16) 0.083(2) Uani 1 1 d . . . . .
O345 O 0.0763(3) 0.60667(19) 0.98720(14) 0.077(2) Uani 1 1 d . . . . .
O346 O 0.0736(2) 1.2003(2) 0.76566(19) 0.079(2) Uani 1 1 d . . . . .
O347 O 0.47991(19) 0.80117(18) 0.60653(12) 0.0499(14) Uani 1 1 d . . . . .
O348 O 0.4675(2) 0.7775(2) 0.50302(13) 0.0621(17) Uani 1 1 d . . . . .
O349 O 0.0360(2) 0.64118(18) 0.39062(12) 0.0570(16) Uani 1 1 d . . . . .
O350 O 0.3801(2) 0.9164(2) 0.61967(13) 0.0602(17) Uani 1 1 d . . . . .
O351 O 0.1298(2) 0.4102(2) 1.03253(17) 0.073(2) Uani 1 1 d . . . . .
O352 O 0.2189(2) 1.1805(2) 0.82176(14) 0.0660(19) Uani 1 1 d . . . . .
O353 O 0.6109(2) 0.95667(19) 0.94612(13) 0.0588(16) Uani 1 1 d . . . . .
O354 O 0.0917(2) 0.7502(2) 0.91366(15) 0.076(2) Uani 1 1 d . . . . .
O355 O 0.3216(2) 0.61030(17) 0.52983(12) 0.0501(14) Uani 1 1 d . . . . .
O356 O 0.4235(2) 0.8711(2) 1.02019(13) 0.0620(17) Uani 1 1 d . . . . .
O357 O 0.4170(2) 0.84067(19) 0.51537(12) 0.0570(16) Uani 1 1 d . . . . .
O358 O 0.7410(3) 0.8269(3) 0.92466(14) 0.082(2) Uani 1 1 d . U . . .
O359 O 0.3400(2) 0.69316(19) 0.44559(12) 0.0567(16) Uani 1 1 d . . . . .
O360 O 0.9040(2) 0.68617(19) 0.92231(13) 0.0643(19) Uani 1 1 d . . . . .
O361 O 0.1873(2) 0.64900(17) 0.47851(12) 0.0523(15) Uani 1 1 d . . . . .
O362 O 0.1190(2) 1.40830(17) 0.66497(12) 0.0515(15) Uani 1 1 d . . . . .
O363 O 0.3772(2) 0.65240(18) 0.48635(12) 0.0528(15) Uani 1 1 d . . . . .
O364 O 0.7109(2) 0.4459(2) 0.77434(19) 0.081(2) Uani 1 1 d . . . . .
O365 O 0.3182(2) 0.94869(19) 0.69193(13) 0.0605(17) Uani 1 1 d . . . . .
O366 O 0.1521(2) 1.16965(18) 0.77587(16) 0.0637(18) Uani 1 1 d . . . . .
O367 O 0.0711(3) 0.5275(2) 0.47226(16) 0.085(2) Uani 1 1 d . . . . .
O368 O 0.2454(2) 0.8094(2) 0.73418(14) 0.0677(18) Uani 1 1 d . . . . .
O369 O 0.1937(3) 0.7836(2) 0.33344(16) 0.082(2) Uani 1 1 d . . . . .
O370 O 0.1955(2) 0.6653(2) 0.58424(15) 0.076(2) Uani 1 1 d . . . . .
O371 O 0.2985(3) 1.3719(3) 0.6660(2) 0.100(3) Uani 1 1 d . . . . .
O372 O 0.5223(3) 0.8231(2) 0.97422(19) 0.090(3) Uani 1 1 d . . . . .
O373 O 0.2607(3) 0.7069(3) 0.9159(2) 0.106(3) Uani 1 1 d . U . . .
O374 O 0.5312(3) 0.6608(2) 0.7608(2) 0.094(3) Uani 1 1 d . U . . .
O375 O 0.1120(3) 0.79017(19) 0.30044(17) 0.080(2) Uani 1 1 d . . . . .
O376 O 0.2081(2) 1.4263(2) 0.66592(15) 0.0655(18) Uani 1 1 d . . . . .
O377 O 0.0316(2) 0.5970(3) 0.46802(14) 0.079(2) Uani 1 1 d . . . . .
O378 O 0.2512(2) 0.7519(2) 0.64915(16) 0.079(2) Uani 1 1 d . . . . .
O379 O 0.7792(3) 0.7167(3) 0.9239(2) 0.093(3) Uani 1 1 d . . . . .
O380 O 0.6258(2) 0.8789(2) 0.95105(13) 0.070(2) Uani 1 1 d . . . . .
O381 O 0.2689(3) 0.8838(2) 1.09975(17) 0.093(3) Uani 1 1 d . . . . .
O382 O 0.8097(3) 0.8719(3) 0.9035(2) 0.102(3) Uani 1 1 d . . . . .
O383 O 0.4456(3) 0.9930(2) 0.53971(15) 0.089(3) Uani 1 1 d . . . . .
O384 O 0.2094(2) 1.3475(2) 0.64181(14) 0.0641(18) Uani 1 1 d . . . . .
O385 O -0.0340(4) 1.1786(3) 0.6896(2) 0.120(4) Uani 1 1 d . . . . .
O386 O 0.4414(3) 1.2164(2) 0.6670(2) 0.109(3) Uani 1 1 d . . . . .
O387 O 0.1839(3) 0.6681(2) 0.89351(19) 0.094(3) Uani 1 1 d . U . . .
O388 O -0.0592(2) 0.6475(2) 0.36771(16) 0.0710(19) Uani 1 1 d . . . . .
O389 O 0.4139(2) 1.2727(2) 0.74685(17) 0.073(2) Uani 1 1 d . . . . .
O390 O 0.2629(3) 0.79078(19) 1.04132(15) 0.069(2) Uani 1 1 d . . . . .
O391 O 0.1392(3) 0.9015(2) 0.7398(2) 0.088(2) Uani 1 1 d . . . . .
O392 O 0.5095(2) 0.8550(2) 1.02713(14) 0.0673(19) Uani 1 1 d . . . . .
O393 O 0.4268(2) 1.07984(18) 0.63086(13) 0.0614(18) Uani 1 1 d . . . . .
O394 O 0.5045(2) 0.8635(2) 0.54197(16) 0.078(2) Uani 1 1 d . . . . .
O395 O 0.7022(3) 0.8552(3) 0.97070(15) 0.095(3) Uani 1 1 d . U . . .
O396 O 0.4006(4) 0.9053(2) 0.48706(17) 0.103(3) Uani 1 1 d . . . . .
O397 O 0.1296(3) 1.1099(3) 0.8126(3) 0.118(3) Uani 1 1 d . U . . .
O398 O 0.0909(3) 0.6557(3) 0.88236(18) 0.101(3) Uani 1 1 d . . . . .
O399 O 0.2397(3) 0.7323(2) 0.36342(17) 0.085(3) Uani 1 1 d . . . . .
O400 O 0.2377(3) 0.8658(3) 0.66100(16) 0.082(2) Uani 1 1 d . . . . .
O401 O 0.2146(3) 0.8926(2) 0.77123(16) 0.077(2) Uani 1 1 d . . . . .
O402 O 0.6623(3) 0.3746(3) 0.7678(2) 0.100(3) Uani 1 1 d . U . . .
O403 O -0.0155(2) 0.49805(18) 0.34363(14) 0.0584(16) Uani 1 1 d . . . . .
O404 O 0.4019(3) 1.1402(2) 0.64609(15) 0.072(2) Uani 1 1 d . . . . .
O405 O 0.6855(2) 0.5144(2) 0.74775(18) 0.077(2) Uani 1 1 d . . . . .
O406 O 0.1475(3) 0.5784(3) 0.9681(2) 0.067(3) Uiso 0.7 1 d . . P E .
O407 O 0.5426(3) 0.9295(2) 1.01955(13) 0.074(2) Uani 1 1 d . . . . .
O408 O -0.1236(3) 0.5428(2) 0.3804(2) 0.094(3) Uani 1 1 d . . . . .
O409 O 0.7912(3) 0.7843(3) 0.95841(14) 0.088(3) Uani 1 1 d . . . . .
O410 O 0.8477(3) 0.6494(3) 0.9563(2) 0.100(3) Uani 1 1 d . . . F 1
O411 O 0.7007(3) 0.4079(3) 0.8197(2) 0.112(3) Uani 1 1 d . . . A 1
O412 O -0.0098(4) 0.5534(3) 0.5074(2) 0.064(3) Uiso 0.6 1 d . . P H .
O413 O 0.0899(3) 0.6128(2) 0.93050(17) 0.083(2) Uani 1 1 d . . . . .
O414 O 0.2215(2) 1.0449(2) 0.7698(2) 0.082(2) Uani 1 1 d . . . . .
O415 O 0.3359(3) 0.7718(2) 0.42931(16) 0.093(3) Uani 1 1 d . . . . .
O416 O 0.9465(3) 0.7303(2) 0.97012(15) 0.072(2) Uani 1 1 d . . . . .
O417 O 0.1231(3) 1.2278(2) 0.81607(17) 0.081(2) Uani 1 1 d . . . . .
O418 O 0.7424(3) 0.3814(2) 0.74678(19) 0.100(3) Uani 1 1 d . . . . .
O419 O 0.1962(2) 0.9665(2) 0.76004(19) 0.082(2) Uani 1 1 d . . . . .
O420 O 0.1014(3) 0.5324(2) 0.92407(18) 0.087(2) Uani 1 1 d . . . . .
O421 O 0.1792(3) 0.6985(3) 0.63629(17) 0.094(3) Uani 1 1 d . . . . .
O422 O 0.4866(3) 0.7211(3) 0.74032(18) 0.098(3) Uani 1 1 d . . . . .
O423 O 0.1755(3) 0.7763(3) 0.6259(2) 0.073(3) Uiso 0.7 1 d . . P B 1
O424 O 0.0162(3) 1.1514(3) 0.7965(2) 0.071(3) Uiso 0.7 1 d . . P . .
O425 O 0.4283(4) 1.0161(3) 0.5937(2) 0.058(2) Uiso 0.7 1 d . . P D 1
O426 O 0.2055(3) 0.7205(3) 0.6931(2) 0.063(2) Uiso 0.7 1 d . . P . .
O427 O 0.4148(3) 0.7389(3) 0.43854(17) 0.106(3) Uani 1 1 d . . . . .
O428 O 0.5414(3) 0.6924(3) 0.8164(2) 0.099(3) Uani 1 1 d . . . . .
O429 O 0.1836(3) 0.9450(3) 0.7014(2) 0.113(3) Uani 1 1 d . . . . .
O430 O 0.1402(3) 1.1143(3) 0.7287(2) 0.107(3) Uani 1 1 d . . . . .
O431 O -0.0570(3) 0.5964(3) 0.46885(18) 0.101(3) Uani 1 1 d . U . . .
O432 O 0.5922(2) 0.8684(3) 1.00306(15) 0.078(2) Uani 1 1 d . . . . .
O433 O 0.1154(3) 0.7597(2) 0.35242(15) 0.082(2) Uani 1 1 d . . . . .
O434 O 0.1672(3) 0.7195(3) 0.85364(19) 0.107(3) Uani 1 1 d . . . . .
O435 O 0.5124(7) 0.9558(6) 0.5893(5) 0.121(7) Uiso 0.5 1 d . . P . .
O436 O -0.0690(5) 0.6709(4) 0.4540(3) 0.083(4) Uiso 0.6 1 d . . P H 1
O437 O -0.1419(4) 0.5674(3) 0.4477(3) 0.075(3) Uiso 0.65 1 d . . P . .
O438 O 0.3871(3) 0.7213(3) 0.7628(2) 0.059(2) Uiso 0.7 1 d . . P . .
O439 O 0.3195(5) 1.2536(4) 0.6045(3) 0.101(4) Uiso 0.7 1 d . . P D 2
O440 O 0.5097(3) 1.0484(2) 0.62735(19) 0.092(3) Uani 1 1 d . . . . .
O441 O -0.0914(3) 1.1443(3) 0.7256(2) 0.063(2) Uiso 0.7 1 d . . P . .
O442 O 0.3075(3) 0.7887(3) 0.3751(2) 0.058(2) Uiso 0.7 1 d . . P . .
O443 O 0.7500(4) 0.8072(4) 1.0053(3) 0.081(3) Uiso 0.7 1 d . . P C 2
O444 O 0.6247(3) 0.6063(3) 0.7297(2) 0.060(2) Uiso 0.7 1 d . . P . .
O445 O 0.1060(3) 0.6795(3) 0.5164(2) 0.065(2) Uiso 0.7 1 d . . P . .
O446 O 0.3734(2) 1.21912(19) 0.70083(14) 0.0413(15) Uiso 0.8 1 d . . P . .
O447 O 0.4594(3) 0.6890(2) 0.78917(18) 0.062(2) Uiso 0.8 1 d . . P . .
O448 O -0.0128(3) 1.1869(2) 0.7484(2) 0.097(3) Uani 1 1 d . . . . .
O449 O 0.0422(3) 0.6249(3) 0.5244(2) 0.067(3) Uiso 0.7 1 d . . P H .
O450 O 0.3652(5) 0.9523(4) 0.5284(3) 0.106(4) Uiso 0.7 1 d . . P D 1
O452 O 0.4806(3) 0.9120(3) 1.0670(2) 0.072(3) Uiso 0.7 1 d . . P . .
O453 O 0.3266(3) 0.8354(3) 1.07519(19) 0.102(3) Uani 1 1 d . . . . .
O454 O -0.0095(4) 1.1061(3) 0.7453(2) 0.079(3) Uiso 0.7 1 d . . P . .
O455 O -0.0830(3) 0.6080(3) 0.41359(15) 0.089(3) Uani 1 1 d . . . . .
O456 O 0.1072(4) 0.6600(4) 0.5679(2) 0.069(3) Uiso 0.7 1 d . . P B 1
O457 O 0.3621(5) 1.0081(4) 0.5537(3) 0.055(3) Uiso 0.5 1 d . . P D 1
O458 O 0.7029(5) 0.7728(4) 0.9597(3) 0.102(4) Uiso 0.7 1 d D . P C 1
O459 O 0.2502(3) 0.6968(2) 0.85855(19) 0.090(3) Uani 1 1 d . U . . .
O460 O 0.6709(4) 0.9177(3) 1.0010(2) 0.059(3) Uiso 0.6 1 d . . P . .
O461 O 0.1314(3) 0.7446(3) 0.6698(2) 0.058(2) Uiso 0.7 1 d . . P . .
O462 O 0.2263(3) 1.3964(3) 0.5975(2) 0.072(3) Uiso 0.7 1 d . . P . .
O463 O -0.0938(3) 1.2124(2) 0.75784(18) 0.0474(19) Uiso 0.7 1 d . . P . .
O464 O 0.1081(4) 0.9821(3) 0.7562(2) 0.081(3) Uiso 0.7 1 d . . P . .
O465 O 0.4448(3) 0.8506(3) 0.4602(2) 0.055(3) Uiso 0.6 1 d . . P . .
O466 O 0.3002(4) 0.6503(3) 0.8270(2) 0.076(3) Uiso 0.7 1 d . . P . .
O467 O 0.6969(3) 0.2626(3) 0.8422(2) 0.059(2) Uiso 0.7 1 d . . P . .
O468 O 0.2739(3) 1.2986(3) 0.63807(16) 0.091(3) Uani 1 1 d . . . . .
O469 O 0.3766(3) 0.6507(3) 0.7876(2) 0.057(3) Uiso 0.6 1 d . . P . .
O470 O -0.1288(4) 0.6309(4) 0.4861(3) 0.057(3) Uiso 0.5 1 d . . P . .
O471 O 0.1455(4) 1.2998(4) 0.6067(3) 0.076(3) Uiso 0.6 1 d . . P . .
O472 O 0.1525(4) 1.3555(3) 0.5691(2) 0.062(3) Uiso 0.6 1 d . . P . .
O473 O 0.2272(3) 1.3172(3) 0.5901(2) 0.054(2) Uiso 0.6 1 d . . P . .
O474 O 0.2360(6) 1.2409(6) 0.5978(4) 0.096(5) Uiso 0.5 1 d D . P D 1
O475 O 0.2875(7) 1.1819(5) 0.5995(4) 0.092(5) Uiso 0.5 1 d D . P . .
O476 O 0.2792(5) 1.2764(4) 0.5573(3) 0.089(4) Uiso 0.6 1 d . . P . .
O479 O 0.3567(3) 1.2042(3) 0.63972(19) 0.065(2) Uiso 0.8 1 d . . P . .
O480 O 0.3624(4) 1.1528(4) 0.5924(3) 0.060(3) Uiso 0.6 1 d . . P . .
O481 O 0.3359(4) 1.0861(3) 0.6149(2) 0.058(3) Uiso 0.6 1 d . . P . .
O482 O 0.4533(4) 1.1438(3) 0.5993(2) 0.056(3) Uiso 0.6 1 d . . P D 1
O483 O 0.3928(3) 1.0795(3) 0.5746(2) 0.060(2) Uiso 0.7 1 d . . P . .
O484 O 0.4159(4) 1.0611(3) 0.5208(2) 0.069(3) Uiso 0.7 1 d . . P D 1
O485 O 0.5365(6) 1.1194(5) 0.6113(4) 0.086(5) Uiso 0.5 1 d . . P . .
O486 O 0.4012(6) 0.9832(4) 0.4855(3) 0.071(4) Uiso 0.5 1 d . . P D 2
O487 O 0.4831(3) 0.9476(3) 0.5002(2) 0.055(3) Uiso 0.6 1 d . . P . .
O488 O 0.3301(3) 0.8534(3) 0.4965(2) 0.058(3) Uiso 0.6 1 d . . P . .
O489 O 0.3568(3) 0.8500(3) 0.4438(2) 0.058(2) Uiso 0.7 1 d . . P . .
O490 O 0.3334(3) 0.8671(3) 0.3901(2) 0.057(3) Uiso 0.6 1 d . . P . .
O492 O 0.2752(4) 0.8228(4) 0.4226(3) 0.075(3) Uiso 0.6 1 d . . P . .
O493 O 0.2623(4) 0.8408(3) 0.3438(2) 0.061(3) Uiso 0.6 1 d . . P . .
O494 O 0.2778(4) 0.7710(3) 0.3189(2) 0.060(3) Uiso 0.6 1 d . . P . .
O495 O -0.0055(5) 0.6619(4) 0.4873(3) 0.089(4) Uiso 0.6 1 d . . P H .
O496 O -0.0470(4) 0.6194(4) 0.5258(3) 0.076(3) Uiso 0.6 1 d . . P H .
O498 O 0.0957(4) 0.5770(4) 0.5517(3) 0.092(4) Uiso 0.7 1 d . . P B .
O499 O 0.0924(5) 0.6796(5) 0.6243(3) 0.085(4) Uiso 0.6 1 d . . P B 1
O500 O 0.1399(4) 0.6236(4) 0.6175(3) 0.071(3) Uiso 0.6 1 d . . P . .
O501 O 0.1478(4) 0.7277(4) 0.5879(3) 0.080(4) Uiso 0.6 1 d . . P B 1
O502 O 0.7209(5) 0.2616(4) 0.7863(3) 0.084(4) Uiso 0.6 1 d . . P A 1
O503 O 0.7066(5) 0.3414(4) 0.8492(3) 0.110(4) Uiso 0.7 1 d . . P A 1
O504 O 0.1353(3) 1.0591(3) 0.7672(2) 0.063(2) Uiso 0.7 1 d . . P . .
O505 O 0.0766(3) 1.1197(3) 0.7657(2) 0.047(2) Uiso 0.6 1 d . . P . .
O506 O 0.0480(5) 1.1516(4) 0.7165(3) 0.084(4) Uiso 0.6 1 d . . P . .
O508 O 0.1617(4) 1.0064(4) 0.8057(3) 0.073(3) Uiso 0.6 1 d . . P . .
O509 O 0.2595(4) 0.7113(3) 0.8016(3) 0.069(3) Uiso 0.6 1 d . . P . .
O510 O 0.3368(4) 0.7008(4) 0.8714(3) 0.082(4) Uiso 0.6 1 d . . P . .
O511 O 0.2875(4) 0.8151(3) 1.1599(3) 0.066(3) Uiso 0.6 1 d . . P . .
O512 O 0.2908(4) 0.7265(3) 1.1006(2) 0.065(3) Uiso 0.6 1 d . . P . .
O513 O 0.3428(4) 0.7961(4) 1.1244(3) 0.066(3) Uiso 0.6 1 d . . P G 1
O514 O 0.7940(4) 0.8650(3) 0.9726(2) 0.065(3) Uiso 0.6 1 d . . P . .
O515 O 0.6553(5) 0.3003(4) 0.7996(3) 0.085(4) Uiso 0.6 1 d . . P A 1
O516 O 0.5894(4) 0.6126(3) 0.7830(3) 0.067(3) Uiso 0.6 1 d . . P . .
O517 O 0.5642(4) 0.6531(3) 0.7076(2) 0.065(3) Uiso 0.6 1 d . . P . .
O518 O 0.6273(4) 0.8096(4) 0.9763(3) 0.058(3) Uiso 0.5 1 d D . P C 1
O519 O 0.1655(4) 1.0191(4) 0.7226(3) 0.082(4) Uiso 0.6 1 d . . P . .
O520 O 0.6432(4) 0.5686(3) 0.7788(3) 0.068(3) Uiso 0.6 1 d . . P I 1
O521 O 0.5357(4) 0.5883(3) 0.7329(3) 0.068(3) Uiso 0.6 1 d . . P . .
O523 O 0.1390(4) 0.5941(3) 0.8854(2) 0.058(3) Uiso 0.6 1 d . . P . .
O524 O 0.1796(4) 0.6265(4) 0.9391(3) 0.083(4) Uiso 0.6 1 d . . P E 1
O525 O 0.6758(4) 0.8531(4) 1.0243(3) 0.073(3) Uiso 0.6 1 d . . P C 1
O526 O 0.6005(4) 0.5251(3) 0.7298(2) 0.065(3) Uiso 0.6 1 d . . P I 1
O527 O 0.6674(4) 0.5529(3) 0.6989(2) 0.064(3) Uiso 0.6 1 d . . P . .
O528 O 0.3919(4) 0.8150(4) 0.3967(3) 0.073(3) Uiso 0.6 1 d . . P . .
O529 O 0.2224(4) 0.8028(3) 0.3871(2) 0.064(3) Uiso 0.6 1 d . . P . .
O530 O 0.4777(3) 1.0686(3) 0.5594(2) 0.053(2) Uiso 0.6 1 d . . P . .
O531 O 0.4065(6) 1.2325(5) 0.5989(3) 0.099(4) Uiso 0.6 1 d . . P . .
O532 O 0.3411(4) 1.2108(4) 0.5588(3) 0.078(3) Uiso 0.6 1 d . . P . .
O533 O 0.4139(4) 0.8549(3) 1.0751(3) 0.066(3) Uiso 0.6 1 d . . P . .
O534 O 0.5015(3) 0.8408(3) 1.0840(2) 0.064(3) Uiso 0.6 1 d D . P . .
O535 O 0.4493(4) 0.8050(3) 1.0415(2) 0.079(3) Uiso 0.7 1 d . . P . .
O536 O 0.3856(11) 0.7897(6) 1.0798(6) 0.131(11) Uiso 0.4 1 d D . P G 1
O537 O 0.3742(6) 0.8711(5) 1.1271(4) 0.102(6) Uiso 0.5 1 d D . P . .
O538 O 0.4318(5) 0.8070(4) 1.1205(3) 0.074(4) Uiso 0.45 1 d D . P . .
O541 O 0.3163(5) 1.3345(4) 0.5952(3) 0.088(4) Uiso 0.6 1 d . . P . .
O601 O 0.2852(2) 0.83840(18) 0.78647(13) 0.0538(15) Uiso 1 1 d . . . . .
O602 O 0.5655(3) 0.8692(2) 0.70203(17) 0.058(2) Uiso 0.8 1 d . . P . .
O603 O 0.9290(3) 0.5313(2) 0.69344(17) 0.058(2) Uiso 0.8 1 d . . P . .
O604 O 0.3989(2) 1.0157(2) 0.99797(15) 0.0667(18) Uiso 1 1 d . . . . .
O605 O -0.0121(3) 0.7355(3) 1.2148(2) 0.077(3) Uiso 0.8 1 d . . P . .
O606 O -0.1431(2) 1.2787(2) 0.77343(16) 0.0690(18) Uiso 1 1 d . . . . .
O607 O 0.2910(3) 0.7457(3) 0.74425(19) 0.067(2) Uiso 0.8 1 d . . P . .
O608 O 0.8216(3) 0.3429(3) 0.7832(2) 0.065(3) Uiso 0.7 1 d . . P . .
O609 O 0.3510(3) 0.7948(3) 0.7938(2) 0.082(3) Uiso 0.8 1 d . . P . .
O610 O 0.0690(3) 1.3706(3) 0.8444(2) 0.077(3) Uiso 0.8 1 d . . P . .
O611 O 0.4057(3) 1.0141(3) 0.85079(19) 0.056(2) Uiso 0.7 1 d . . P . .
O612 O 0.3454(4) 0.9227(3) 1.0506(2) 0.093(3) Uiso 0.8 1 d . . P . .
O613 O 0.2439(3) 0.7024(3) 0.2714(2) 0.057(2) Uiso 0.7 1 d . . P . .
O614 O 0.0311(4) 0.6863(3) 0.9626(2) 0.078(3) Uiso 0.7 1 d . . P . .
O615 O 0.0003(4) 0.6471(4) 0.9089(3) 0.102(4) Uiso 0.7 1 d . . P . .
O616 O 0.2807(3) 0.9771(3) 0.79682(19) 0.055(2) Uiso 0.7 1 d . . P . .
O617 O 0.2894(4) 1.0010(3) 0.8962(2) 0.060(3) Uiso 0.6 1 d . . P . .
O618 O -0.0338(4) 0.7421(4) 1.1181(3) 0.083(4) Uiso 0.6 1 d . . P . .
O619 O 0.8425(3) 0.6264(3) 0.6871(2) 0.056(3) Uiso 0.6 1 d . . P . .
O620 O 0.0666(4) 1.2861(4) 0.8329(3) 0.071(3) Uiso 0.6 1 d . . P . .
O621 O 0.7560(4) 0.5210(3) 0.6853(2) 0.076(3) Uiso 0.7 1 d . . P . .
O622 O 0.1783(4) 0.8699(3) 0.8314(2) 0.063(3) Uiso 0.6 1 d . . P . .
O623 O 0.7055(5) 0.6742(5) 0.7148(3) 0.100(5) Uiso 0.6 1 d . . P . .
O624 O 0.3182(4) 1.0271(4) 0.8451(3) 0.090(3) Uiso 0.7 1 d . . P . .
O625 O 0.5610(8) 0.9826(7) 0.7555(5) 0.171(9) Uiso 0.6 1 d . . P . .
O626 O 0.6636(4) 0.7932(4) 0.6935(3) 0.074(3) Uiso 0.6 1 d . . P . .
O627 O 0.5859(6) 0.3613(5) 0.7348(4) 0.117(5) Uiso 0.6 1 d . . P . .
O628 O 0.1220(4) 0.4497(3) 0.9400(2) 0.063(3) Uiso 0.6 1 d . . P . .
O629 O 0.7698(5) 0.8960(5) 0.7567(3) 0.079(4) Uiso 0.5 1 d . . P . .
O630 O 0.7104(4) 0.9120(4) 0.9240(3) 0.072(3) Uiso 0.6 1 d . . P . .
O631 O 0.5374(5) 0.7361(4) 0.6956(3) 0.092(4) Uiso 0.6 1 d . . P . .
O632 O 0.9615(4) 0.7997(3) 0.9414(2) 0.059(3) Uiso 0.6 1 d . . P . .
O633 O 0.1902(4) 0.7528(4) 0.8039(3) 0.071(3) Uiso 0.6 1 d . . P . .
O634 O -0.0297(4) 1.2098(4) 0.8199(3) 0.082(4) Uiso 0.6 1 d . . P . .
O635 O 0.9162(5) 0.6816(5) 0.6993(3) 0.077(4) Uiso 0.5 1 d . . P . .
O636 O 0.2063(4) 0.4871(4) 0.3637(3) 0.061(3) Uiso 0.5 1 d . . P . .
O637 O 0.5305(7) 1.0095(6) 0.8117(5) 0.119(7) Uiso 0.5 1 d . . P . .
O638 O 0.2160(5) 0.9495(4) 0.8313(3) 0.067(4) Uiso 0.5 1 d . . P . .
O639 O 0.5786(5) 0.8023(5) 0.6704(3) 0.077(4) Uiso 0.5 1 d . . P . .
O640 O -0.2067(4) 0.5281(3) 0.3944(2) 0.060(3) Uiso 0.6 1 d . . P . .
O641 O 0.5236(4) 0.8732(3) 0.4891(2) 0.061(3) Uiso 0.6 1 d . . P . .
O642 O 0.1182(5) 0.8191(4) 1.1835(3) 0.094(4) Uiso 0.6 1 d . . P . .
O643 O -0.0327(5) 0.5309(4) 0.4271(3) 0.067(4) Uiso 0.5 1 d . . P . .
O644 O 0.1354(5) 0.4428(5) 0.3410(3) 0.079(4) Uiso 0.5 1 d . . P . .
O645 O 0.1037(5) 0.8792(4) 0.8656(3) 0.069(4) Uiso 0.5 1 d . . P . .
O648 O 0.3241(6) 1.1081(5) 0.8571(4) 0.093(5) Uiso 0.5 1 d . . P . .
O649 O 0.5912(4) 0.9098(3) 1.0680(3) 0.068(3) Uiso 0.6 1 d . . P . .
O650 O -0.2336(5) 0.4916(4) 0.4415(3) 0.072(4) Uiso 0.5 1 d . . P . .
O651 O 0.0914(5) 1.1645(4) 0.8424(3) 0.074(4) Uiso 0.5 1 d . . P . .
O652 O 0.3887(5) 0.6943(4) 0.7047(3) 0.075(4) Uiso 0.5 1 d . . P . .
O653 O 0.1508(7) 1.4526(6) 0.7939(4) 0.111(6) Uiso 0.5 1 d . . P . .
O654 O 0.5814(6) 1.0406(5) 0.6622(4) 0.090(5) Uiso 0.5 1 d . . P . .
O655 O 0.2842(6) 0.5992(5) 0.3109(4) 0.093(5) Uiso 0.5 1 d . . P . .
O656 O 0.9607(5) 0.7120(5) 0.7511(4) 0.085(5) Uiso 0.5 1 d . . P . .
O657 O 0.4011(8) 1.1554(7) 0.8643(5) 0.129(7) Uiso 0.5 1 d . . P . .
O658 O 0.5827(7) 1.0405(6) 0.8588(5) 0.118(7) Uiso 0.5 1 d . . P . .
O659 O 0.8774(7) 0.8138(6) 0.7427(4) 0.109(6) Uiso 0.5 1 d . . P . .
O660 O 0.5108(6) 1.0827(6) 0.8024(4) 0.105(6) Uiso 0.5 1 d . . P . .
O661 O 0.2678(5) 0.6628(5) 0.6369(4) 0.061(4) Uiso 0.4 1 d . . P . .
O662 O 0.7690(7) 0.5363(6) 0.8630(5) 0.085(6) Uiso 0.4 1 d . . P . .
O663 O 0.4090(6) 0.5718(5) 0.5070(4) 0.074(5) Uiso 0.4 1 d . . P . .
O664 O 0.1863(6) 1.0779(6) 0.8515(4) 0.127(6) Uiso 0.6 1 d . . P . .
O665 O 0.0885(5) 0.5005(5) 0.5270(3) 0.055(4) Uiso 0.4 1 d . . P . .
O666 O 0.4659(7) 0.6741(6) 0.4413(5) 0.086(6) Uiso 0.4 1 d . . P . .
O667 O 0.4806(6) 0.7905(5) 0.4318(4) 0.067(4) Uiso 0.4 1 d . . P . .
O668 O 0.6036(5) 0.8312(5) 1.0692(3) 0.077(4) Uiso 0.5 1 d . . P . .
O669 O 0.5877(5) 0.7859(5) 0.6130(3) 0.079(4) Uiso 0.5 1 d . . P . .
O670 O 0.3743(7) 1.2945(6) 0.6685(4) 0.081(5) Uiso 0.4 1 d . . P . .
O671 O 0.0802(6) 0.7324(6) 0.8547(4) 0.077(5) Uiso 0.4 1 d . . P . .
O672 O 0.4514(5) 1.0739(4) 0.8836(3) 0.070(4) Uiso 0.5 1 d . . P . .
O673 O 0.0622(6) 0.8209(5) 0.8967(4) 0.063(4) Uiso 0.4 1 d . . P . .
O674 O 0.5711(5) 0.8265(5) 0.5647(3) 0.058(4) Uiso 0.4 1 d . . P . .
O675 O 0.3328(7) 1.4206(6) 0.7124(5) 0.089(6) Uiso 0.4 1 d . . P . .
O676 O 0.6071(7) 1.0145(6) 0.7128(5) 0.088(6) Uiso 0.4 1 d . . P . .
O677 O 0.7554(6) 0.1937(6) 0.7921(4) 0.075(5) Uiso 0.4 1 d . . P . .
O678 O 0.3388(7) 0.7024(6) 0.3784(5) 0.090(6) Uiso 0.4 1 d . . P . .
O679 O 0.6946(5) 0.9935(5) 0.9453(4) 0.062(4) Uiso 0.4 1 d . . P . .
O680 O 0.3179(6) 0.5105(5) 0.4346(4) 0.069(5) Uiso 0.4 1 d . . P . .
O681 O 0.4165(4) 0.9724(4) 1.0697(3) 0.080(4) Uiso 0.6 1 d . . P . .
O682 O 0.6608(5) 0.9557(4) 1.0513(3) 0.075(4) Uiso 0.5 1 d . . P . .
O683 O 0.2075(5) 0.9382(5) 1.0952(3) 0.078(4) Uiso 0.5 1 d . . P . .
O684 O 1.0326(6) 0.6063(6) 0.7751(4) 0.077(5) Uiso 0.4 1 d . . P . .
O685 O 0.1014(6) 0.6442(5) 0.8226(4) 0.073(5) Uiso 0.4 1 d . . P . .
O686 O 0.0935(6) 0.4585(6) 0.4415(4) 0.077(5) Uiso 0.4 1 d . . P . .
O687 O 0.7332(6) 0.9963(5) 0.8940(4) 0.068(5) Uiso 0.4 1 d . . P . .
O688 O -0.2176(6) 0.5411(5) 0.4910(4) 0.071(5) Uiso 0.4 1 d . . P . .
O689 O 0.5035(6) 1.2121(6) 0.6271(4) 0.077(5) Uiso 0.4 1 d . . P . .
O690 O 0.1830(6) 0.9787(5) 0.9575(4) 0.074(5) Uiso 0.4 1 d . . P . .
O691 O 0.2049(6) 0.8302(6) 0.2725(4) 0.079(5) Uiso 0.4 1 d . . P . .
O692 O 0.5795(7) 1.0784(6) 0.5753(4) 0.080(5) Uiso 0.4 1 d . . P . .
O693 O 0.2473(6) 1.3931(5) 0.5392(4) 0.073(5) Uiso 0.4 1 d . . P . .
O694 O -0.1225(6) 0.4754(6) 0.3476(4) 0.078(5) Uiso 0.4 1 d . . P . .
O695 O 0.1400(7) 0.9619(6) 1.0618(4) 0.082(5) Uiso 0.4 1 d . . P . .
O696 O 0.0393(6) 0.9674(6) 0.5041(4) 0.103(6) Uiso 0.5 1 d . . P . .
O697 O 0.0507(8) 1.5059(7) 0.7505(5) 0.099(7) Uiso 0.4 1 d . . P . .
O698 O 0.3815(7) 1.3027(6) 0.8214(5) 0.087(6) Uiso 0.4 1 d . . P . .
O725 O 0.4503(8) 1.0249(6) 0.5953(4) 0.048(5) Uiso 0.3 1 d . . P D 2
O739 O 0.3404(6) 1.2673(5) 0.6094(4) 0.038(4) Uiso 0.3 1 d . . P D 1
O743 O 0.7663(7) 0.8245(6) 1.0063(4) 0.044(5) Uiso 0.3 1 d . . P C 1
O756 O 0.1072(6) 0.6436(6) 0.5729(4) 0.042(5) Uiso 0.3 1 d . . P B 2
O780 O 0.3826(9) 1.1645(7) 0.5944(5) 0.062(6) Uiso 0.3 1 d . . P D 2
O783 O 0.4161(8) 1.0931(6) 0.5765(4) 0.052(5) Uiso 0.3 1 d . . P D 2
O784 O 0.3962(9) 1.0544(7) 0.5194(5) 0.055(6) Uiso 0.3 1 d . . P D 2
O786 O 0.4255(7) 0.9852(6) 0.4816(4) 0.070(5) Uiso 0.4 1 d . . P D 1
O799 O 0.0893(7) 0.6984(7) 0.6161(5) 0.056(5) Uiso 0.3 1 d . . P B 2
O813 O 0.3440(6) 0.7795(6) 1.1138(4) 0.070(5) Uiso 0.4 1 d . . P G 2
O815 O 0.6494(8) 0.3153(7) 0.8137(6) 0.067(6) Uiso 0.3 1 d . . P A 2
O825 O 0.6627(8) 0.8315(7) 1.0224(5) 0.059(6) Uiso 0.3 1 d . . P C 2
O836 O 0.3808(9) 0.7726(8) 1.0695(6) 0.074(7) Uiso 0.3 1 d . . P G 2
C1 C 0.2390(5) 0.8040(4) 0.4121(3) 0.039(3) Uiso 0.5 1 d D . P . .
C2 C 0.2079(6) 0.7828(6) 0.4302(4) 0.057(6) Uiso 0.4 1 d D . P . .
C3 C 0.2220(8) 0.7867(7) 0.4612(4) 0.083(7) Uiso 0.5 1 d D . P . .
C11 C 0.3569(6) 0.9754(6) 0.5496(4) 0.058(5) Uiso 0.5 1 d D . P . .
C12 C 0.3269(8) 0.9526(7) 0.5678(5) 0.094(8) Uiso 0.5 1 d D . P D .
C13 C 0.3151(9) 0.9766(8) 0.5936(5) 0.093(8) Uiso 0.5 1 d D . P . .
C21 C -0.0223(10) 0.6736(9) 0.4618(7) 0.089(9) Uiso 0.4 1 d D . P . .
C22 C 0.0050(9) 0.6940(9) 0.4405(5) 0.083(8) Uiso 0.4 1 d D . P H .
C23 C -0.0216(10) 0.7049(9) 0.4143(6) 0.082(8) Uiso 0.4 1 d D . P . .
C31 C 0.1741(6) 0.7577(5) 0.6003(4) 0.053(4) Uiso 0.5 1 d D . P . .
C32 C 0.2004(7) 0.7804(6) 0.5802(4) 0.080(6) Uiso 0.5 1 d D . P B .
C33 C 0.2010(8) 0.7686(7) 0.5491(4) 0.080(6) Uiso 0.5 1 d D . P . .
C51 C 0.1862(13) 0.9857(12) 0.7062(8) 0.113(12) Uiso 0.4 1 d D . P . .
C52 C 0.2149(12) 1.0089(8) 0.6874(7) 0.112(12) Uiso 0.4 1 d D . P . .
C53 C 0.2152(15) 1.0525(9) 0.6852(10) 0.126(14) Uiso 0.4 1 d D . P . .
C61 C 0.2582(10) 1.2095(8) 0.6104(7) 0.103(9) Uiso 0.4 1 d D U P D .
C62 C 0.2324(10) 1.1896(9) 0.6324(8) 0.107(8) Uiso 0.4 1 d D U P . .
C63 C 0.1906(10) 1.2065(10) 0.6388(8) 0.098(9) Uiso 0.4 1 d D U P D .
C71 C 0.6276(6) 0.5999(6) 0.7913(4) 0.061(5) Uiso 0.5 1 d D U P I .
C72 C 0.6522(6) 0.6187(6) 0.8188(4) 0.066(5) Uiso 0.5 1 d D U P . .
C73 C 0.6217(10) 0.6394(9) 0.8374(6) 0.114(9) Uiso 0.5 1 d D U P I .
C81 C 0.6583(7) 0.7926(9) 0.9543(6) 0.102(8) Uiso 0.4 1 d D U P . .
C82 C 0.6324(8) 0.7698(8) 0.9286(6) 0.084(7) Uiso 0.4 1 d D U P C .
C83 C 0.5840(8) 0.7733(10) 0.9234(7) 0.088(8) Uiso 0.4 1 d D U P . .
C91 C 0.1720(6) 0.6122(5) 0.9647(4) 0.034(4) Uiso 0.4 1 d D U P . .
C92 C 0.2019(7) 0.6366(6) 0.9874(4) 0.060(5) Uiso 0.4 1 d D U P E .
C93 C 0.2496(8) 0.6424(13) 0.9808(10) 0.129(12) Uiso 0.4 1 d D U P . .
C101 C 0.8479(4) 0.6124(3) 0.9517(2) 0.043(3) Uiso 0.7 1 d D U P . .
C102 C 0.8167(4) 0.5961(4) 0.9264(3) 0.057(3) Uiso 0.7 1 d D U P F .
C103 C 0.8151(7) 0.5529(4) 0.9214(5) 0.101(6) Uiso 0.7 1 d D U P . .
N0 N 0.1617(7) 0.7740(11) 0.4214(8) 0.142(13) Uiso 0.4 1 d D . P . .
N1 N 0.3040(13) 0.9139(8) 0.5598(9) 0.162(15) Uiso 0.4 1 d D . P . .
N2 N 0.0488(10) 0.7116(13) 0.4516(9) 0.166(16) Uiso 0.4 1 d D . P . .
N3 N 0.2267(9) 0.8168(7) 0.5891(7) 0.108(9) Uiso 0.4 1 d D . P . .
N5 N 0.2393(8) 0.9852(7) 0.6689(5) 0.080(7) Uiso 0.4 1 d D . P . .
N6 N 0.2420(11) 1.1510(8) 0.6407(7) 0.119(10) Uiso 0.4 1 d D . P D .
N7 N 0.6790(10) 0.5907(8) 0.8326(7) 0.116(10) Uiso 0.4 1 d D . P I .
N8 N 0.6523(10) 0.7424(8) 0.9105(6) 0.106(9) Uiso 0.4 1 d D . P . .
N9 N 0.1968(7) 0.6183(6) 1.0136(4) 0.066(5) Uiso 0.4 1 d D . P . .
N10 N 0.7749(6) 0.6143(7) 0.9244(5) 0.080(7) Uiso 0.4 1 d D . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O162 Mo1A O311 100.6(3) . . ?
O162 Mo1A O89 100.4(3) . . ?
O311 Mo1A O89 71.8(2) . . ?
O162 Mo1A O167 93.5(3) . . ?
O311 Mo1A O167 71.5(2) . . ?
O89 Mo1A O167 142.6(2) . . ?
O162 Mo1A O172 94.2(2) . . ?
O311 Mo1A O172 142.5(2) . . ?
O89 Mo1A O172 71.7(2) . . ?
O167 Mo1A O172 142.0(2) . . ?
O162 Mo1A O82 98.4(3) . . ?
O311 Mo1A O82 138.5(2) . . ?
O89 Mo1A O82 139.3(2) . . ?
O167 Mo1A O82 70.83(19) . . ?
O172 Mo1A O82 71.2(2) . . ?
O162 Mo1A O135 172.7(3) . . ?
O311 Mo1A O135 85.2(2) . . ?
O89 Mo1A O135 85.4(2) . . ?
O167 Mo1A O135 84.3(2) . . ?
O172 Mo1A O135 83.5(2) . . ?
O82 Mo1A O135 74.36(19) . . ?
O75 Mo1B O69 103.7(3) . . ?
O75 Mo1B O109 105.9(2) . . ?
O69 Mo1B O109 98.9(2) . . ?
O75 Mo1B O32 106.0(3) . . ?
O69 Mo1B O32 96.5(2) . . ?
O109 Mo1B O32 139.9(2) . . ?
O75 Mo1B O55 97.9(3) . . ?
O69 Mo1B O55 158.4(2) . . ?
O109 Mo1B O55 76.5(2) . . ?
O32 Mo1B O55 75.7(2) . . ?
O75 Mo1B O23 177.2(2) . . ?
O69 Mo1B O23 73.5(2) . . ?
O109 Mo1B O23 74.82(18) . . ?
O32 Mo1B O23 74.51(19) . . ?
O55 Mo1B O23 84.94(19) . . ?
O70 Mo1C O318 104.6(4) . . ?
O70 Mo1C O183 100.8(3) . . ?
O318 Mo1C O183 105.9(3) . . ?
O70 Mo1C O91 95.8(3) . . ?
O318 Mo1C O91 89.9(3) . . ?
O183 Mo1C O91 153.2(2) . . ?
O70 Mo1C O34 94.0(3) . . ?
O318 Mo1C O34 152.9(3) . . ?
O183 Mo1C O34 89.5(2) . . ?
O91 Mo1C O34 68.3(2) . . ?
O70 Mo1C O258 171.4(3) . . ?
O318 Mo1C O258 83.1(4) . . ?
O183 Mo1C O258 80.4(2) . . ?
O91 Mo1C O258 80.3(2) . . ?
O34 Mo1C O258 77.5(2) . . ?
O154 Mo1D O356 102.9(3) . . ?
O154 Mo1D O161 101.1(3) . . ?
O356 Mo1D O161 106.2(3) . . ?
O154 Mo1D O262 96.9(3) . . ?
O356 Mo1D O262 89.3(3) . . ?
O161 Mo1D O262 152.8(2) . . ?
O154 Mo1D O12 94.5(2) . . ?
O356 Mo1D O12 153.7(3) . . ?
O161 Mo1D O12 89.3(2) . . ?
O262 Mo1D O12 68.9(2) . . ?
O154 Mo1D O298 171.2(3) . . ?
O356 Mo1D O298 83.6(3) . . ?
O161 Mo1D O298 82.5(2) . . ?
O262 Mo1D O298 77.1(2) . . ?
O12 Mo1D O298 77.4(2) . . ?
O94 Mo1E O189 103.8(3) . . ?
O94 Mo1E O49 99.3(3) . . ?
O189 Mo1E O49 89.0(2) . . ?
O94 Mo1E O297 103.1(3) . . ?
O189 Mo1E O297 86.9(2) . . ?
O49 Mo1E O297 157.5(2) . . ?
O94 Mo1E O63 99.6(3) . . ?
O189 Mo1E O63 156.5(2) . . ?
O49 Mo1E O63 88.9(2) . . ?
O297 Mo1E O63 86.2(2) . . ?
O94 Mo1E O59 167.3(2) . . ?
O189 Mo1E O59 87.1(2) . . ?
O49 Mo1E O59 74.1(2) . . ?
O297 Mo1E O59 83.7(2) . . ?
O63 Mo1E O59 69.84(19) . . ?
O115 Mo1F O231 99.8(3) . . ?
O115 Mo1F O236 101.4(3) . . ?
O231 Mo1F O236 71.3(3) . . ?
O115 Mo1F O269 94.3(3) . . ?
O231 Mo1F O269 71.8(2) . . ?
O236 Mo1F O269 141.8(2) . . ?
O115 Mo1F O181 93.7(3) . . ?
O231 Mo1F O181 142.4(2) . . ?
O236 Mo1F O181 71.6(2) . . ?
O269 Mo1F O181 142.2(2) . . ?
O115 Mo1F O24 98.3(3) . . ?
O231 Mo1F O24 139.7(2) . . ?
O236 Mo1F O24 138.7(2) . . ?
O269 Mo1F O24 71.1(2) . . ?
O181 Mo1F O24 71.1(2) . . ?
O115 Mo1F O278 171.6(3) . . ?
O231 Mo1F O278 87.1(2) . . ?
O236 Mo1F O278 85.3(2) . . ?
O269 Mo1F O278 83.2(2) . . ?
O181 Mo1F O278 83.6(2) . . ?
O24 Mo1F O278 73.3(2) . . ?
O284 Mo1G O139 99.3(3) . . ?
O284 Mo1G O163 101.8(3) . . ?
O139 Mo1G O163 71.3(2) . . ?
O284 Mo1G O164 93.2(2) . . ?
O139 Mo1G O164 142.5(2) . . ?
O163 Mo1G O164 71.6(2) . . ?
O284 Mo1G O272 94.8(2) . . ?
O139 Mo1G O272 72.2(2) . . ?
O163 Mo1G O272 141.7(2) . . ?
O164 Mo1G O272 141.9(2) . . ?
O284 Mo1G O19 97.0(3) . . ?
O139 Mo1G O19 140.9(2) . . ?
O163 Mo1G O19 138.7(2) . . ?
O164 Mo1G O19 70.9(2) . . ?
O272 Mo1G O19 71.2(2) . . ?
O284 Mo1G O53 170.9(3) . . ?
O139 Mo1G O53 88.3(2) . . ?
O163 Mo1G O53 85.4(2) . . ?
O164 Mo1G O53 83.6(2) . . ?
O272 Mo1G O53 82.7(2) . . ?
O19 Mo1G O53 73.9(2) . . ?
O309 Mo1H O380 104.1(3) . . ?
O309 Mo1H O97 100.7(3) . . ?
O380 Mo1H O97 105.4(3) . . ?
O309 Mo1H O27 96.5(3) . . ?
O380 Mo1H O27 88.8(3) . . ?
O97 Mo1H O27 154.0(2) . . ?
O309 Mo1H O104 94.2(3) . . ?
O380 Mo1H O104 152.8(3) . . ?
O97 Mo1H O104 90.4(2) . . ?
O27 Mo1H O104 69.0(2) . . ?
O309 Mo1H O353 171.3(3) . . ?
O380 Mo1H O353 83.6(3) . . ?
O97 Mo1H O353 80.8(2) . . ?
O27 Mo1H O353 79.4(2) . . ?
O104 Mo1H O353 77.2(2) . . ?
O216 Mo1I O252 102.7(3) . . ?
O216 Mo1I O52 103.4(3) . . ?
O252 Mo1I O52 97.5(3) . . ?
O216 Mo1I O198 104.8(3) . . ?
O252 Mo1I O198 88.1(2) . . ?
O52 Mo1I O198 149.2(2) . . ?
O216 Mo1I O46 97.0(2) . 2_576 ?
O252 Mo1I O46 154.8(2) . 2_576 ?
O52 Mo1I O46 92.9(2) . 2_576 ?
O198 Mo1I O46 71.7(2) . 2_576 ?
O216 Mo1I O116 170.2(3) . . ?
O252 Mo1I O116 86.9(2) . . ?
O52 Mo1I O116 72.6(2) . . ?
O198 Mo1I O116 77.5(2) . . ?
O46 Mo1I O116 74.45(19) 2_576 . ?
O103 Mo1J O40 103.6(3) . . ?
O103 Mo1J O193 103.2(3) . . ?
O40 Mo1J O193 98.2(3) . . ?
O103 Mo1J O169 104.6(3) . . ?
O40 Mo1J O169 148.6(2) . . ?
O193 Mo1J O169 88.7(2) . . ?
O103 Mo1J O77 96.4(2) . . ?
O40 Mo1J O77 91.6(2) . . ?
O193 Mo1J O77 155.3(2) . . ?
O169 Mo1J O77 71.8(2) . . ?
O103 Mo1J O238 169.7(3) . . ?
O40 Mo1J O238 72.4(2) . . ?
O193 Mo1J O238 86.9(2) . . ?
O169 Mo1J O238 77.5(2) . . ?
O77 Mo1J O238 74.47(19) . . ?
O51 Mo1K O135 103.8(3) . . ?
O51 Mo1K O59 105.7(3) . . ?
O135 Mo1K O59 98.5(2) . . ?
O51 Mo1K O47 105.4(3) . . ?
O135 Mo1K O47 97.7(2) . . ?
O59 Mo1K O47 140.1(2) . . ?
O51 Mo1K O63 97.3(2) . . ?
O135 Mo1K O63 158.8(2) . . ?
O59 Mo1K O63 76.3(2) . . ?
O47 Mo1K O63 75.5(2) . . ?
O51 Mo1K O82 177.4(2) . . ?
O135 Mo1K O82 73.6(2) . . ?
O59 Mo1K O82 75.51(19) . . ?
O47 Mo1K O82 74.52(19) . . ?
O63 Mo1K O82 85.19(19) . . ?
O151 Mo1L O250 100.0(3) . . ?
O151 Mo1L O108 101.2(3) . . ?
O250 Mo1L O108 72.0(2) . . ?
O151 Mo1L O169 94.9(2) . . ?
O250 Mo1L O169 71.4(2) . . ?
O108 Mo1L O169 142.0(2) . . ?
O151 Mo1L O206 94.5(2) . . ?
O250 Mo1L O206 142.4(2) . . ?
O108 Mo1L O206 71.1(2) . . ?
O169 Mo1L O206 141.8(2) . . ?
O151 Mo1L O77 97.8(2) . . ?
O250 Mo1L O77 139.4(2) . . ?
O108 Mo1L O77 138.7(2) . . ?
O169 Mo1L O77 70.9(2) . . ?
O206 Mo1L O77 71.1(2) . . ?
O151 Mo1L O203 171.8(3) . . ?
O250 Mo1L O203 86.6(2) . . ?
O108 Mo1L O203 85.3(2) . . ?
O169 Mo1L O203 82.5(2) . . ?
O206 Mo1L O203 83.0(2) . . ?
O77 Mo1L O203 74.0(2) . . ?
O129 Mo1M O303 104.4(4) . . ?
O129 Mo1M O221 100.3(3) . . ?
O303 Mo1M O221 105.0(3) . . ?
O129 Mo1M O89 95.2(3) . . ?
O303 Mo1M O89 90.2(3) . . ?
O221 Mo1M O89 154.6(2) . . ?
O129 Mo1M O172 95.1(3) . . ?
O303 Mo1M O172 152.4(3) . . ?
O221 Mo1M O172 90.2(2) . . ?
O89 Mo1M O172 68.3(2) . . ?
O129 Mo1M O354 171.8(3) . . ?
O303 Mo1M O354 82.6(3) . . ?
O221 Mo1M O354 81.7(2) . . ?
O89 Mo1M O354 80.2(2) . . ?
O172 Mo1M O354 76.9(2) . . ?
O209 Mo1N O341 99.5(3) . . ?
O209 Mo1N O153 101.6(3) . . ?
O341 Mo1N O153 71.2(2) . . ?
O209 Mo1N O198 95.3(3) . 2_576 ?
O341 Mo1N O198 72.1(2) . 2_576 ?
O153 Mo1N O198 141.6(2) . 2_576 ?
O209 Mo1N O212 92.9(3) . . ?
O341 Mo1N O212 142.8(2) . . ?
O153 Mo1N O212 71.9(2) . . ?
O198 Mo1N O212 141.7(2) 2_576 . ?
O209 Mo1N O46 98.1(2) . . ?
O341 Mo1N O46 140.1(2) . . ?
O153 Mo1N O46 138.6(2) . . ?
O198 Mo1N O46 70.8(2) 2_576 . ?
O212 Mo1N O46 71.0(2) . . ?
O209 Mo1N O179 171.7(3) . 2_576 ?
O341 Mo1N O179 87.8(2) . 2_576 ?
O153 Mo1N O179 84.5(2) . 2_576 ?
O198 Mo1N O179 83.0(2) 2_576 2_576 ?
O212 Mo1N O179 83.5(2) . 2_576 ?
O46 Mo1N O179 73.6(2) . 2_576 ?
O365 Mo1O O245 103.7(3) . . ?
O365 Mo1O O334 100.7(3) . . ?
O245 Mo1O O334 106.2(3) . . ?
O365 Mo1O O108 98.0(3) . . ?
O245 Mo1O O108 88.8(3) . . ?
O334 Mo1O O108 152.3(2) . . ?
O365 Mo1O O206 94.3(3) . . ?
O245 Mo1O O206 152.7(3) . . ?
O334 Mo1O O206 90.1(2) . . ?
O108 Mo1O O206 68.3(2) . . ?
O365 Mo1O O88 173.6(3) . . ?
O245 Mo1O O88 82.7(3) . . ?
O334 Mo1O O88 76.7(2) . . ?
O108 Mo1O O88 82.5(2) . . ?
O206 Mo1O O88 79.97(19) . . ?
O229 Mo1P O273 103.7(3) . . ?
O229 Mo1P O95 100.0(3) . . ?
O273 Mo1P O95 106.3(3) . . ?
O229 Mo1P O311 94.9(3) . . ?
O273 Mo1P O311 89.6(3) . . ?
O95 Mo1P O311 154.8(2) . . ?
O229 Mo1P O167 93.9(2) . . ?
O273 Mo1P O167 153.1(3) . . ?
O95 Mo1P O167 90.2(2) . . ?
O311 Mo1P O167 68.5(2) . . ?
O229 Mo1P O219 171.2(2) . . ?
O273 Mo1P O219 84.2(3) . . ?
O95 Mo1P O219 81.3(2) . . ?
O311 Mo1P O219 81.0(2) . . ?
O167 Mo1P O219 77.4(2) . . ?
O190 Mo1Q O278 103.9(3) . . ?
O190 Mo1Q O114 105.8(3) . . ?
O278 Mo1Q O114 98.1(2) . . ?
O190 Mo1Q O67 104.9(3) . . ?
O278 Mo1Q O67 97.9(2) . . ?
O114 Mo1Q O67 140.5(2) . . ?
O190 Mo1Q O155 97.6(2) . . ?
O278 Mo1Q O155 158.4(2) . . ?
O114 Mo1Q O155 75.8(2) . . ?
O67 Mo1Q O155 76.1(2) . . ?
O190 Mo1Q O24 177.2(2) . . ?
O278 Mo1Q O24 73.4(2) . . ?
O114 Mo1Q O24 75.60(19) . . ?
O67 Mo1Q O24 74.86(19) . . ?
O155 Mo1Q O24 85.04(19) . . ?
O220 Mo1R O192 103.3(4) . . ?
O220 Mo1R O148 99.5(3) . . ?
O192 Mo1R O148 98.3(3) . . ?
O220 Mo1R O200 95.1(3) . . ?
O192 Mo1R O200 94.8(3) . . ?
O148 Mo1R O200 157.5(2) . . ?
O220 Mo1R O351 88.9(4) . . ?
O192 Mo1R O351 167.0(3) . . ?
O148 Mo1R O351 83.7(3) . . ?
O200 Mo1R O351 79.5(3) . . ?
O220 Mo1R O199 162.5(4) . 2_567 ?
O192 Mo1R O199 93.7(3) . 2_567 ?
O148 Mo1R O199 82.1(2) . 2_567 ?
O200 Mo1R O199 78.9(2) . 2_567 ?
O351 Mo1R O199 73.9(3) . 2_567 ?
O374 Mo1S O428 102.0(4) . . ?
O374 Mo1S O447 107.8(4) . . ?
O428 Mo1S O447 99.4(4) . . ?
O374 Mo1S O131 89.2(3) . . ?
O428 Mo1S O131 91.5(3) . . ?
O447 Mo1S O131 157.2(3) . . ?
O374 Mo1S O14 153.3(4) . . ?
O428 Mo1S O14 93.9(3) . . ?
O447 Mo1S O14 90.3(3) . . ?
O131 Mo1S O14 68.8(2) . . ?
O374 Mo1S O422 84.6(4) . . ?
O428 Mo1S O422 170.7(4) . . ?
O447 Mo1S O422 84.6(4) . . ?
O131 Mo1S O422 81.9(3) . . ?
O14 Mo1S O422 77.7(3) . . ?
O403 Mo1T O261 103.4(3) . 2_576 ?
O403 Mo1T O248 98.9(3) . 2_576 ?
O261 Mo1T O248 89.3(2) 2_576 2_576 ?
O403 Mo1T O305 102.4(3) . . ?
O261 Mo1T O305 86.7(3) 2_576 . ?
O248 Mo1T O305 158.6(2) 2_576 . ?
O403 Mo1T O259 99.7(3) . . ?
O261 Mo1T O259 156.8(2) 2_576 . ?
O248 Mo1T O259 89.2(2) 2_576 . ?
O305 Mo1T O259 86.4(3) . . ?
O403 Mo1T O235 167.3(3) . . ?
O261 Mo1T O235 87.7(2) 2_576 . ?
O248 Mo1T O235 74.5(2) 2_576 . ?
O305 Mo1T O235 84.3(2) . . ?
O259 Mo1T O235 69.7(2) . . ?
O286 Mo1U O213 103.0(3) . . ?
O286 Mo1U O333 101.1(3) . . ?
O213 Mo1U O333 106.2(3) . . ?
O286 Mo1U O153 98.7(3) . . ?
O213 Mo1U O153 88.6(3) . . ?
O333 Mo1U O153 151.8(2) . . ?
O286 Mo1U O212 94.7(3) . . ?
O213 Mo1U O212 153.1(3) . . ?
O333 Mo1U O212 89.7(2) . . ?
O153 Mo1U O212 68.6(2) . . ?
O286 Mo1U O312 173.7(3) . . ?
O213 Mo1U O312 83.2(3) . . ?
O333 Mo1U O312 77.0(2) . . ?
O153 Mo1U O312 81.2(2) . . ?
O212 Mo1U O312 79.4(2) . . ?
O218 Mo1V O261 103.2(3) . . ?
O218 Mo1V O325 103.0(3) . . ?
O261 Mo1V O325 98.0(3) . . ?
O218 Mo1V O362 104.1(3) . . ?
O261 Mo1V O362 88.1(2) . . ?
O325 Mo1V O362 150.0(2) . . ?
O218 Mo1V O22 95.6(3) . . ?
O261 Mo1V O22 155.2(2) . . ?
O325 Mo1V O22 93.2(2) . . ?
O362 Mo1V O22 71.6(2) . . ?
O218 Mo1V O178 168.5(3) . . ?
O261 Mo1V O178 88.1(2) . . ?
O325 Mo1V O178 73.1(2) . . ?
O362 Mo1V O178 77.8(2) . . ?
O22 Mo1V O178 74.0(2) . . ?
O201 Mo1W O253 103.5(3) . . ?
O201 Mo1W O304 103.4(3) . . ?
O253 Mo1W O304 98.3(3) . . ?
O201 Mo1W O239 104.1(3) . . ?
O253 Mo1W O239 87.8(3) . . ?
O304 Mo1W O239 149.5(3) . . ?
O201 Mo1W O22 96.2(3) . . ?
O253 Mo1W O22 155.0(2) . . ?
O304 Mo1W O22 91.8(3) . . ?
O239 Mo1W O22 72.4(2) . . ?
O201 Mo1W O85 169.4(3) . . ?
O253 Mo1W O85 86.9(2) . . ?
O304 Mo1W O85 72.7(2) . . ?
O239 Mo1W O85 77.8(2) . . ?
O22 Mo1W O85 74.3(2) . . ?
O287 Mo1X O355 104.0(3) . . ?
O287 Mo1X O251 99.1(3) . . ?
O355 Mo1X O251 88.9(3) . . ?
O287 Mo1X O211 101.5(3) . . ?
O355 Mo1X O211 86.9(3) . . ?
O251 Mo1X O211 159.4(2) . . ?
O287 Mo1X O83 99.9(3) . . ?
O355 Mo1X O83 156.1(2) . . ?
O251 Mo1X O83 89.0(2) . . ?
O211 Mo1X O83 86.7(2) . . ?
O287 Mo1X O217 167.4(3) . . ?
O355 Mo1X O217 86.7(2) . . ?
O251 Mo1X O217 74.1(2) . . ?
O211 Mo1X O217 85.5(2) . . ?
O83 Mo1X O217 69.8(2) . . ?
O331 Mo1Y O328 104.7(4) . . ?
O331 Mo1Y O204 101.3(3) . . ?
O328 Mo1Y O204 105.4(3) . . ?
O331 Mo1Y O357 95.3(3) . . ?
O328 Mo1Y O357 89.4(3) . . ?
O204 Mo1Y O357 153.9(3) . . ?
O331 Mo1Y O315 94.7(3) . . ?
O328 Mo1Y O315 151.9(3) . . ?
O204 Mo1Y O315 90.1(2) . . ?
O357 Mo1Y O315 68.4(2) . . ?
O331 Mo1Y O394 171.0(3) . . ?
O328 Mo1Y O394 83.6(3) . . ?
O204 Mo1Y O394 79.3(3) . . ?
O357 Mo1Y O394 81.2(3) . . ?
O315 Mo1Y O394 76.3(3) . . ?
O226 Mo1Z O142 103.4(3) . . ?
O226 Mo1Z O141 99.1(3) . . ?
O142 Mo1Z O141 90.2(2) . . ?
O226 Mo1Z O323 102.6(3) . . ?
O142 Mo1Z O323 86.7(2) . . ?
O141 Mo1Z O323 158.2(2) . . ?
O226 Mo1Z O227 99.1(3) . . ?
O142 Mo1Z O227 157.4(2) . . ?
O141 Mo1Z O227 87.9(2) . . ?
O323 Mo1Z O227 86.8(3) . . ?
O226 Mo1Z O107 167.0(3) . . ?
O142 Mo1Z O107 88.1(2) . . ?
O141 Mo1Z O107 74.4(2) . . ?
O323 Mo1Z O107 83.9(2) . . ?
O227 Mo1Z O107 69.7(2) . . ?
O267 Mo2A O363 103.8(3) . . ?
O267 Mo2A O251 102.6(3) . . ?
O363 Mo2A O251 98.1(3) . . ?
O267 Mo2A O223 104.4(3) . . ?
O363 Mo2A O223 88.2(3) . . ?
O251 Mo2A O223 149.9(2) . . ?
O267 Mo2A O160 95.7(3) . . ?
O363 Mo2A O160 155.0(2) . . ?
O251 Mo2A O160 92.6(2) . . ?
O223 Mo2A O160 71.7(2) . . ?
O267 Mo2A O217 168.7(3) . . ?
O363 Mo2A O217 87.2(2) . . ?
O251 Mo2A O217 73.1(2) . . ?
O223 Mo2A O217 77.9(2) . . ?
O160 Mo2A O217 74.3(2) . . ?
O257 Mo2B O347 104.2(3) . . ?
O257 Mo2B O40 99.8(3) . . ?
O347 Mo2B O40 89.5(2) . . ?
O257 Mo2B O204 101.3(3) . . ?
O347 Mo2B O204 86.8(2) . . ?
O40 Mo2B O204 158.8(2) . . ?
O257 Mo2B O227 99.9(3) . . ?
O347 Mo2B O227 155.7(2) . . ?
O40 Mo2B O227 88.8(2) . . ?
O204 Mo2B O227 86.0(2) . . ?
O257 Mo2B O238 167.7(2) . . ?
O347 Mo2B O238 86.6(2) . . ?
O40 Mo2B O238 73.9(2) . . ?
O204 Mo2B O238 85.0(2) . . ?
O227 Mo2B O238 69.7(2) . . ?
O271 Mo2C O249 103.6(3) . . ?
O271 Mo2C O224 105.2(3) . . ?
O249 Mo2C O224 98.5(3) . . ?
O271 Mo2C O217 105.8(3) . . ?
O249 Mo2C O217 98.3(2) . . ?
O224 Mo2C O217 139.9(2) . . ?
O271 Mo2C O83 98.2(3) . . ?
O249 Mo2C O83 158.2(2) . . ?
O224 Mo2C O83 75.8(2) . . ?
O217 Mo2C O83 75.1(2) . . ?
O271 Mo2C O160 177.2(3) . . ?
O249 Mo2C O160 73.6(2) . . ?
O224 Mo2C O160 75.2(2) . . ?
O217 Mo2C O160 75.1(2) . . ?
O83 Mo2C O160 84.6(2) . . ?
O348 Mo2D O357 99.6(3) . . ?
O348 Mo2D O338 100.7(3) . . ?
O357 Mo2D O338 71.4(3) . . ?
O348 Mo2D O223 94.0(3) . . ?
O357 Mo2D O223 142.1(2) . . ?
O338 Mo2D O223 71.3(3) . . ?
O348 Mo2D O315 94.9(3) . . ?
O357 Mo2D O315 71.9(2) . . ?
O338 Mo2D O315 142.0(3) . . ?
O223 Mo2D O315 142.1(2) . . ?
O348 Mo2D O160 97.5(3) . . ?
O357 Mo2D O160 140.3(2) . . ?
O338 Mo2D O160 139.1(3) . . ?
O223 Mo2D O160 71.2(2) . . ?
O315 Mo2D O160 71.1(2) . . ?
O348 Mo2D O249 171.4(3) . . ?
O357 Mo2D O249 87.6(2) . . ?
O338 Mo2D O249 85.9(3) . . ?
O223 Mo2D O249 83.0(2) . . ?
O315 Mo2D O249 82.8(2) . . ?
O160 Mo2D O249 73.9(2) . . ?
O111 Mo2E O280 99.1(3) . . ?
O111 Mo2E O330 101.1(3) . . ?
O280 Mo2E O330 70.9(3) . . ?
O111 Mo2E O302 94.1(3) . . ?
O280 Mo2E O302 71.4(2) . . ?
O330 Mo2E O302 141.1(3) . . ?
O111 Mo2E O275 94.3(3) . . ?
O280 Mo2E O275 142.5(2) . . ?
O330 Mo2E O275 72.2(2) . . ?
O302 Mo2E O275 142.4(2) . . ?
O111 Mo2E O256 97.3(3) . . ?
O280 Mo2E O256 140.1(2) . . ?
O330 Mo2E O256 140.0(3) . . ?
O302 Mo2E O256 71.4(2) . . ?
O275 Mo2E O256 71.2(2) . . ?
O111 Mo2E O361 171.3(3) . . ?
O280 Mo2E O361 87.9(3) . . ?
O330 Mo2E O361 86.0(2) . . ?
O302 Mo2E O361 83.3(2) . . ?
O275 Mo2E O361 82.9(2) . . ?
O256 Mo2E O361 74.0(2) . . ?
O337 Mo2F O186 103.7(3) . . ?
O337 Mo2F O120 102.7(3) . . ?
O186 Mo2F O120 98.6(3) . . ?
O337 Mo2F O324 104.7(3) . . ?
O186 Mo2F O324 87.9(3) . . ?
O120 Mo2F O324 149.4(3) . . ?
O337 Mo2F O137 96.1(3) . . ?
O186 Mo2F O137 154.9(3) . . ?
O120 Mo2F O137 91.9(2) . . ?
O324 Mo2F O137 72.0(2) . . ?
O337 Mo2F O146 169.1(3) . . ?
O186 Mo2F O146 87.0(2) . . ?
O120 Mo2F O146 73.0(2) . . ?
O324 Mo2F O146 77.6(2) . . ?
O137 Mo2F O146 74.3(2) . . ?
O296 Mo2G O355 103.0(3) . . ?
O296 Mo2G O322 103.0(3) . . ?
O355 Mo2G O322 98.7(3) . . ?
O296 Mo2G O275 104.6(3) . . ?
O355 Mo2G O275 87.6(2) . . ?
O322 Mo2G O275 149.5(2) . . ?
O296 Mo2G O256 96.1(3) . . ?
O355 Mo2G O256 155.1(2) . . ?
O322 Mo2G O256 92.3(2) . . ?
O275 Mo2G O256 72.1(2) . . ?
O296 Mo2G O279 169.4(3) . . ?
O355 Mo2G O279 87.5(2) . . ?
O322 Mo2G O279 73.0(2) . . ?
O275 Mo2G O279 77.4(2) . . ?
O256 Mo2G O279 74.4(2) . . ?
O285 Mo2H O142 103.0(3) . . ?
O285 Mo2H O105 103.5(3) . . ?
O142 Mo2H O105 97.9(2) . . ?
O285 Mo2H O268 104.2(3) . . ?
O142 Mo2H O268 88.2(2) . . ?
O105 Mo2H O268 149.5(3) . . ?
O285 Mo2H O137 95.3(3) . . ?
O142 Mo2H O137 155.6(3) . . ?
O105 Mo2H O137 93.1(2) . . ?
O268 Mo2H O137 71.7(2) . . ?
O285 Mo2H O191 168.6(2) . . ?
O142 Mo2H O191 88.1(2) . . ?
O105 Mo2H O191 72.4(2) . . ?
O268 Mo2H O191 78.0(2) . . ?
O137 Mo2H O191 74.6(2) . . ?
O350 Mo2I O203 103.7(3) . . ?
O350 Mo2I O107 105.4(3) . . ?
O203 Mo2I O107 98.8(2) . . ?
O350 Mo2I O238 105.4(3) . . ?
O203 Mo2I O238 97.7(3) . . ?
O107 Mo2I O238 140.2(2) . . ?
O350 Mo2I O227 98.8(3) . . ?
O203 Mo2I O227 157.5(2) . . ?
O107 Mo2I O227 75.2(2) . . ?
O238 Mo2I O227 75.7(2) . . ?
O350 Mo2I O77 177.0(3) . . ?
O203 Mo2I O77 73.4(2) . . ?
O107 Mo2I O77 75.0(2) . . ?
O238 Mo2I O77 75.6(2) . . ?
O227 Mo2I O77 84.1(2) . . ?
O185 Mo2J O200 107.4(2) . . ?
O185 Mo2J O214 93.6(3) . . ?
O200 Mo2J O214 92.7(3) . . ?
O185 Mo2J O33 91.8(2) . . ?
O200 Mo2J O33 160.8(2) . . ?
O214 Mo2J O33 87.3(3) . . ?
O185 Mo2J O119 161.7(2) . . ?
O200 Mo2J O119 90.7(2) . . ?
O214 Mo2J O119 87.5(3) . . ?
O33 Mo2J O119 70.05(19) . . ?
O185 Mo2J O72 94.82(18) . . ?
O200 Mo2J O72 94.7(2) . . ?
O214 Mo2J O72 166.5(2) . . ?
O33 Mo2J O72 81.98(15) . . ?
O119 Mo2J O72 81.20(15) . . ?
O349 Mo2K O179 104.4(3) . . ?
O349 Mo2K O116 106.7(3) . . ?
O179 Mo2K O116 97.7(3) . . ?
O349 Mo2K O235 104.9(3) . . ?
O179 Mo2K O235 97.6(3) . . ?
O116 Mo2K O235 139.9(2) . . ?
O349 Mo2K O259 98.5(3) . . ?
O179 Mo2K O259 157.1(2) . . ?
O116 Mo2K O259 76.1(2) . . ?
O235 Mo2K O259 75.5(2) . . ?
O349 Mo2K O46 176.6(2) . 2_576 ?
O179 Mo2K O46 72.5(2) . 2_576 ?
O116 Mo2K O46 75.3(2) . 2_576 ?
O235 Mo2K O46 74.4(2) . 2_576 ?
O259 Mo2K O46 84.6(2) . 2_576 ?
O390 Mo2L O453 103.0(5) . . ?
O390 Mo2L O297 100.1(3) . . ?
O453 Mo2L O297 105.3(3) . . ?
O390 Mo2L O236 96.5(3) . . ?
O453 Mo2L O236 90.8(3) . . ?
O297 Mo2L O236 153.5(3) . . ?
O390 Mo2L O181 93.9(3) . . ?
O453 Mo2L O181 154.8(3) . . ?
O297 Mo2L O181 89.7(2) . . ?
O236 Mo2L O181 68.6(2) . . ?
O390 Mo2L O381 171.5(3) . . ?
O453 Mo2L O381 85.2(4) . . ?
O297 Mo2L O381 79.9(3) . . ?
O236 Mo2L O381 80.6(3) . . ?
O181 Mo2L O381 77.5(3) . . ?
O281 Mo2M O347 103.2(3) . . ?
O281 Mo2M O171 102.5(3) . . ?
O347 Mo2M O171 98.4(3) . . ?
O281 Mo2M O315 104.8(3) . . ?
O347 Mo2M O315 87.6(2) . . ?
O171 Mo2M O315 149.8(3) . . ?
O281 Mo2M O160 95.6(3) . . ?
O347 Mo2M O160 155.1(2) . . ?
O171 Mo2M O160 93.1(3) . . ?
O315 Mo2M O160 71.8(2) . . ?
O281 Mo2M O224 168.8(3) . . ?
O347 Mo2M O224 87.7(2) . . ?
O171 Mo2M O224 73.0(2) . . ?
O315 Mo2M O224 77.8(2) . . ?
O160 Mo2M O224 74.6(2) . . ?
O295 Mo2N O378 102.7(4) . . ?
O295 Mo2N O230 100.7(3) . . ?
O378 Mo2N O230 105.8(3) . . ?
O295 Mo2N O250 96.1(3) . . ?
O378 Mo2N O250 89.1(3) . . ?
O230 Mo2N O250 154.3(2) . . ?
O295 Mo2N O169 94.2(3) . . ?
O378 Mo2N O169 152.9(3) . . ?
O230 Mo2N O169 91.5(2) . . ?
O250 Mo2N O169 67.9(2) . . ?
O295 Mo2N O332 172.5(3) . . ?
O378 Mo2N O332 84.3(4) . . ?
O230 Mo2N O332 79.6(3) . . ?
O250 Mo2N O332 81.2(2) . . ?
O169 Mo2N O332 78.4(3) . . ?
O352 Mo2O O366 100.3(3) . . ?
O352 Mo2O O147 100.0(3) . . ?
O366 Mo2O O147 71.4(3) . . ?
O352 Mo2O O112 94.3(3) . . ?
O366 Mo2O O112 142.7(3) . . ?
O147 Mo2O O112 72.3(3) . . ?
O352 Mo2O O62 93.7(3) . . ?
O366 Mo2O O62 72.0(3) . . ?
O147 Mo2O O62 142.6(3) . . ?
O112 Mo2O O62 141.3(3) . . ?
O352 Mo2O O263 96.9(3) . . ?
O366 Mo2O O263 139.8(2) . . ?
O147 Mo2O O263 140.2(2) . . ?
O112 Mo2O O263 70.7(2) . . ?
O62 Mo2O O263 70.8(2) . . ?
O352 Mo2O O93 170.7(3) . . ?
O366 Mo2O O93 87.2(3) . . ?
O147 Mo2O O93 87.6(3) . . ?
O112 Mo2O O93 82.8(2) . . ?
O62 Mo2O O93 83.3(2) . . ?
O263 Mo2O O93 73.8(2) . . ?
O264 Mo2P O414 104.1(4) . . ?
O264 Mo2P O195 100.3(3) . . ?
O414 Mo2P O195 105.9(3) . . ?
O264 Mo2P O147 95.6(3) . . ?
O414 Mo2P O147 89.5(3) . . ?
O195 Mo2P O147 154.2(3) . . ?
O264 Mo2P O112 93.6(3) . . ?
O414 Mo2P O112 153.2(3) . . ?
O195 Mo2P O112 90.2(3) . . ?
O147 Mo2P O112 68.6(2) . . ?
O264 Mo2P O329 170.6(3) . . ?
O414 Mo2P O329 84.8(4) . . ?
O195 Mo2P O329 80.0(3) . . ?
O147 Mo2P O329 81.1(3) . . ?
O112 Mo2P O329 77.0(3) . . ?
O283 Mo2Q O222 103.9(3) . . ?
O283 Mo2Q O85 105.5(3) . . ?
O222 Mo2Q O85 98.6(3) . . ?
O283 Mo2Q O178 105.4(3) . . ?
O222 Mo2Q O178 97.4(2) . . ?
O85 Mo2Q O178 140.4(2) . . ?
O283 Mo2Q O138 97.7(3) . . ?
O222 Mo2Q O138 158.4(3) . . ?
O85 Mo2Q O138 76.4(2) . . ?
O178 Mo2Q O138 75.5(2) . . ?
O283 Mo2Q O22 177.1(3) . . ?
O222 Mo2Q O22 73.2(2) . . ?
O85 Mo2Q O22 75.7(2) . . ?
O178 Mo2Q O22 74.7(2) . . ?
O138 Mo2Q O22 85.2(2) . . ?
O400 Mo2R O307 101.9(4) . . ?
O400 Mo2R O274 101.8(4) . . ?
O307 Mo2R O274 105.4(3) . . ?
O400 Mo2R O250 95.4(3) . . ?
O307 Mo2R O250 154.0(3) . . ?
O274 Mo2R O250 89.7(3) . . ?
O400 Mo2R O108 96.6(3) . . ?
O307 Mo2R O108 89.6(3) . . ?
O274 Mo2R O108 153.1(3) . . ?
O250 Mo2R O108 69.0(2) . . ?
O400 Mo2R O368 175.6(3) . . ?
O307 Mo2R O368 81.2(3) . . ?
O274 Mo2R O368 80.3(3) . . ?
O250 Mo2R O368 80.6(2) . . ?
O108 Mo2R O368 80.1(2) . . ?
O379 Mo2S O409 100.5(4) . . ?
O379 Mo2S O288 100.3(4) . . ?
O409 Mo2S O288 106.3(3) . . ?
O379 Mo2S O139 95.5(3) . . ?
O409 Mo2S O139 154.7(3) . . ?
O288 Mo2S O139 89.7(3) . . ?
O379 Mo2S O163 95.8(4) . . ?
O409 Mo2S O163 90.1(3) . . ?
O288 Mo2S O163 154.3(3) . . ?
O139 Mo2S O163 68.8(2) . . ?
O379 Mo2S O292 174.5(4) . . ?
O409 Mo2S O292 82.3(4) . . ?
O288 Mo2S O292 83.3(4) . . ?
O139 Mo2S O292 80.3(3) . . ?
O163 Mo2S O292 79.4(3) . . ?
O165 Mo2T O363 104.2(3) . . ?
O165 Mo2T O322 99.3(3) . . ?
O363 Mo2T O322 88.9(3) . . ?
O165 Mo2T O359 102.2(3) . . ?
O363 Mo2T O359 87.0(3) . . ?
O322 Mo2T O359 158.5(3) . . ?
O165 Mo2T O184 99.9(3) . . ?
O363 Mo2T O184 155.8(2) . . ?
O322 Mo2T O184 88.7(3) . . ?
O359 Mo2T O184 86.4(3) . . ?
O165 Mo2T O279 167.7(3) . . ?
O363 Mo2T O279 86.4(2) . . ?
O322 Mo2T O279 74.3(2) . . ?
O359 Mo2T O279 84.4(2) . . ?
O184 Mo2T O279 69.8(2) . . ?
O306 Mo2U O253 103.9(3) . . ?
O306 Mo2U O232 99.7(3) . . ?
O253 Mo2U O232 89.0(3) . . ?
O306 Mo2U O339 102.1(3) . . ?
O253 Mo2U O339 87.0(3) . . ?
O232 Mo2U O339 158.2(3) . . ?
O306 Mo2U O177 99.8(3) . . ?
O253 Mo2U O177 156.2(3) . . ?
O232 Mo2U O177 88.8(2) . . ?
O339 Mo2U O177 86.3(3) . . ?
O306 Mo2U O225 167.4(3) . . ?
O253 Mo2U O225 87.1(2) . . ?
O232 Mo2U O225 73.9(3) . . ?
O339 Mo2U O225 84.5(3) . . ?
O177 Mo2U O225 69.6(2) . . ?
O320 Mo2V O291 103.5(3) . . ?
O320 Mo2V O207 102.9(3) . . ?
O291 Mo2V O207 98.6(3) . . ?
O320 Mo2V O112 105.0(3) . . ?
O291 Mo2V O112 87.8(3) . . ?
O207 Mo2V O112 149.1(3) . . ?
O320 Mo2V O263 96.0(3) . . ?
O291 Mo2V O263 154.9(3) . . ?
O207 Mo2V O263 92.1(3) . . ?
O112 Mo2V O263 71.9(2) . . ?
O320 Mo2V O266 168.7(3) . . ?
O291 Mo2V O266 87.6(2) . . ?
O207 Mo2V O266 72.5(3) . . ?
O112 Mo2V O266 77.6(2) . . ?
O263 Mo2V O266 74.1(2) . . ?
O265 Mo2W O361 103.6(3) . . ?
O265 Mo2W O279 105.1(3) . . ?
O361 Mo2W O279 98.4(3) . . ?
O265 Mo2W O101 105.2(3) . . ?
O361 Mo2W O101 97.9(3) . . ?
O279 Mo2W O101 140.9(2) . . ?
O265 Mo2W O184 98.5(3) . . ?
O361 Mo2W O184 157.9(3) . . ?
O279 Mo2W O184 76.1(2) . . ?
O101 Mo2W O184 75.5(2) . . ?
O265 Mo2W O256 177.0(3) . . ?
O361 Mo2W O256 73.4(2) . . ?
O279 Mo2W O256 75.6(2) . . ?
O101 Mo2W O256 75.5(2) . . ?
O184 Mo2W O256 84.5(2) . . ?
O387 Mo2X O459 108.6(3) . . ?
O387 Mo2X O373 97.0(5) . . ?
O459 Mo2X O373 96.1(4) . . ?
O387 Mo2X O89 91.1(3) . . ?
O459 Mo2X O89 157.8(3) . . ?
O373 Mo2X O89 91.2(3) . . ?
O387 Mo2X O311 158.8(3) . . ?
O459 Mo2X O311 90.0(3) . . ?
O373 Mo2X O311 90.7(4) . . ?
O89 Mo2X O311 68.9(2) . . ?
O387 Mo2X O434 86.9(4) . . ?
O459 Mo2X O434 86.7(4) . . ?
O373 Mo2X O434 174.2(4) . . ?
O89 Mo2X O434 84.4(3) . . ?
O311 Mo2X O434 84.2(3) . . ?
O300 Mo2Y O399 103.1(4) . . ?
O300 Mo2Y O180 100.5(3) . . ?
O399 Mo2Y O180 106.0(3) . . ?
O300 Mo2Y O341 95.3(3) . 2_576 ?
O399 Mo2Y O341 89.2(3) . 2_576 ?
O180 Mo2Y O341 154.7(2) . 2_576 ?
O300 Mo2Y O198 94.1(3) . . ?
O399 Mo2Y O198 153.2(3) . . ?
O180 Mo2Y O198 90.7(2) . . ?
O341 Mo2Y O198 68.5(2) 2_576 . ?
O300 Mo2Y O344 171.5(3) . . ?
O399 Mo2Y O344 84.7(4) . . ?
O180 Mo2Y O344 80.4(3) . . ?
O341 Mo2Y O344 81.1(3) 2_576 . ?
O198 Mo2Y O344 77.4(3) . . ?
O233 Mo2Z O314 104.1(3) . . ?
O233 Mo2Z O146 105.5(3) . . ?
O314 Mo2Z O146 98.4(3) . . ?
O233 Mo2Z O191 105.5(3) . . ?
O314 Mo2Z O191 97.4(2) . . ?
O146 Mo2Z O191 140.3(3) . . ?
O233 Mo2Z O289 98.0(3) . . ?
O314 Mo2Z O289 157.9(3) . . ?
O146 Mo2Z O289 76.2(2) . . ?
O191 Mo2Z O289 75.6(2) . . ?
O233 Mo2Z O137 177.3(3) . . ?
O314 Mo2Z O137 73.1(3) . . ?
O146 Mo2Z O137 75.4(2) . . ?
O191 Mo2Z O137 74.8(2) . . ?
O289 Mo2Z O137 84.7(2) . . ?
O310 Mo3A O415 103.7(4) . . ?
O310 Mo3A O359 101.1(3) . . ?
O415 Mo3A O359 105.9(3) . . ?
O310 Mo3A O338 95.8(3) . . ?
O415 Mo3A O338 89.0(3) . . ?
O359 Mo3A O338 153.9(3) . . ?
O310 Mo3A O223 95.2(3) . . ?
O415 Mo3A O223 151.9(3) . . ?
O359 Mo3A O223 90.3(2) . . ?
O338 Mo3A O223 68.3(2) . . ?
O310 Mo3A O427 172.2(3) . . ?
O415 Mo3A O427 83.5(4) . . ?
O359 Mo3A O427 79.6(3) . . ?
O338 Mo3A O427 81.1(3) . . ?
O223 Mo3A O427 77.0(3) . . ?
O388 Mo3B O455 103.5(4) . . ?
O388 Mo3B O305 99.7(3) . . ?
O455 Mo3B O305 106.2(3) . . ?
O388 Mo3B O244 96.9(3) . 2_576 ?
O455 Mo3B O244 89.3(3) . 2_576 ?
O305 Mo3B O244 153.8(3) . 2_576 ?
O388 Mo3B O362 93.3(3) . 2_576 ?
O455 Mo3B O362 153.2(3) . 2_576 ?
O305 Mo3B O362 91.0(3) . 2_576 ?
O244 Mo3B O362 67.8(2) 2_576 2_576 ?
O388 Mo3B O408 171.8(4) . . ?
O455 Mo3B O408 84.5(4) . . ?
O305 Mo3B O408 79.2(3) . . ?
O244 Mo3B O408 81.5(3) 2_576 . ?
O362 Mo3B O408 78.6(3) 2_576 . ?
O326 Mo3C O425 97.0(4) . . ?
O326 Mo3C O725 119.9(8) . . ?
O326 Mo3C O323 100.0(3) . . ?
O425 Mo3C O323 107.8(4) . . ?
O725 Mo3C O323 103.0(7) . . ?
O326 Mo3C O393 95.6(3) . . ?
O425 Mo3C O393 89.0(4) . . ?
O725 Mo3C O393 85.3(7) . . ?
O323 Mo3C O393 155.3(3) . . ?
O326 Mo3C O268 94.9(3) . . ?
O425 Mo3C O268 155.8(4) . . ?
O725 Mo3C O268 138.7(8) . . ?
O323 Mo3C O268 90.7(2) . . ?
O393 Mo3C O268 68.8(2) . . ?
O326 Mo3C O440 171.9(3) . . ?
O425 Mo3C O440 90.3(4) . . ?
O725 Mo3C O440 67.3(8) . . ?
O323 Mo3C O440 81.1(3) . . ?
O393 Mo3C O440 80.9(3) . . ?
O268 Mo3C O440 77.0(3) . . ?
O488 Mo3D O396 102.9(5) . . ?
O488 Mo3D O489 98.5(5) . . ?
O396 Mo3D O489 105.8(4) . . ?
O488 Mo3D O357 95.5(4) . . ?
O396 Mo3D O357 90.3(3) . . ?
O489 Mo3D O357 155.6(3) . . ?
O488 Mo3D O338 95.2(4) . . ?
O396 Mo3D O338 154.0(4) . . ?
O489 Mo3D O338 89.5(3) . . ?
O357 Mo3D O338 69.3(3) . . ?
O488 Mo3D O465 173.9(4) . . ?
O396 Mo3D O465 82.2(5) . . ?
O489 Mo3D O465 83.1(4) . . ?
O357 Mo3D O465 81.1(3) . . ?
O338 Mo3D O465 78.9(3) . . ?
O512 Mo3E O813 83.7(8) . . ?
O512 Mo3E O513 107.6(6) . . ?
O512 Mo3E O467 98.3(5) . 2_667 ?
O513 Mo3E O467 106.4(5) . 2_667 ?
O512 Mo3E O236 93.8(4) . . ?
O813 Mo3E O236 93.2(7) . . ?
O513 Mo3E O236 89.7(4) . . ?
O467 Mo3E O236 155.7(3) 2_667 . ?
O512 Mo3E O231 92.1(4) . . ?
O813 Mo3E O231 161.7(7) . . ?
O513 Mo3E O231 152.3(5) . . ?
O467 Mo3E O231 89.3(3) 2_667 . ?
O236 Mo3E O231 69.2(2) . . ?
O512 Mo3E O511 173.1(5) . . ?
O813 Mo3E O511 101.7(8) . . ?
O513 Mo3E O511 77.8(5) . . ?
O467 Mo3E O511 83.9(4) 2_667 . ?
O236 Mo3E O511 81.8(4) . . ?
O231 Mo3E O511 81.4(4) . . ?
O255 Mo3F O468 104.0(4) . . ?
O255 Mo3F O339 99.2(3) . . ?
O468 Mo3F O339 106.3(3) . . ?
O255 Mo3F O384 96.5(3) . . ?
O468 Mo3F O384 88.8(3) . . ?
O339 Mo3F O384 154.8(3) . . ?
O255 Mo3F O239 94.9(3) . . ?
O468 Mo3F O239 152.2(3) . . ?
O339 Mo3F O239 90.3(3) . . ?
O384 Mo3F O239 68.7(2) . . ?
O255 Mo3F O371 172.3(3) . . ?
O468 Mo3F O371 83.4(4) . . ?
O339 Mo3F O371 80.7(3) . . ?
O384 Mo3F O371 81.1(3) . . ?
O239 Mo3F O371 77.4(3) . . ?
O401 Mo3G O391 104.8(4) . . ?
O401 Mo3G O419 99.1(4) . . ?
O391 Mo3G O419 99.5(3) . . ?
O401 Mo3G O307 95.7(3) . . ?
O391 Mo3G O307 93.3(3) . . ?
O419 Mo3G O307 157.2(4) . . ?
O401 Mo3G O245 92.0(3) . . ?
O391 Mo3G O245 162.6(4) . . ?
O419 Mo3G O245 82.0(3) . . ?
O307 Mo3G O245 80.2(3) . . ?
O401 Mo3G O429 167.8(4) . . ?
O391 Mo3G O429 86.5(4) . . ?
O419 Mo3G O429 83.3(4) . . ?
O307 Mo3G O429 78.7(4) . . ?
O245 Mo3G O429 76.4(3) . . ?
O445 Mo3H O449 99.5(5) . . ?
O445 Mo3H O456 94.0(5) . . ?
O449 Mo3H O456 106.9(5) . . ?
O445 Mo3H O756 113.0(8) . . ?
O449 Mo3H O756 104.7(7) . . ?
O445 Mo3H O330 95.7(4) . . ?
O449 Mo3H O330 155.1(4) . . ?
O456 Mo3H O330 91.5(4) . . ?
O756 Mo3H O330 87.2(6) . . ?
O445 Mo3H O280 95.1(4) . . ?
O449 Mo3H O280 90.3(4) . . ?
O456 Mo3H O280 158.9(4) . . ?
O756 Mo3H O280 144.9(7) . . ?
O330 Mo3H O280 68.6(2) . . ?
O445 Mo3H O498 174.9(5) . . ?
O449 Mo3H O498 83.8(5) . . ?
O456 Mo3H O498 88.8(5) . . ?
O756 Mo3H O498 69.7(7) . . ?
O330 Mo3H O498 79.9(4) . . ?
O280 Mo3H O498 80.9(4) . . ?
O402 Mo3I O418 104.4(5) . . ?
O402 Mo3I O270 99.4(4) . . ?
O418 Mo3I O270 99.1(4) . . ?
O402 Mo3I O364 95.1(4) . . ?
O418 Mo3I O364 96.5(4) . . ?
O270 Mo3I O364 155.3(4) . . ?
O402 Mo3I O411 90.4(4) . . ?
O418 Mo3I O411 164.7(4) . . ?
O270 Mo3I O411 81.9(5) . . ?
O364 Mo3I O411 78.1(4) . . ?
O402 Mo3I O194 165.8(4) . . ?
O418 Mo3I O194 89.3(3) . . ?
O270 Mo3I O194 81.9(3) . . ?
O364 Mo3I O194 79.2(2) . . ?
O411 Mo3I O194 75.7(3) . . ?
O336 Mo3J O479 102.3(4) . . ?
O336 Mo3J O446 100.7(3) . . ?
O479 Mo3J O446 106.0(3) . . ?
O336 Mo3J O404 95.9(3) . . ?
O479 Mo3J O404 89.2(3) . . ?
O446 Mo3J O404 154.3(3) . . ?
O336 Mo3J O324 94.8(3) . . ?
O479 Mo3J O324 153.3(3) . . ?
O446 Mo3J O324 90.5(3) . . ?
O404 Mo3J O324 68.6(3) . . ?
O336 Mo3J O386 172.7(3) . . ?
O479 Mo3J O386 84.1(4) . . ?
O446 Mo3J O386 80.9(3) . . ?
O404 Mo3J O386 80.3(3) . . ?
O324 Mo3J O386 78.0(3) . . ?
O430 Mo3K O504 99.7(4) . . ?
O430 Mo3K O505 100.3(4) . . ?
O504 Mo3K O505 106.8(4) . . ?
O430 Mo3K O147 93.5(4) . . ?
O504 Mo3K O147 89.8(4) . . ?
O505 Mo3K O147 156.1(4) . . ?
O430 Mo3K O366 93.5(4) . . ?
O504 Mo3K O366 156.0(4) . . ?
O505 Mo3K O366 90.3(4) . . ?
O147 Mo3K O366 69.3(3) . . ?
O430 Mo3K O397 174.9(5) . . ?
O504 Mo3K O397 83.0(4) . . ?
O505 Mo3K O397 83.0(4) . . ?
O147 Mo3K O397 82.1(3) . . ?
O366 Mo3K O397 82.5(3) . . ?
O426 Mo3L O461 104.7(5) . . ?
O426 Mo3L O421 100.9(5) . . ?
O461 Mo3L O421 99.9(4) . . ?
O426 Mo3L O274 95.5(4) . . ?
O461 Mo3L O274 92.8(4) . . ?
O421 Mo3L O274 155.9(4) . . ?
O426 Mo3L O378 91.5(4) . . ?
O461 Mo3L O378 162.7(4) . . ?
O421 Mo3L O378 82.6(3) . . ?
O274 Mo3L O378 79.4(3) . . ?
O426 Mo3L O423 165.1(4) . . ?
O461 Mo3L O423 88.9(4) . . ?
O421 Mo3L O423 82.3(4) . . ?
O274 Mo3L O423 77.5(4) . . ?
O378 Mo3L O423 74.4(4) . . ?
O469 Mo3M O438 102.4(5) . . ?
O469 Mo3M O321 100.9(4) . . ?
O438 Mo3M O321 98.2(4) . . ?
O469 Mo3M O175 92.5(4) . . ?
O438 Mo3M O175 164.3(4) . . ?
O321 Mo3M O175 83.6(4) . . ?
O469 Mo3M O447 94.8(4) . . ?
O438 Mo3M O447 93.7(4) . . ?
O321 Mo3M O447 157.7(4) . . ?
O175 Mo3M O447 80.1(3) . . ?
O469 Mo3M O246 168.9(4) . . ?
O438 Mo3M O246 88.0(3) . . ?
O321 Mo3M O246 81.2(3) . . ?
O175 Mo3M O246 76.9(3) . . ?
O447 Mo3M O246 80.5(3) . . ?
O208 Mo3N O420 99.6(4) . . ?
O208 Mo3N O413 98.7(3) . . ?
O420 Mo3N O413 100.9(4) . . ?
O208 Mo3N O185 95.8(3) . . ?
O420 Mo3N O185 93.9(3) . . ?
O413 Mo3N O185 157.2(3) . . ?
O208 Mo3N O406 171.9(4) . . ?
O420 Mo3N O406 86.9(4) . . ?
O413 Mo3N O406 84.7(4) . . ?
O185 Mo3N O406 78.8(3) . . ?
O208 Mo3N O345 100.9(3) . . ?
O420 Mo3N O345 158.7(4) . . ?
O413 Mo3N O345 81.3(3) . . ?
O185 Mo3N O345 78.6(2) . . ?
O406 Mo3N O345 72.2(3) . . ?
O463 Mo3O O441 104.5(4) . . ?
O463 Mo3O O448 99.4(4) . . ?
O441 Mo3O O448 100.3(4) . . ?
O463 Mo3O O375 95.8(4) . 2_576 ?
O441 Mo3O O375 93.8(4) . 2_576 ?
O448 Mo3O O375 155.9(4) . 2_576 ?
O463 Mo3O O213 92.4(3) . . ?
O441 Mo3O O213 162.6(4) . . ?
O448 Mo3O O213 80.9(3) . . ?
O375 Mo3O O213 79.9(3) 2_576 . ?
O463 Mo3O O385 168.9(4) . . ?
O441 Mo3O O385 86.0(4) . . ?
O448 Mo3O O385 82.0(4) . . ?
O375 Mo3O O385 79.5(4) 2_576 . ?
O213 Mo3O O385 76.9(3) . . ?
O471 Mo3P O473 100.2(5) . . ?
O471 Mo3P O472 98.9(6) . . ?
O473 Mo3P O472 107.7(5) . . ?
O471 Mo3P O384 93.7(5) . . ?
O473 Mo3P O384 89.7(4) . . ?
O472 Mo3P O384 156.2(4) . . ?
O471 Mo3P O244 93.0(5) . . ?
O473 Mo3P O244 155.6(4) . . ?
O472 Mo3P O244 90.2(4) . . ?
O384 Mo3P O244 68.9(3) . . ?
O471 Mo3P O462 173.9(5) . . ?
O473 Mo3P O462 83.5(4) . . ?
O472 Mo3P O462 84.6(5) . . ?
O384 Mo3P O462 81.4(3) . . ?
O244 Mo3P O462 81.9(3) . . ?
O466 Mo3Q O321 99.9(4) . . ?
O466 Mo3Q O510 94.2(5) . . ?
O321 Mo3Q O510 91.8(5) . . ?
O466 Mo3Q O509 97.8(5) . . ?
O321 Mo3Q O509 92.5(5) . . ?
O510 Mo3Q O509 166.3(5) . . ?
O466 Mo3Q O459 94.8(4) . . ?
O321 Mo3Q O459 164.9(3) . . ?
O510 Mo3Q O459 83.8(5) . . ?
O509 Mo3Q O459 88.7(5) . . ?
O466 Mo3Q O273 175.5(4) . . ?
O321 Mo3Q O273 83.5(3) . . ?
O510 Mo3Q O273 82.7(4) . . ?
O509 Mo3Q O273 85.0(4) . . ?
O459 Mo3Q O273 81.7(3) . . ?
O743 Mo3R O514 85.7(9) . . ?
O743 Mo3R O395 102.6(7) . . ?
O514 Mo3R O395 99.4(5) . . ?
O743 Mo3R O409 95.6(7) . . ?
O514 Mo3R O409 94.6(5) . . ?
O395 Mo3R O409 157.8(4) . . ?
O743 Mo3R O358 174.0(7) . . ?
O514 Mo3R O358 91.1(5) . . ?
O395 Mo3R O358 82.9(3) . . ?
O409 Mo3R O358 79.6(3) . . ?
O743 Mo3R O458 104.7(9) . . ?
O514 Mo3R O458 167.5(5) . . ?
O395 Mo3R O458 85.3(5) . . ?
O409 Mo3R O458 77.8(5) . . ?
O358 Mo3R O458 77.9(4) . . ?
O487 Mo3S O786 91.3(8) . . ?
O487 Mo3S O383 101.3(5) . . ?
O786 Mo3S O383 99.6(7) . . ?
O487 Mo3S O396 97.0(5) . . ?
O786 Mo3S O396 95.8(7) . . ?
O383 Mo3S O396 155.7(4) . . ?
O487 Mo3S O328 90.9(4) . . ?
O786 Mo3S O328 175.5(7) . . ?
O383 Mo3S O328 83.7(3) . . ?
O396 Mo3S O328 80.0(3) . . ?
O487 Mo3S O450 165.4(5) . . ?
O786 Mo3S O450 102.9(8) . . ?
O383 Mo3S O450 79.5(5) . . ?
O396 Mo3S O450 78.8(5) . . ?
O328 Mo3S O450 74.7(4) . . ?
O480 Mo3T O483 106.2(5) . . ?
O480 Mo3T O481 94.0(6) . . ?
O483 Mo3T O481 93.6(5) . . ?
O480 Mo3T O404 93.3(4) . . ?
O483 Mo3T O404 159.3(4) . . ?
O481 Mo3T O404 92.1(4) . . ?
O480 Mo3T O393 161.7(5) . . ?
O483 Mo3T O393 90.7(4) . . ?
O481 Mo3T O393 91.9(4) . . ?
O404 Mo3T O393 69.2(2) . . ?
O480 Mo3T O482 90.1(5) . . ?
O483 Mo3T O482 90.5(4) . . ?
O481 Mo3T O482 173.2(4) . . ?
O404 Mo3T O482 82.3(4) . . ?
O393 Mo3T O482 82.6(3) . . ?
O525 Mo3U O460 93.3(6) . . ?
O525 Mo3U O395 99.4(5) . . ?
O460 Mo3U O395 97.2(5) . . ?
O525 Mo3U O432 96.2(5) . . ?
O460 Mo3U O432 94.1(4) . . ?
O395 Mo3U O432 160.1(4) . . ?
O525 Mo3U O518 97.8(6) . . ?
O460 Mo3U O518 168.0(5) . . ?
O395 Mo3U O518 85.5(5) . . ?
O432 Mo3U O518 80.3(5) . . ?
O525 Mo3U O380 177.2(6) . . ?
O460 Mo3U O380 89.2(4) . . ?
O395 Mo3U O380 81.7(3) . . ?
O432 Mo3U O380 82.2(3) . . ?
O518 Mo3U O380 79.6(4) . . ?
O494 Mo3V O493 104.1(5) . . ?
O494 Mo3V O442 98.8(5) . . ?
O493 Mo3V O442 99.9(5) . . ?
O494 Mo3V O369 97.0(4) . . ?
O493 Mo3V O369 93.4(4) . . ?
O442 Mo3V O369 156.1(4) . . ?
O494 Mo3V O399 91.8(4) . . ?
O493 Mo3V O399 163.7(4) . . ?
O442 Mo3V O399 81.2(3) . . ?
O369 Mo3V O399 80.6(3) . . ?
O494 Mo3V O529 165.6(5) . . ?
O493 Mo3V O529 89.1(5) . . ?
O442 Mo3V O529 84.2(4) . . ?
O369 Mo3V O529 76.2(4) . . ?
O399 Mo3V O529 74.8(4) . . ?
O499 Mo3W O500 95.1(7) . . ?
O499 Mo3W O421 97.6(6) . . ?
O500 Mo3W O421 99.5(5) . . ?
O499 Mo3W O456 97.0(6) . . ?
O500 Mo3W O456 98.3(5) . . ?
O421 Mo3W O456 155.8(5) . . ?
O499 Mo3W O501 100.4(7) . . ?
O500 Mo3W O501 164.1(5) . . ?
O421 Mo3W O501 82.3(5) . . ?
O456 Mo3W O501 76.2(5) . . ?
O499 Mo3W O370 176.0(6) . . ?
O500 Mo3W O370 88.5(5) . . ?
O421 Mo3W O370 83.7(3) . . ?
O456 Mo3W O370 80.6(4) . . ?
O501 Mo3W O370 75.9(4) . . ?
O523 Mo3X O398 100.4(5) . . ?
O523 Mo3X O413 99.9(4) . . ?
O398 Mo3X O413 97.4(4) . . ?
O523 Mo3X O387 94.2(4) . . ?
O398 Mo3X O387 95.2(4) . . ?
O413 Mo3X O387 159.0(4) . . ?
O523 Mo3X O524 94.3(5) . . ?
O398 Mo3X O524 164.6(5) . . ?
O413 Mo3X O524 84.6(5) . . ?
O387 Mo3X O524 78.9(5) . . ?
O523 Mo3X O303 169.3(4) . . ?
O398 Mo3X O303 88.7(4) . . ?
O413 Mo3X O303 84.3(3) . . ?
O387 Mo3X O303 79.3(3) . . ?
O524 Mo3X O303 76.2(4) . . ?
O496 Mo3Y O412 101.2(6) . . ?
O496 Mo3Y O431 100.4(5) . . ?
O412 Mo3Y O431 96.8(5) . . ?
O496 Mo3Y O449 94.5(5) . . ?
O412 Mo3Y O449 92.7(5) . . ?
O431 Mo3Y O449 160.4(4) . . ?
O496 Mo3Y O495 93.6(6) . . ?
O412 Mo3Y O495 164.3(5) . . ?
O431 Mo3Y O495 85.5(5) . . ?
O449 Mo3Y O495 80.8(5) . . ?
O496 Mo3Y O377 172.0(5) . . ?
O412 Mo3Y O377 85.5(4) . . ?
O431 Mo3Y O377 83.0(3) . . ?
O449 Mo3Y O377 80.8(3) . . ?
O495 Mo3Y O377 79.4(5) . . ?
O454 Mo3Z O506 99.2(6) . . ?
O454 Mo3Z O448 100.1(5) . . ?
O506 Mo3Z O448 95.7(5) . . ?
O454 Mo3Z O505 94.7(5) . . ?
O506 Mo3Z O505 91.0(5) . . ?
O448 Mo3Z O505 162.5(4) . . ?
O454 Mo3Z O424 92.7(5) . . ?
O506 Mo3Z O424 167.0(5) . . ?
O448 Mo3Z O424 87.2(4) . . ?
O505 Mo3Z O424 82.8(4) . . ?
O454 Mo3Z O346 175.3(5) . . ?
O506 Mo3Z O346 84.9(5) . . ?
O448 Mo3Z O346 81.7(3) . . ?
O505 Mo3Z O346 82.9(3) . . ?
O424 Mo3Z O346 82.9(4) . . ?
O237 Mo4A O38 103.4(2) . . ?
O237 Mo4A O74 98.8(2) . . ?
O38 Mo4A O74 88.4(2) . . ?
O237 Mo4A O95 102.8(2) . . ?
O38 Mo4A O95 87.0(2) . . ?
O74 Mo4A O95 158.4(2) . . ?
O237 Mo4A O3 99.8(2) . . ?
O38 Mo4A O3 156.8(2) . . ?
O74 Mo4A O3 89.0(2) . . ?
O95 Mo4A O3 87.1(2) . . ?
O237 Mo4A O21 167.2(2) . . ?
O38 Mo4A O21 87.3(2) . . ?
O74 Mo4A O21 74.22(19) . . ?
O95 Mo4A O21 84.5(2) . . ?
O3 Mo4A O21 69.78(18) . . ?
O58 Mo4B O16 103.7(2) . . ?
O58 Mo4B O5 102.2(2) . . ?
O16 Mo4B O5 98.9(2) . . ?
O58 Mo4B O13 105.2(2) . . ?
O16 Mo4B O13 87.4(2) . . ?
O5 Mo4B O13 149.5(2) . . ?
O58 Mo4B O29 95.0(2) . . ?
O16 Mo4B O29 155.5(2) . . ?
O5 Mo4B O29 92.2(2) . . ?
O13 Mo4B O29 72.46(19) . . ?
O58 Mo4B O125 167.5(2) . . ?
O16 Mo4B O125 88.54(19) . . ?
O5 Mo4B O125 72.91(19) . . ?
O13 Mo4B O125 77.49(18) . . ?
O29 Mo4B O125 73.94(18) . . ?
O73 Mo4C O16 104.2(2) . 2_667 ?
O73 Mo4C O37 99.3(2) . . ?
O16 Mo4C O37 88.6(2) 2_667 . ?
O73 Mo4C O144 101.0(2) . 1_655 ?
O16 Mo4C O144 87.2(2) 2_667 1_655 ?
O37 Mo4C O144 159.7(2) . 1_655 ?
O73 Mo4C O7 100.1(2) . . ?
O16 Mo4C O7 155.7(2) 2_667 . ?
O37 Mo4C O7 87.9(2) . . ?
O144 Mo4C O7 87.79(19) 1_655 . ?
O73 Mo4C O8 167.6(2) . . ?
O16 Mo4C O8 86.21(19) 2_667 . ?
O37 Mo4C O8 73.90(19) . . ?
O144 Mo4C O8 86.01(19) 1_655 . ?
O7 Mo4C O8 69.70(18) . . ?
O61 Mo4D O168 103.4(2) . . ?
O61 Mo4D O15 99.5(2) . . ?
O168 Mo4D O15 89.3(2) . . ?
O61 Mo4D O157 101.3(2) . . ?
O168 Mo4D O157 87.2(2) . . ?
O15 Mo4D O157 159.2(2) . . ?
O61 Mo4D O155 100.0(2) . . ?
O168 Mo4D O155 156.5(2) . . ?
O15 Mo4D O155 88.9(2) . . ?
O157 Mo4D O155 86.2(2) . . ?
O61 Mo4D O114 168.1(2) . . ?
O168 Mo4D O114 86.8(2) . . ?
O15 Mo4D O114 74.2(2) . . ?
O157 Mo4D O114 85.10(19) . . ?
O155 Mo4D O114 70.2(2) . . ?
O124 Mo4E O194 103.9(3) . . ?
O124 Mo4E O132 101.6(2) . . ?
O194 Mo4E O132 105.7(2) . . ?
O124 Mo4E O44 98.3(2) . . ?
O194 Mo4E O44 88.7(2) . . ?
O132 Mo4E O44 151.6(2) . . ?
O124 Mo4E O42 95.8(2) . . ?
O194 Mo4E O42 152.0(2) . . ?
O132 Mo4E O42 89.2(2) . . ?
O44 Mo4E O42 68.8(2) . . ?
O124 Mo4E O243 172.4(2) . . ?
O194 Mo4E O243 82.2(2) . . ?
O132 Mo4E O243 80.7(2) . . ?
O44 Mo4E O243 77.1(2) . . ?
O42 Mo4E O243 76.89(19) . . ?
O110 Mo4F O199 104.8(3) . . ?
O110 Mo4F O144 101.6(2) . . ?
O199 Mo4F O144 105.5(3) . . ?
O110 Mo4F O119 95.7(2) . 2_567 ?
O199 Mo4F O119 89.2(2) . 2_567 ?
O144 Mo4F O119 153.5(2) . 2_567 ?
O110 Mo4F O13 96.5(2) . 2_567 ?
O199 Mo4F O13 150.7(2) . 2_567 ?
O144 Mo4F O13 89.4(2) . 2_567 ?
O119 Mo4F O13 68.64(18) 2_567 2_567 ?
O110 Mo4F O208 174.5(2) . . ?
O199 Mo4F O208 79.2(3) . . ?
O144 Mo4F O208 80.7(2) . . ?
O119 Mo4F O208 80.5(2) 2_567 . ?
O13 Mo4F O208 78.4(2) 2_567 . ?
O45 Mo4G O90 103.6(2) . . ?
O45 Mo4G O10 98.7(3) . . ?
O90 Mo4G O10 88.5(2) . . ?
O45 Mo4G O96 102.8(3) . . ?
O90 Mo4G O96 86.8(2) . . ?
O10 Mo4G O96 158.5(2) . . ?
O45 Mo4G O76 100.2(2) . 2_667 ?
O90 Mo4G O76 156.1(2) . 2_667 ?
O10 Mo4G O76 89.0(2) . 2_667 ?
O96 Mo4G O76 86.8(2) . 2_667 ?
O45 Mo4G O6 167.6(2) . . ?
O90 Mo4G O6 86.59(19) . . ?
O10 Mo4G O6 74.09(18) . . ?
O96 Mo4G O6 84.65(19) . . ?
O76 Mo4G O6 69.93(18) 2_667 . ?
O113 Mo4H O44 104.1(3) . . ?
O113 Mo4H O91 97.6(2) . . ?
O44 Mo4H O91 71.5(2) . . ?
O113 Mo4H O34 96.4(2) . . ?
O44 Mo4H O34 140.0(2) . . ?
O91 Mo4H O34 72.0(2) . . ?
O113 Mo4H O42 91.2(2) . . ?
O44 Mo4H O42 71.6(2) . . ?
O91 Mo4H O42 143.0(2) . . ?
O34 Mo4H O42 142.7(2) . . ?
O113 Mo4H O4 97.3(2) . . ?
O44 Mo4H O4 137.4(2) . . ?
O91 Mo4H O4 141.6(2) . . ?
O34 Mo4H O4 71.3(2) . . ?
O42 Mo4H O4 71.5(2) . . ?
O113 Mo4H O66 170.3(2) . . ?
O44 Mo4H O66 82.2(2) . . ?
O91 Mo4H O66 91.3(2) . . ?
O34 Mo4H O66 82.82(19) . . ?
O42 Mo4H O66 83.75(18) . . ?
O4 Mo4H O66 73.31(18) . . ?
O240 Mo4I O131 97.9(3) . . ?
O240 Mo4I O14 103.9(3) . . ?
O131 Mo4I O14 71.9(2) . . ?
O240 Mo4I O68 91.6(2) . . ?
O131 Mo4I O68 143.3(2) . . ?
O14 Mo4I O68 71.4(2) . . ?
O240 Mo4I O106 95.3(2) . . ?
O131 Mo4I O106 72.0(2) . . ?
O14 Mo4I O106 140.9(2) . . ?
O68 Mo4I O106 142.4(2) . . ?
O240 Mo4I O23 98.1(3) . . ?
O131 Mo4I O23 140.9(2) . . ?
O14 Mo4I O23 136.9(2) . . ?
O68 Mo4I O23 71.3(2) . . ?
O106 Mo4I O23 71.1(2) . . ?
O240 Mo4I O69 172.2(2) . . ?
O131 Mo4I O69 89.2(2) . . ?
O14 Mo4I O69 81.3(2) . . ?
O68 Mo4I O69 84.55(19) . . ?
O106 Mo4I O69 83.8(2) . . ?
O23 Mo4I O69 74.3(2) . . ?
O121 Mo4J O246 104.2(3) . . ?
O121 Mo4J O100 102.0(2) . . ?
O246 Mo4J O100 105.2(2) . . ?
O121 Mo4J O14 98.3(2) . . ?
O246 Mo4J O14 89.1(2) . . ?
O100 Mo4J O14 151.3(2) . . ?
O121 Mo4J O68 94.5(2) . . ?
O246 Mo4J O68 152.8(2) . . ?
O100 Mo4J O68 89.8(2) . . ?
O14 Mo4J O68 68.4(2) . . ?
O121 Mo4J O64 173.1(2) . . ?
O246 Mo4J O64 81.7(2) . . ?
O100 Mo4J O64 79.75(19) . . ?
O14 Mo4J O64 77.8(2) . . ?
O68 Mo4J O64 78.7(2) . . ?
O170 Mo4K O345 105.0(4) . . ?
O170 Mo4K O157 101.4(3) . . ?
O345 Mo4K O157 104.9(3) . . ?
O170 Mo4K O33 96.4(2) . . ?
O345 Mo4K O33 90.6(3) . . ?
O157 Mo4K O33 152.3(2) . . ?
O170 Mo4K O79 95.2(3) . . ?
O345 Mo4K O79 152.1(3) . . ?
O157 Mo4K O79 89.3(2) . . ?
O33 Mo4K O79 67.96(18) . . ?
O170 Mo4K O192 174.6(3) . 2_567 ?
O345 Mo4K O192 79.3(3) . 2_567 ?
O157 Mo4K O192 80.3(2) . 2_567 ?
O33 Mo4K O192 80.2(2) . 2_567 ?
O79 Mo4K O192 79.7(2) . 2_567 ?
O254 Mo4L O196 103.4(3) . . ?
O254 Mo4L O176 100.2(3) . . ?
O196 Mo4L O176 89.3(2) . . ?
O254 Mo4L O123 102.3(3) . . ?
O196 Mo4L O123 86.9(2) . . ?
O176 Mo4L O123 157.4(2) . . ?
O254 Mo4L O55 98.7(2) . . ?
O196 Mo4L O55 157.8(2) . . ?
O176 Mo4L O55 88.8(2) . . ?
O123 Mo4L O55 86.4(2) . . ?
O254 Mo4L O32 167.4(2) . . ?
O196 Mo4L O32 87.8(2) . . ?
O176 Mo4L O32 73.9(2) . . ?
O123 Mo4L O32 83.7(2) . . ?
O55 Mo4L O32 70.41(19) . . ?
O143 Mo4M O90 103.0(2) . . ?
O143 Mo4M O15 101.6(3) . . ?
O90 Mo4M O15 98.1(2) . . ?
O143 Mo4M O269 105.2(3) . . ?
O90 Mo4M O269 87.9(2) . . ?
O15 Mo4M O269 150.4(2) . . ?
O143 Mo4M O24 96.4(2) . . ?
O90 Mo4M O24 155.2(2) . . ?
O15 Mo4M O24 93.0(2) . . ?
O269 Mo4M O24 72.0(2) . . ?
O143 Mo4M O114 168.9(2) . . ?
O90 Mo4M O114 87.55(19) . . ?
O15 Mo4M O114 73.00(19) . . ?
O269 Mo4M O114 78.38(19) . . ?
O24 Mo4M O114 74.51(18) . . ?
O182 Mo4N O136 103.9(2) . . ?
O182 Mo4N O31 99.7(3) . . ?
O136 Mo4N O31 89.3(2) . . ?
O182 Mo4N O221 102.1(3) . . ?
O136 Mo4N O221 86.9(2) . . ?
O31 Mo4N O221 158.2(2) . . ?
O182 Mo4N O155 99.6(2) . . ?
O136 Mo4N O155 156.4(2) . . ?
O31 Mo4N O155 89.3(2) . . ?
O221 Mo4N O155 85.7(2) . . ?
O182 Mo4N O67 167.9(2) . . ?
O136 Mo4N O67 86.6(2) . . ?
O31 Mo4N O67 74.1(2) . . ?
O221 Mo4N O67 84.3(2) . . ?
O155 Mo4N O67 70.3(2) . . ?
O188 Mo4O O27 98.0(3) . . ?
O188 Mo4O O262 103.8(2) . . ?
O27 Mo4O O262 72.0(2) . . ?
O188 Mo4O O12 92.3(2) . . ?
O27 Mo4O O12 143.8(2) . . ?
O262 Mo4O O12 71.8(2) . . ?
O188 Mo4O O104 94.6(2) . . ?
O27 Mo4O O104 72.1(2) . . ?
O262 Mo4O O104 141.5(2) . . ?
O12 Mo4O O104 141.7(2) . . ?
O188 Mo4O O36 99.9(2) . . ?
O27 Mo4O O36 139.9(2) . . ?
O262 Mo4O O36 136.0(2) . . ?
O12 Mo4O O36 70.72(19) . . ?
O104 Mo4O O36 71.0(2) . . ?
O188 Mo4O O86 173.7(2) . . ?
O27 Mo4O O86 87.5(2) . . ?
O262 Mo4O O86 80.7(2) . . ?
O12 Mo4O O86 84.92(19) . . ?
O104 Mo4O O86 84.2(2) . . ?
O36 Mo4O O86 73.83(18) . . ?
O145 Mo4P O98 103.5(2) . . ?
O145 Mo4P O81 102.7(3) . . ?
O98 Mo4P O81 98.1(2) . . ?
O145 Mo4P O34 104.9(3) . . ?
O98 Mo4P O34 87.8(2) . . ?
O81 Mo4P O34 149.5(2) . . ?
O145 Mo4P O4 96.2(2) . . ?
O98 Mo4P O4 154.9(2) . . ?
O81 Mo4P O4 92.5(2) . . ?
O34 Mo4P O4 72.0(2) . . ?
O145 Mo4P O17 168.4(2) . . ?
O98 Mo4P O17 87.7(2) . . ?
O81 Mo4P O17 72.35(19) . . ?
O34 Mo4P O17 78.07(19) . . ?
O4 Mo4P O17 73.78(17) . . ?
O28 Mo4Q O86 104.2(2) . . ?
O28 Mo4Q O21 106.4(3) . . ?
O86 Mo4Q O21 100.0(2) . . ?
O28 Mo4Q O80 105.7(2) . . ?
O86 Mo4Q O80 95.5(2) . . ?
O21 Mo4Q O80 139.5(2) . . ?
O28 Mo4Q O3 97.6(2) . . ?
O86 Mo4Q O3 158.0(2) . . ?
O21 Mo4Q O3 76.4(2) . . ?
O80 Mo4Q O3 75.4(2) . . ?
O28 Mo4Q O36 177.2(2) . . ?
O86 Mo4Q O36 73.12(19) . . ?
O21 Mo4Q O36 74.69(19) . . ?
O80 Mo4Q O36 74.41(18) . . ?
O3 Mo4Q O36 85.08(17) . . ?
O25 Mo4R O127 103.8(2) . . ?
O25 Mo4R O176 102.7(3) . . ?
O127 Mo4R O176 97.8(2) . . ?
O25 Mo4R O106 104.5(3) . . ?
O127 Mo4R O106 88.1(2) . . ?
O176 Mo4R O106 149.9(2) . . ?
O25 Mo4R O23 95.1(2) . . ?
O127 Mo4R O23 155.6(2) . . ?
O176 Mo4R O23 92.9(2) . . ?
O106 Mo4R O23 72.1(2) . . ?
O25 Mo4R O32 167.6(2) . . ?
O127 Mo4R O32 88.4(2) . . ?
O176 Mo4R O32 72.4(2) . . ?
O106 Mo4R O32 78.26(19) . . ?
O23 Mo4R O32 74.04(19) . . ?
O87 Mo4S O20 103.9(2) . . ?
O87 Mo4S O125 105.6(2) . . ?
O20 Mo4S O125 98.3(2) . . ?
O87 Mo4S O6 105.3(2) . . ?
O20 Mo4S O6 97.7(2) . . ?
O125 Mo4S O6 140.5(2) . . ?
O87 Mo4S O76 98.0(2) . 2_667 ?
O20 Mo4S O76 158.1(2) . 2_667 ?
O125 Mo4S O76 76.12(19) . 2_667 ?
O6 Mo4S O76 75.67(19) . 2_667 ?
O87 Mo4S O29 177.6(2) . . ?
O20 Mo4S O29 73.72(19) . . ?
O125 Mo4S O29 75.04(18) . . ?
O6 Mo4S O29 75.15(18) . . ?
O76 Mo4S O29 84.42(18) 2_667 . ?
O56 Mo4T O66 104.1(3) . . ?
O56 Mo4T O17 106.0(2) . . ?
O66 Mo4T O17 97.9(2) . . ?
O56 Mo4T O8 104.6(2) . . ?
O66 Mo4T O8 97.8(2) . . ?
O17 Mo4T O8 140.7(2) . . ?
O56 Mo4T O7 98.6(2) . . ?
O66 Mo4T O7 157.3(2) . . ?
O17 Mo4T O7 76.4(2) . . ?
O8 Mo4T O7 75.33(19) . . ?
O56 Mo4T O4 176.8(2) . . ?
O66 Mo4T O4 72.9(2) . . ?
O17 Mo4T O4 75.86(18) . . ?
O8 Mo4T O4 74.83(17) . . ?
O7 Mo4T O4 84.42(18) . . ?
O247 Mo4U O189 103.6(3) . . ?
O247 Mo4U O31 103.2(3) . . ?
O189 Mo4U O31 98.4(2) . . ?
O247 Mo4U O181 104.7(3) . . ?
O189 Mo4U O181 87.5(2) . . ?
O31 Mo4U O181 149.3(2) . . ?
O247 Mo4U O24 96.2(2) . . ?
O189 Mo4U O24 154.7(2) . . ?
O31 Mo4U O24 92.1(2) . . ?
O181 Mo4U O24 72.2(2) . . ?
O247 Mo4U O67 168.9(2) . . ?
O189 Mo4U O67 87.2(2) . . ?
O31 Mo4U O67 72.7(2) . . ?
O181 Mo4U O67 77.5(2) . . ?
O24 Mo4U O67 73.97(18) . . ?
O202 Mo4V O136 103.3(3) . . ?
O202 Mo4V O49 102.6(3) . . ?
O136 Mo4V O49 98.5(2) . . ?
O202 Mo4V O172 104.9(3) . . ?
O136 Mo4V O172 87.5(2) . . ?
O49 Mo4V O172 149.7(2) . . ?
O202 Mo4V O82 95.2(2) . . ?
O136 Mo4V O82 155.5(2) . . ?
O49 Mo4V O82 92.8(2) . . ?
O172 Mo4V O82 72.2(2) . . ?
O202 Mo4V O59 168.5(2) . . ?
O136 Mo4V O59 87.9(2) . . ?
O49 Mo4V O59 72.7(2) . . ?
O172 Mo4V O59 77.91(19) . . ?
O82 Mo4V O59 74.77(18) . . ?
O210 Mo4W O343 104.7(4) . . ?
O210 Mo4W O26 101.4(3) . . ?
O343 Mo4W O26 106.0(3) . . ?
O210 Mo4W O131 95.5(3) . . ?
O343 Mo4W O131 89.1(3) . . ?
O26 Mo4W O131 153.4(2) . . ?
O210 Mo4W O106 94.1(2) . . ?
O343 Mo4W O106 151.9(3) . . ?
O26 Mo4W O106 90.1(2) . . ?
O131 Mo4W O106 68.2(2) . . ?
O210 Mo4W O159 171.9(3) . . ?
O343 Mo4W O159 82.4(4) . . ?
O26 Mo4W O159 80.1(3) . . ?
O131 Mo4W O159 80.4(2) . . ?
O106 Mo4W O159 77.9(2) . . ?
O149 Mo4X O38 103.3(2) . . ?
O149 Mo4X O92 102.6(3) . . ?
O38 Mo4X O92 98.3(2) . . ?
O149 Mo4X O167 104.6(3) . . ?
O38 Mo4X O167 87.9(2) . . ?
O92 Mo4X O167 149.8(2) . . ?
O149 Mo4X O82 95.5(2) . . ?
O38 Mo4X O82 155.5(2) . . ?
O92 Mo4X O82 92.7(2) . . ?
O167 Mo4X O82 72.0(2) . . ?
O149 Mo4X O47 168.4(2) . . ?
O38 Mo4X O47 87.9(2) . . ?
O92 Mo4X O47 72.4(2) . . ?
O167 Mo4X O47 78.41(19) . . ?
O82 Mo4X O47 74.53(19) . . ?
O134 Mo4Y O360 103.9(3) . . ?
O134 Mo4Y O122 100.9(3) . . ?
O360 Mo4Y O122 105.6(3) . . ?
O134 Mo4Y O139 95.1(2) . . ?
O360 Mo4Y O139 90.1(2) . . ?
O122 Mo4Y O139 154.0(2) . . ?
O134 Mo4Y O272 95.2(3) . . ?
O360 Mo4Y O272 152.7(3) . . ?
O122 Mo4Y O272 89.4(2) . . ?
O139 Mo4Y O272 68.7(2) . . ?
O134 Mo4Y O197 171.4(3) . . ?
O360 Mo4Y O197 83.7(3) . . ?
O122 Mo4Y O197 80.8(2) . . ?
O139 Mo4Y O197 80.5(2) . . ?
O272 Mo4Y O197 76.3(2) . . ?
O228 Mo4Z O98 104.1(2) . . ?
O228 Mo4Z O57 98.8(3) . . ?
O98 Mo4Z O57 89.6(2) . . ?
O228 Mo4Z O183 101.6(3) . . ?
O98 Mo4Z O183 87.4(2) . . ?
O57 Mo4Z O183 159.5(2) . . ?
O228 Mo4Z O84 100.8(2) . . ?
O98 Mo4Z O84 155.0(2) . . ?
O57 Mo4Z O84 88.5(2) . . ?
O183 Mo4Z O84 85.7(2) . . ?
O228 Mo4Z O41 167.8(2) . . ?
O98 Mo4Z O41 85.89(19) . . ?
O57 Mo4Z O41 73.8(2) . . ?
O183 Mo4Z O41 85.7(2) . . ?
O84 Mo4Z O41 69.62(19) . . ?
O156 Mo10 O50 104.0(2) . . ?
O156 Mo10 O78 98.9(3) . . ?
O50 Mo10 O78 88.6(2) . . ?
O156 Mo10 O97 102.6(3) . . ?
O50 Mo10 O97 86.7(2) . . ?
O78 Mo10 O97 158.5(2) . . ?
O156 Mo10 O55 98.4(2) . . ?
O50 Mo10 O55 157.6(2) . . ?
O78 Mo10 O55 88.7(2) . . ?
O97 Mo10 O55 87.6(2) . . ?
O156 Mo10 O109 167.0(2) . . ?
O50 Mo10 O109 87.2(2) . . ?
O78 Mo10 O109 74.46(19) . . ?
O97 Mo10 O109 84.3(2) . . ?
O55 Mo10 O109 70.59(19) . . ?
O71 Mo11 O102 104.5(2) . . ?
O71 Mo11 O141 103.5(3) . . ?
O102 Mo11 O141 98.6(2) . . ?
O71 Mo11 O206 103.7(3) . . ?
O102 Mo11 O206 87.6(2) . . ?
O141 Mo11 O206 149.6(2) . . ?
O71 Mo11 O77 94.2(2) . . ?
O102 Mo11 O77 155.4(2) . . ?
O141 Mo11 O77 92.4(2) . . ?
O206 Mo11 O77 72.2(2) . . ?
O71 Mo11 O107 167.9(2) . . ?
O102 Mo11 O107 87.6(2) . . ?
O141 Mo11 O107 73.0(2) . . ?
O206 Mo11 O107 77.5(2) . . ?
O77 Mo11 O107 74.6(2) . . ?
O293 Mo12 O196 102.9(3) . . ?
O293 Mo12 O35 102.4(3) . . ?
O196 Mo12 O35 98.0(2) . . ?
O293 Mo12 O164 105.2(3) . . ?
O196 Mo12 O164 88.2(2) . . ?
O35 Mo12 O164 149.6(2) . . ?
O293 Mo12 O19 95.6(2) . . ?
O196 Mo12 O19 156.0(2) . . ?
O35 Mo12 O19 92.8(2) . . ?
O164 Mo12 O19 72.1(2) . . ?
O293 Mo12 O43 167.9(2) . . ?
O196 Mo12 O43 88.8(2) . . ?
O35 Mo12 O43 72.8(2) . . ?
O164 Mo12 O43 77.6(2) . . ?
O19 Mo12 O43 73.9(2) . . ?
O205 Mo13 O65 103.8(3) . . ?
O205 Mo13 O248 104.2(3) . . ?
O65 Mo13 O248 98.0(3) . . ?
O205 Mo13 O212 103.0(3) . . ?
O65 Mo13 O212 87.8(2) . . ?
O248 Mo13 O212 149.9(2) . . ?
O205 Mo13 O46 94.7(3) . . ?
O65 Mo13 O46 155.4(2) . . ?
O248 Mo13 O46 93.0(2) . . ?
O212 Mo13 O46 72.1(2) . . ?
O205 Mo13 O235 168.2(2) . 2_576 ?
O65 Mo13 O235 88.0(2) . 2_576 ?
O248 Mo13 O235 73.4(2) . 2_576 ?
O212 Mo13 O235 77.4(2) . 2_576 ?
O46 Mo13 O235 74.2(2) . 2_576 ?
O133 Mo14 O102 103.8(2) . . ?
O133 Mo14 O105 99.7(3) . . ?
O102 Mo14 O105 89.5(2) . . ?
O133 Mo14 O334 103.3(3) . . ?
O102 Mo14 O334 86.8(2) . . ?
O105 Mo14 O334 156.9(2) . . ?
O133 Mo14 O289 98.3(2) . . ?
O102 Mo14 O289 157.9(2) . . ?
O105 Mo14 O289 88.3(2) . . ?
O334 Mo14 O289 86.6(2) . . ?
O133 Mo14 O191 166.7(2) . . ?
O102 Mo14 O191 88.1(2) . . ?
O105 Mo14 O191 74.2(2) . . ?
O334 Mo14 O191 82.9(2) . . ?
O289 Mo14 O191 70.1(2) . . ?
O174 Mo15 O127 104.4(2) . . ?
O174 Mo15 O35 99.5(3) . . ?
O127 Mo15 O35 88.9(2) . . ?
O174 Mo15 O26 102.0(3) . . ?
O127 Mo15 O26 87.2(2) . . ?
O35 Mo15 O26 158.4(2) . . ?
O174 Mo15 O84 99.2(2) . . ?
O127 Mo15 O84 156.4(2) . . ?
O35 Mo15 O84 88.1(2) . . ?
O26 Mo15 O84 87.0(2) . . ?
O174 Mo15 O43 167.0(2) . . ?
O127 Mo15 O43 86.9(2) . . ?
O35 Mo15 O43 73.9(2) . . ?
O26 Mo15 O43 84.7(2) . . ?
O84 Mo15 O43 69.78(19) . . ?
O130 Mo16 O65 103.5(3) . . ?
O130 Mo16 O325 100.0(3) . . ?
O65 Mo16 O325 89.3(2) . . ?
O130 Mo16 O333 103.2(3) . . ?
O65 Mo16 O333 86.8(2) . . ?
O325 Mo16 O333 156.8(2) . . ?
O130 Mo16 O138 98.1(3) . . ?
O65 Mo16 O138 158.4(2) . . ?
O325 Mo16 O138 88.9(2) . . ?
O333 Mo16 O138 86.4(2) . . ?
O130 Mo16 O178 166.7(3) . . ?
O65 Mo16 O178 88.7(2) . . ?
O325 Mo16 O178 74.7(2) . . ?
O333 Mo16 O178 82.4(2) . . ?
O138 Mo16 O178 70.0(2) . . ?
O150 Mo17 O54 103.1(3) . . ?
O150 Mo17 O57 101.9(3) . . ?
O54 Mo17 O57 98.6(2) . . ?
O150 Mo17 O272 105.3(3) . . ?
O54 Mo17 O272 87.7(2) . . ?
O57 Mo17 O272 149.8(2) . . ?
O150 Mo17 O19 96.0(3) . . ?
O54 Mo17 O19 155.6(2) . . ?
O57 Mo17 O19 92.2(2) . . ?
O272 Mo17 O19 72.4(2) . . ?
O150 Mo17 O41 168.8(2) . . ?
O54 Mo17 O41 87.6(2) . . ?
O57 Mo17 O41 72.9(2) . . ?
O272 Mo17 O41 78.0(2) . . ?
O19 Mo17 O41 74.65(19) . . ?
O241 Mo18 O126 102.8(2) . . ?
O241 Mo18 O92 100.1(3) . . ?
O126 Mo18 O92 88.8(2) . . ?
O241 Mo18 O161 102.4(3) . . ?
O126 Mo18 O161 87.2(2) . . ?
O92 Mo18 O161 157.4(2) . . ?
O241 Mo18 O63 100.0(2) . . ?
O126 Mo18 O63 157.2(2) . . ?
O92 Mo18 O63 88.7(2) . . ?
O161 Mo18 O63 86.5(2) . . ?
O241 Mo18 O47 168.2(3) . . ?
O126 Mo18 O47 87.39(19) . . ?
O92 Mo18 O47 74.0(2) . . ?
O161 Mo18 O47 83.7(2) . . ?
O63 Mo18 O47 70.10(19) . . ?
O60 Mo19 O53 103.6(3) . . ?
O60 Mo19 O43 105.3(2) . . ?
O53 Mo19 O43 98.5(2) . . ?
O60 Mo19 O41 105.1(2) . . ?
O53 Mo19 O41 97.9(2) . . ?
O43 Mo19 O41 140.7(2) . . ?
O60 Mo19 O84 98.9(2) . . ?
O53 Mo19 O84 157.5(2) . . ?
O43 Mo19 O84 75.9(2) . . ?
O41 Mo19 O84 75.35(19) . . ?
O60 Mo19 O19 177.4(2) . . ?
O53 Mo19 O19 73.8(2) . . ?
O43 Mo19 O19 75.2(2) . . ?
O41 Mo19 O19 75.6(2) . . ?
O84 Mo19 O19 83.7(2) . . ?
O313 Mo20 O277 104.7(3) . . ?
O313 Mo20 O52 99.0(3) . . ?
O277 Mo20 O52 89.3(2) . . ?
O313 Mo20 O117 102.2(3) . . ?
O277 Mo20 O117 86.6(2) . . ?
O52 Mo20 O117 158.7(2) . . ?
O313 Mo20 O259 99.3(3) . . ?
O277 Mo20 O259 155.9(2) . . ?
O52 Mo20 O259 88.8(2) . . ?
O117 Mo20 O259 86.4(2) . . ?
O313 Mo20 O116 166.9(3) . . ?
O277 Mo20 O116 86.8(2) . . ?
O52 Mo20 O116 74.4(2) . . ?
O117 Mo20 O116 84.5(2) . . ?
O259 Mo20 O116 69.6(2) . . ?
O260 Mo21 O358 102.5(4) . . ?
O260 Mo21 O123 100.4(3) . . ?
O358 Mo21 O123 106.4(3) . . ?
O260 Mo21 O163 97.0(3) . . ?
O358 Mo21 O163 89.2(3) . . ?
O123 Mo21 O163 153.3(3) . . ?
O260 Mo21 O164 93.4(3) . . ?
O358 Mo21 O164 154.1(3) . . ?
O123 Mo21 O164 90.4(2) . . ?
O163 Mo21 O164 68.4(2) . . ?
O260 Mo21 O382 171.7(3) . . ?
O358 Mo21 O382 84.8(4) . . ?
O123 Mo21 O382 81.0(3) . . ?
O163 Mo21 O382 79.0(3) . . ?
O164 Mo21 O382 78.4(3) . . ?
O282 Mo22 O173 102.9(3) . . ?
O282 Mo22 O232 103.1(3) . . ?
O173 Mo22 O232 98.5(3) . . ?
O282 Mo22 O62 104.7(3) . . ?
O173 Mo22 O62 87.6(3) . . ?
O232 Mo22 O62 149.5(3) . . ?
O282 Mo22 O263 96.5(3) . . ?
O173 Mo22 O263 155.0(3) . . ?
O232 Mo22 O263 92.3(2) . . ?
O62 Mo22 O263 72.2(2) . . ?
O282 Mo22 O225 169.9(3) . . ?
O173 Mo22 O225 87.0(2) . . ?
O232 Mo22 O225 73.0(2) . . ?
O62 Mo22 O225 77.5(2) . . ?
O263 Mo22 O225 74.7(2) . . ?
O294 Mo23 O173 103.5(3) . . ?
O294 Mo23 O304 98.6(3) . . ?
O173 Mo23 O304 89.1(3) . . ?
O294 Mo23 O276 102.3(3) . . ?
O173 Mo23 O276 86.8(3) . . ?
O304 Mo23 O276 159.1(2) . . ?
O294 Mo23 O138 99.6(3) . . ?
O173 Mo23 O138 156.8(2) . . ?
O304 Mo23 O138 89.4(2) . . ?
O276 Mo23 O138 86.4(2) . . ?
O294 Mo23 O85 167.0(3) . . ?
O173 Mo23 O85 87.4(2) . . ?
O304 Mo23 O85 74.3(2) . . ?
O276 Mo23 O85 85.1(2) . . ?
O138 Mo23 O85 69.9(2) . . ?
O128 Mo24 O291 104.2(3) . . ?
O128 Mo24 O120 98.6(3) . . ?
O291 Mo24 O120 89.1(3) . . ?
O128 Mo24 O195 102.6(3) . . ?
O291 Mo24 O195 86.7(3) . . ?
O120 Mo24 O195 158.8(3) . . ?
O128 Mo24 O289 100.2(3) . . ?
O291 Mo24 O289 155.6(2) . . ?
O120 Mo24 O289 89.1(2) . . ?
O195 Mo24 O289 86.2(2) . . ?
O128 Mo24 O146 167.3(2) . . ?
O291 Mo24 O146 86.4(2) . . ?
O120 Mo24 O146 74.4(2) . . ?
O195 Mo24 O146 84.6(2) . . ?
O289 Mo24 O146 69.6(2) . . ?
O234 Mo25 O252 104.8(3) . . ?
O234 Mo25 O242 98.9(3) . . ?
O252 Mo25 O242 89.1(3) . . ?
O234 Mo25 O180 102.3(3) . . ?
O252 Mo25 O180 86.7(2) . . ?
O242 Mo25 O180 158.7(3) . . ?
O234 Mo25 O184 99.9(3) . . ?
O252 Mo25 O184 155.2(2) . . ?
O242 Mo25 O184 88.6(3) . . ?
O180 Mo25 O184 86.6(2) . . ?
O234 Mo25 O101 167.1(2) . . ?
O252 Mo25 O101 86.2(2) . . ?
O242 Mo25 O101 74.3(2) . . ?
O180 Mo25 O101 84.6(2) . . ?
O184 Mo25 O101 69.4(2) . . ?
O158 Mo26 O193 103.9(3) . . ?
O158 Mo26 O171 99.7(3) . . ?
O193 Mo26 O171 88.3(3) . . ?
O158 Mo26 O230 101.6(3) . . ?
O193 Mo26 O230 87.3(2) . . ?
O171 Mo26 O230 158.7(2) . . ?
O158 Mo26 O83 99.8(3) . . ?
O193 Mo26 O83 156.3(2) . . ?
O171 Mo26 O83 88.8(2) . . ?
O230 Mo26 O83 86.8(2) . . ?
O158 Mo26 O224 167.8(2) . . ?
O193 Mo26 O224 86.5(2) . . ?
O171 Mo26 O224 73.8(2) . . ?
O230 Mo26 O224 85.1(2) . . ?
O83 Mo26 O224 70.2(2) . . ?
O166 Mo27 O277 103.0(3) . . ?
O166 Mo27 O242 103.4(3) . . ?
O277 Mo27 O242 98.1(3) . . ?
O166 Mo27 O302 104.4(3) . . ?
O277 Mo27 O302 87.7(2) . . ?
O242 Mo27 O302 149.4(3) . . ?
O166 Mo27 O256 96.5(3) . . ?
O277 Mo27 O256 154.7(2) . . ?
O242 Mo27 O256 92.6(3) . . ?
O302 Mo27 O256 71.9(2) . . ?
O166 Mo27 O101 169.4(3) . . ?
O277 Mo27 O101 87.4(2) . . ?
O242 Mo27 O101 72.7(2) . . ?
O302 Mo27 O101 77.7(2) . . ?
O256 Mo27 O101 74.1(2) . . ?
O340 Mo28 O405 102.9(4) . . ?
O340 Mo28 O364 100.1(4) . . ?
O405 Mo28 O364 106.2(3) . . ?
O340 Mo28 O91 95.8(3) . . ?
O405 Mo28 O91 89.0(3) . . ?
O364 Mo28 O91 154.8(3) . . ?
O340 Mo28 O44 97.4(3) . . ?
O405 Mo28 O44 151.4(3) . . ?
O364 Mo28 O44 89.6(3) . . ?
O91 Mo28 O44 68.9(2) . . ?
O340 Mo28 O290 172.9(3) . . ?
O405 Mo28 O290 83.2(3) . . ?
O364 Mo28 O290 81.4(4) . . ?
O91 Mo28 O290 80.6(2) . . ?
O44 Mo28 O290 75.6(2) . . ?
O152 Mo29 O215 104.6(4) . . ?
O152 Mo29 O96 100.3(3) . . ?
O215 Mo29 O96 106.2(3) . . ?
O152 Mo29 O231 95.3(3) . . ?
O215 Mo29 O231 88.8(3) . . ?
O96 Mo29 O231 154.7(2) . . ?
O152 Mo29 O269 94.5(3) . . ?
O215 Mo29 O269 151.8(3) . . ?
O96 Mo29 O269 90.2(2) . . ?
O231 Mo29 O269 68.7(2) . . ?
O152 Mo29 O299 171.5(3) . . ?
O215 Mo29 O299 83.0(3) . . ?
O96 Mo29 O299 80.9(2) . . ?
O231 Mo29 O299 80.9(3) . . ?
O269 Mo29 O299 77.0(2) . . ?
O376 Mo30 O244 100.2(3) . . ?
O376 Mo30 O384 101.1(3) . . ?
O244 Mo30 O384 71.3(3) . . ?
O376 Mo30 O362 95.0(3) . . ?
O244 Mo30 O362 71.4(2) . . ?
O384 Mo30 O362 141.4(3) . . ?
O376 Mo30 O239 93.3(3) . . ?
O244 Mo30 O239 142.7(2) . . ?
O384 Mo30 O239 72.0(3) . . ?
O362 Mo30 O239 142.1(2) . . ?
O376 Mo30 O22 98.3(3) . . ?
O244 Mo30 O22 139.2(3) . . ?
O384 Mo30 O22 139.1(2) . . ?
O362 Mo30 O22 71.0(2) . . ?
O239 Mo30 O22 71.2(2) . . ?
O376 Mo30 O222 172.1(3) . . ?
O244 Mo30 O222 86.8(3) . . ?
O384 Mo30 O222 84.6(3) . . ?
O362 Mo30 O222 83.7(2) . . ?
O239 Mo30 O222 83.2(2) . . ?
O22 Mo30 O222 73.9(2) . . ?
O372 Mo31 O392 100.2(4) . . ?
O372 Mo31 O432 100.5(4) . . ?
O392 Mo31 O432 107.0(3) . . ?
O372 Mo31 O262 96.3(3) . . ?
O392 Mo31 O262 91.1(3) . . ?
O432 Mo31 O262 152.5(3) . . ?
O372 Mo31 O27 91.9(3) . . ?
O392 Mo31 O27 157.9(3) . . ?
O432 Mo31 O27 88.6(3) . . ?
O262 Mo31 O27 69.1(2) . . ?
O372 Mo31 O407 172.8(4) . . ?
O392 Mo31 O407 82.1(3) . . ?
O432 Mo31 O407 85.2(3) . . ?
O262 Mo31 O407 76.8(2) . . ?
O27 Mo31 O407 83.7(2) . . ?
O118 Mo32 O346 104.2(4) . . ?
O118 Mo32 O276 100.2(3) . . ?
O346 Mo32 O276 105.0(3) . . ?
O118 Mo32 O366 95.9(3) . . ?
O346 Mo32 O366 89.9(3) . . ?
O276 Mo32 O366 154.4(3) . . ?
O118 Mo32 O62 94.7(3) . . ?
O346 Mo32 O62 152.9(3) . . ?
O276 Mo32 O62 90.3(3) . . ?
O366 Mo32 O62 68.6(3) . . ?
O118 Mo32 O417 172.0(3) . . ?
O346 Mo32 O417 83.3(4) . . ?
O276 Mo32 O417 80.0(3) . . ?
O366 Mo32 O417 81.3(3) . . ?
O62 Mo32 O417 77.4(3) . . ?
O316 Mo33 O370 103.6(4) . . ?
O316 Mo33 O211 101.0(3) . . ?
O370 Mo33 O211 105.3(3) . . ?
O316 Mo33 O330 94.7(3) . . ?
O370 Mo33 O330 89.7(3) . . ?
O211 Mo33 O330 155.0(3) . . ?
O316 Mo33 O275 94.9(3) . . ?
O370 Mo33 O275 152.9(3) . . ?
O211 Mo33 O275 90.1(2) . . ?
O330 Mo33 O275 69.0(2) . . ?
O316 Mo33 O335 171.1(3) . . ?
O370 Mo33 O335 83.0(3) . . ?
O211 Mo33 O335 82.8(3) . . ?
O330 Mo33 O335 79.2(3) . . ?
O275 Mo33 O335 76.9(2) . . ?
O389 Mo34 O186 103.9(3) . . ?
O389 Mo34 O207 99.9(3) . . ?
O186 Mo34 O207 88.6(3) . . ?
O389 Mo34 O446 102.5(3) . . ?
O186 Mo34 O446 87.3(3) . . ?
O207 Mo34 O446 157.6(3) . . ?
O389 Mo34 O177 99.9(3) . . ?
O186 Mo34 O177 156.1(3) . . ?
O207 Mo34 O177 89.1(3) . . ?
O446 Mo34 O177 85.7(3) . . ?
O389 Mo34 O266 167.7(3) . . ?
O186 Mo34 O266 86.6(2) . . ?
O207 Mo34 O266 73.6(3) . . ?
O446 Mo34 O266 84.1(2) . . ?
O177 Mo34 O266 70.0(2) . . ?
O317 Mo35 O404 100.9(3) . . ?
O317 Mo35 O393 100.8(3) . . ?
O404 Mo35 O393 71.6(3) . . ?
O317 Mo35 O268 94.0(3) . . ?
O404 Mo35 O268 142.6(3) . . ?
O393 Mo35 O268 72.0(2) . . ?
O317 Mo35 O324 93.0(3) . . ?
O404 Mo35 O324 71.8(3) . . ?
O393 Mo35 O324 142.6(3) . . ?
O268 Mo35 O324 141.8(2) . . ?
O317 Mo35 O137 97.9(3) . . ?
O404 Mo35 O137 138.9(2) . . ?
O393 Mo35 O137 139.3(2) . . ?
O268 Mo35 O137 70.9(2) . . ?
O324 Mo35 O137 71.0(2) . . ?
O317 Mo35 O314 172.4(3) . . ?
O404 Mo35 O314 84.9(3) . . ?
O393 Mo35 O314 85.8(3) . . ?
O268 Mo35 O314 84.1(2) . . ?
O324 Mo35 O314 84.0(2) . . ?
O137 Mo35 O314 74.5(2) . . ?
O317 Mo35 M3T 88.0(4) . . ?
O404 Mo35 M3T 37.8(3) . . ?
O393 Mo35 M3T 39.3(3) . . ?
O268 Mo35 M3T 110.0(3) . . ?
O324 Mo35 M3T 107.7(3) . . ?
O137 Mo35 M3T 174.0(3) . . ?
O314 Mo35 M3T 99.6(3) . . ?
O308 Mo36 O377 103.8(4) . . ?
O308 Mo36 O117 100.9(3) . . ?
O377 Mo36 O117 105.9(3) . . ?
O308 Mo36 O280 97.0(3) . . ?
O377 Mo36 O280 88.8(3) . . ?
O117 Mo36 O280 153.2(3) . . ?
O308 Mo36 O302 93.8(3) . . ?
O377 Mo36 O302 152.7(3) . . ?
O117 Mo36 O302 90.8(3) . . ?
O280 Mo36 O302 68.2(2) . . ?
O308 Mo36 O367 171.6(3) . . ?
O377 Mo36 O367 83.9(4) . . ?
O117 Mo36 O367 79.9(3) . . ?
O280 Mo36 O367 79.5(3) . . ?
O302 Mo36 O367 77.9(3) . . ?
O327 Mo37 O93 103.8(3) . . ?
O327 Mo37 O266 106.1(3) . . ?
O93 Mo37 O266 97.7(3) . . ?
O327 Mo37 O225 105.0(3) . . ?
O93 Mo37 O225 98.4(3) . . ?
O266 Mo37 O225 140.2(3) . . ?
O327 Mo37 O177 97.9(3) . . ?
O93 Mo37 O177 158.3(3) . . ?
O266 Mo37 O177 75.9(2) . . ?
O225 Mo37 O177 75.7(2) . . ?
O327 Mo37 O263 177.0(3) . . ?
O93 Mo37 O263 73.2(3) . . ?
O266 Mo37 O263 75.0(2) . . ?
O225 Mo37 O263 75.3(2) . . ?
O177 Mo37 O263 85.0(2) . . ?
O433 Mo38 O375 101.5(4) . . ?
O433 Mo38 O369 100.1(4) . . ?
O375 Mo38 O369 105.9(3) . . ?
O433 Mo38 O341 94.9(3) . 2_576 ?
O375 Mo38 O341 154.6(3) . 2_576 ?
O369 Mo38 O341 90.0(3) . 2_576 ?
O433 Mo38 O153 96.9(3) . 2_576 ?
O375 Mo38 O153 89.6(3) . 2_576 ?
O369 Mo38 O153 154.1(3) . 2_576 ?
O341 Mo38 O153 69.1(2) 2_576 2_576 ?
O433 Mo38 O319 176.0(3) . . ?
O375 Mo38 O319 81.9(3) . . ?
O369 Mo38 O319 80.9(3) . . ?
O341 Mo38 O319 81.2(3) 2_576 . ?
O153 Mo38 O319 80.9(2) 2_576 . ?
O416 Mo39 O342 104.9(4) . . ?
O416 Mo39 O148 98.3(3) . 2_667 ?
O342 Mo39 O148 99.4(3) . 2_667 ?
O416 Mo39 O288 96.1(3) . . ?
O342 Mo39 O288 92.0(3) . . ?
O148 Mo39 O288 158.6(3) 2_667 . ?
O416 Mo39 O410 164.0(4) . . ?
O342 Mo39 O410 90.6(4) . . ?
O148 Mo39 O410 82.8(3) 2_667 . ?
O288 Mo39 O410 79.0(3) . . ?
O416 Mo39 O360 88.9(3) . . ?
O342 Mo39 O360 164.9(4) . . ?
O148 Mo39 O360 84.5(2) 2_667 . ?
O288 Mo39 O360 80.1(2) . . ?
O410 Mo39 O360 75.3(3) . . ?
O533 Mo40 O538 113.9(11) . . ?
O533 Mo40 O537 110.6(9) . . ?
O538 Mo40 O537 115.2(9) . . ?
O533 Mo40 O536 83.6(12) . . ?
O538 Mo40 O536 81.0(13) . . ?
O537 Mo40 O536 148.6(16) . . ?
O533 Mo40 O513 149.5(9) . . ?
O538 Mo40 O513 84.9(8) . . ?
O537 Mo40 O513 79.1(8) . . ?
O536 Mo40 O513 75.7(13) . . ?
O533 Mo40 O453 79.9(5) . . ?
O538 Mo40 O453 146.7(10) . . ?
O537 Mo40 O453 84.5(8) . . ?
O536 Mo40 O453 70.2(12) . . ?
O513 Mo40 O453 72.2(6) . . ?
O515 Mo41 O502 97.1(7) . . ?
O515 Mo41 O270 98.1(6) . . ?
O502 Mo41 O270 100.5(6) . . ?
O515 Mo41 O467 97.3(6) . . ?
O502 Mo41 O467 95.6(5) . . ?
O270 Mo41 O467 156.1(4) . . ?
O515 Mo41 O215 173.6(6) . 2_667 ?
O502 Mo41 O215 89.2(5) . 2_667 ?
O270 Mo41 O215 81.8(3) . 2_667 ?
O467 Mo41 O215 80.9(3) . 2_667 ?
O515 Mo41 O503 95.9(7) . . ?
O502 Mo41 O503 166.6(6) . . ?
O270 Mo41 O503 80.9(5) . . ?
O467 Mo41 O503 79.5(5) . . ?
O215 Mo41 O503 77.8(5) 2_667 . ?
O464 Mo42 O419 100.3(5) . . ?
O464 Mo42 O504 93.9(5) . . ?
O419 Mo42 O504 165.8(4) . . ?
O464 Mo42 O519 95.3(6) . . ?
O419 Mo42 O519 91.3(5) . . ?
O504 Mo42 O519 86.9(5) . . ?
O464 Mo42 O508 95.1(5) . . ?
O419 Mo42 O508 90.9(4) . . ?
O504 Mo42 O508 88.3(5) . . ?
O519 Mo42 O508 168.8(5) . . ?
O464 Mo42 O414 175.7(4) . . ?
O419 Mo42 O414 83.5(3) . . ?
O504 Mo42 O414 82.4(3) . . ?
O519 Mo42 O414 82.5(5) . . ?
O508 Mo42 O414 86.9(4) . . ?
O470 Mo43 O437 104.8(6) . . ?
O470 Mo43 O431 98.6(5) . . ?
O437 Mo43 O431 99.6(5) . . ?
O470 Mo43 O472 93.3(5) . 2_576 ?
O437 Mo43 O472 98.2(5) . 2_576 ?
O431 Mo43 O472 155.3(5) . 2_576 ?
O470 Mo43 O455 162.4(5) . . ?
O437 Mo43 O455 92.2(5) . . ?
O431 Mo43 O455 82.7(3) . . ?
O472 Mo43 O455 79.6(4) 2_576 . ?
O470 Mo43 O436 87.4(6) . . ?
O437 Mo43 O436 167.5(5) . . ?
O431 Mo43 O436 80.7(5) . . ?
O472 Mo43 O436 78.3(5) 2_576 . ?
O455 Mo43 O436 75.4(4) . . ?
O530 Mo44 O484 96.8(6) . . ?
O530 Mo44 O383 100.6(5) . . ?
O484 Mo44 O383 99.9(4) . . ?
O530 Mo44 O483 98.5(5) . . ?
O484 Mo44 O483 94.8(5) . . ?
O383 Mo44 O483 154.2(4) . . ?
O530 Mo44 O425 96.0(5) . . ?
O484 Mo44 O425 166.3(5) . . ?
O383 Mo44 O425 82.2(3) . . ?
O483 Mo44 O425 78.7(4) . . ?
O530 Mo44 O457 167.0(5) . . ?
O484 Mo44 O457 95.0(6) . . ?
O383 Mo44 O457 82.4(5) . . ?
O483 Mo44 O457 75.3(5) . . ?
O425 Mo44 O457 71.8(4) . . ?
O490 Mo45 O528 103.0(6) . . ?
O490 Mo45 O442 99.5(5) . . ?
O528 Mo45 O442 98.4(5) . . ?
O490 Mo45 O489 93.1(5) . . ?
O528 Mo45 O489 97.0(5) . . ?
O442 Mo45 O489 157.4(4) . . ?
O490 Mo45 O415 165.9(5) . . ?
O528 Mo45 O415 90.2(5) . . ?
O442 Mo45 O415 83.2(3) . . ?
O489 Mo45 O415 80.3(3) . . ?
O490 Mo45 O492 92.3(5) . . ?
O528 Mo45 O492 164.2(5) . . ?
O442 Mo45 O492 82.8(4) . . ?
O489 Mo45 O492 78.0(4) . . ?
O415 Mo45 O492 74.3(4) . . ?
O527 Mo46 O526 105.8(6) . . ?
O527 Mo46 O444 99.8(5) . . ?
O526 Mo46 O444 100.7(5) . . ?
O527 Mo46 O405 94.2(5) . . ?
O526 Mo46 O405 90.6(4) . . ?
O444 Mo46 O405 158.8(4) . . ?
O527 Mo46 O318 93.0(5) . . ?
O526 Mo46 O318 159.7(5) . . ?
O444 Mo46 O318 83.0(3) . . ?
O405 Mo46 O318 80.4(3) . . ?
O527 Mo46 O520 164.4(5) . . ?
O526 Mo46 O520 88.4(5) . . ?
O444 Mo46 O520 83.2(4) . . ?
O405 Mo46 O520 79.2(4) . . ?
O318 Mo46 O520 72.1(4) . . ?
O517 Mo47 O521 105.2(6) . . ?
O517 Mo47 O444 98.7(5) . . ?
O521 Mo47 O444 99.4(5) . . ?
O517 Mo47 O374 95.5(5) . . ?
O521 Mo47 O374 93.7(5) . . ?
O444 Mo47 O374 157.5(4) . . ?
O517 Mo47 O343 93.8(5) . . ?
O521 Mo47 O343 160.7(5) . . ?
O444 Mo47 O343 81.1(3) . . ?
O374 Mo47 O343 80.5(3) . . ?
O517 Mo47 O516 165.7(5) . . ?
O521 Mo47 O516 88.0(5) . . ?
O444 Mo47 O516 84.2(4) . . ?
O374 Mo47 O516 78.0(4) . . ?
O343 Mo47 O516 72.8(4) . . ?
O541 Mo48 O476 104.4(7) . . ?
O541 Mo48 O473 93.8(6) . . ?
O476 Mo48 O473 92.8(6) . . ?
O541 Mo48 O739 86.1(7) . . ?
O476 Mo48 O739 104.6(7) . . ?
O473 Mo48 O739 162.0(6) . . ?
O541 Mo48 O468 91.3(6) . . ?
O476 Mo48 O468 163.4(6) . . ?
O473 Mo48 O468 80.4(4) . . ?
O739 Mo48 O468 81.6(5) . . ?
O541 Mo48 O474 167.5(7) . . ?
O476 Mo48 O474 86.3(7) . . ?
O473 Mo48 O474 78.9(6) . . ?
O739 Mo48 O474 97.6(7) . . ?
O468 Mo48 O474 77.6(6) . . ?
O30 Mo51 O9 103.9(2) . . ?
O30 Mo51 O1 101.7(2) . . ?
O9 Mo51 O1 88.2(2) . . ?
O30 Mo51 O100 102.6(2) . . ?
O9 Mo51 O100 87.5(2) . . ?
O1 Mo51 O100 155.7(2) . . ?
O30 Mo51 O3 98.0(2) . . ?
O9 Mo51 O3 158.0(2) . . ?
O1 Mo51 O3 88.2(2) . . ?
O100 Mo51 O3 86.9(2) . . ?
O30 Mo51 O80 167.4(2) . . ?
O9 Mo51 O80 88.0(2) . . ?
O1 Mo51 O80 74.22(18) . . ?
O100 Mo51 O80 81.69(18) . . ?
O3 Mo51 O80 70.19(19) . . ?
O140 Mo52 O119 100.9(2) . . ?
O140 Mo52 O33 102.5(2) . . ?
O119 Mo52 O33 71.8(2) . . ?
O140 Mo52 O79 93.2(2) . . ?
O119 Mo52 O79 142.2(2) . . ?
O33 Mo52 O79 70.98(19) . . ?
O140 Mo52 O13 93.6(2) . . ?
O119 Mo52 O13 71.45(19) . . ?
O33 Mo52 O13 141.99(19) . . ?
O79 Mo52 O13 142.84(19) . . ?
O140 Mo52 O29 96.4(2) . . ?
O119 Mo52 O29 139.58(19) . . ?
O33 Mo52 O29 138.7(2) . . ?
O79 Mo52 O29 71.67(18) . . ?
O13 Mo52 O29 71.28(18) . . ?
O140 Mo52 O20 170.7(2) . . ?
O119 Mo52 O20 86.55(19) . . ?
O33 Mo52 O20 85.06(19) . . ?
O79 Mo52 O20 84.00(19) . . ?
O13 Mo52 O20 83.46(19) . . ?
O29 Mo52 O20 74.23(18) . . ?
O18 Mo53 O11 104.8(2) . . ?
O18 Mo53 O5 101.2(2) . 2_667 ?
O11 Mo53 O5 88.8(2) . 2_667 ?
O18 Mo53 O132 101.8(2) . . ?
O11 Mo53 O132 87.0(2) . . ?
O5 Mo53 O132 156.8(2) 2_667 . ?
O18 Mo53 O76 97.7(2) . . ?
O11 Mo53 O76 157.4(2) . . ?
O5 Mo53 O76 88.3(2) 2_667 . ?
O132 Mo53 O76 86.9(2) . . ?
O18 Mo53 O125 167.3(2) . 2_667 ?
O11 Mo53 O125 87.28(19) . 2_667 ?
O5 Mo53 O125 74.63(18) 2_667 2_667 ?
O132 Mo53 O125 82.42(19) . 2_667 ?
O76 Mo53 O125 70.39(18) . 2_667 ?
O2 Mo54 O11 103.8(2) . . ?
O2 Mo54 O37 102.6(2) . . ?
O11 Mo54 O37 99.0(2) . . ?
O2 Mo54 O42 105.0(2) . . ?
O11 Mo54 O42 87.4(2) . . ?
O37 Mo54 O42 149.2(2) . . ?
O2 Mo54 O4 95.4(2) . . ?
O11 Mo54 O4 154.9(2) . . ?
O37 Mo54 O4 92.2(2) . . ?
O42 Mo54 O4 72.0(2) . . ?
O2 Mo54 O8 167.8(2) . . ?
O11 Mo54 O8 88.15(19) . . ?
O37 Mo54 O8 72.77(18) . . ?
O42 Mo54 O8 77.39(18) . . ?
O4 Mo54 O8 73.82(17) . . ?
O99 Mo55 O9 102.9(2) . . ?
O99 Mo55 O78 103.5(2) . . ?
O9 Mo55 O78 99.2(2) . . ?
O99 Mo55 O68 105.2(2) . . ?
O9 Mo55 O68 87.5(2) . . ?
O78 Mo55 O68 148.2(2) . . ?
O99 Mo55 O23 95.4(2) . . ?
O9 Mo55 O23 155.4(2) . . ?
O78 Mo55 O23 92.3(2) . . ?
O68 Mo55 O23 71.8(2) . . ?
O99 Mo55 O109 167.8(2) . . ?
O9 Mo55 O109 89.16(19) . . ?
O78 Mo55 O109 72.28(19) . . ?
O68 Mo55 O109 76.82(18) . . ?
O23 Mo55 O109 73.61(18) . . ?
O48 Mo56 O50 103.7(2) . . ?
O48 Mo56 O1 101.9(2) . . ?
O50 Mo56 O1 98.6(2) . . ?
O48 Mo56 O104 103.8(2) . . ?
O50 Mo56 O104 87.3(2) . . ?
O1 Mo56 O104 151.4(2) . . ?
O48 Mo56 O36 94.4(2) . . ?
O50 Mo56 O36 155.2(2) . . ?
O1 Mo56 O36 93.8(2) . . ?
O104 Mo56 O36 71.9(2) . . ?
O48 Mo56 O80 167.0(2) . . ?
O50 Mo56 O80 89.02(19) . . ?
O1 Mo56 O80 72.89(19) . . ?
O104 Mo56 O80 79.26(19) . . ?
O36 Mo56 O80 74.30(17) . . ?
O187 Mo57 O126 102.9(2) . . ?
O187 Mo57 O74 103.7(2) . . ?
O126 Mo57 O74 98.9(2) . . ?
O187 Mo57 O12 104.6(2) . . ?
O126 Mo57 O12 87.4(2) . . ?
O74 Mo57 O12 148.9(2) . . ?
O187 Mo57 O36 96.5(2) . . ?
O126 Mo57 O36 155.0(2) . . ?
O74 Mo57 O36 91.5(2) . . ?
O12 Mo57 O36 72.5(2) . . ?
O187 Mo57 O21 168.9(2) . . ?
O126 Mo57 O21 88.1(2) . . ?
O74 Mo57 O21 72.42(18) . . ?
O12 Mo57 O21 77.38(18) . . ?
O36 Mo57 O21 73.45(18) . . ?
O39 Mo58 O168 103.2(2) . . ?
O39 Mo58 O10 103.4(2) . . ?
O168 Mo58 O10 98.1(2) . . ?
O39 Mo58 O79 105.3(2) . . ?
O168 Mo58 O79 87.9(2) . . ?
O10 Mo58 O79 148.5(2) . . ?
O39 Mo58 O29 96.4(2) . . ?
O168 Mo58 O29 155.4(2) . . ?
O10 Mo58 O29 91.4(2) . . ?
O79 Mo58 O29 72.60(18) . . ?
O39 Mo58 O6 168.6(2) . . ?
O168 Mo58 O6 87.9(2) . . ?
O10 Mo58 O6 72.09(19) . . ?
O79 Mo58 O6 77.28(18) . . ?
O29 Mo58 O6 73.52(18) . . ?
O301 Mo59 O54 104.1(2) . . ?
O301 Mo59 O81 98.9(3) . . ?
O54 Mo59 O81 89.7(2) . . ?
O301 Mo59 O122 101.6(3) . . ?
O54 Mo59 O122 87.0(2) . . ?
O81 Mo59 O122 159.4(2) . . ?
O301 Mo59 O7 99.6(2) . . ?
O54 Mo59 O7 156.2(2) . . ?
O81 Mo59 O7 89.0(2) . . ?
O122 Mo59 O7 86.0(2) . . ?
O301 Mo59 O17 167.4(2) . . ?
O54 Mo59 O17 86.8(2) . . ?
O81 Mo59 O17 74.6(2) . . ?
O122 Mo59 O17 85.0(2) . . ?
O7 Mo59 O17 69.98(19) . . ?
O531 Mo60 O532 103.9(7) . . ?
O531 Mo60 O739 85.1(8) . . ?
O532 Mo60 O739 104.8(7) . . ?
O531 Mo60 O480 101.5(7) . . ?
O532 Mo60 O480 90.0(6) . . ?
O739 Mo60 O480 162.0(6) . . ?
O531 Mo60 O479 90.6(6) . . ?
O532 Mo60 O479 164.4(6) . . ?
O739 Mo60 O479 81.7(6) . . ?
O480 Mo60 O479 81.5(4) . . ?
O531 Mo60 O475 167.0(7) . . ?
O532 Mo60 O475 88.3(7) . . ?
O739 Mo60 O475 96.3(7) . . ?
O480 Mo60 O475 73.6(6) . . ?
O479 Mo60 O475 76.8(5) . . ?
O534 Mo61 O452 100.5(6) . . ?
O534 Mo61 O533 98.1(6) . . ?
O452 Mo61 O533 97.7(7) . . ?
O534 Mo61 O392 94.1(6) . . ?
O452 Mo61 O392 97.7(6) . . ?
O533 Mo61 O392 158.2(6) . . ?
O534 Mo61 O535 87.0(6) . . ?
O452 Mo61 O535 172.1(6) . . ?
O533 Mo61 O535 83.8(6) . . ?
O392 Mo61 O535 78.8(5) . . ?
O534 Mo61 O356 166.1(7) . . ?
O452 Mo61 O356 93.1(5) . . ?
O533 Mo61 O356 83.0(5) . . ?
O392 Mo61 O356 80.9(3) . . ?
O535 Mo61 O356 79.3(5) . . ?
O402 M3I O364 91.4(6) . . ?
O402 M3I O270 88.8(7) . . ?
O364 M3I O270 144.1(10) . . ?
O402 M3I O194 143.3(10) . . ?
O364 M3I O194 80.1(5) . . ?
O270 M3I O194 78.6(5) . . ?
O461 M3L O274 95.7(8) . . ?
O461 M3L O421 89.0(8) . . ?
O274 M3L O421 153.6(10) . . ?
O461 M3L O378 153.1(10) . . ?
O274 M3L O378 85.0(7) . . ?
O421 M3L O378 79.4(6) . . ?
O461 M3L O426 77.4(7) . . ?
O274 M3L O426 80.1(7) . . ?
O421 M3L O426 75.6(6) . . ?
O378 M3L O426 76.2(6) . . ?
O461 M3L C31 114.3(9) . . ?
O274 M3L C31 128.5(9) . . ?
O421 M3L C31 71.5(7) . . ?
O378 M3L C31 85.1(7) . . ?
O426 M3L C31 144.5(8) . . ?
O443 M3R O409 84.0(6) . . ?
O443 M3R O395 86.6(7) . . ?
O409 M3R O395 133.7(10) . . ?
O443 M3R C81 116.9(11) . . ?
O409 M3R C81 150.7(10) . . ?
O395 M3R C81 71.2(9) . . ?
O443 M3R O358 138.9(11) . . ?
O409 M3R O358 78.9(5) . . ?
O395 M3R O358 79.2(5) . . ?
C81 M3R O358 94.7(11) . . ?
O486 M3S O396 89.8(8) . . ?
O486 M3S C11 113.4(9) . . ?
O396 M3S C11 150.7(9) . . ?
O486 M3S O383 82.5(7) . . ?
O396 M3S O383 127.4(9) . . ?
C11 M3S O383 75.5(7) . . ?
O486 M3S O328 134.2(10) . . ?
O396 M3S O328 78.3(6) . . ?
C11 M3S O328 95.8(7) . . ?
O383 M3S O328 71.1(5) . . ?
O486 M3S M44 85.3(10) . . ?
O396 M3S M44 174.6(11) . . ?
C11 M3S M44 34.6(9) . . ?
O383 M3S M44 49.6(8) . . ?
O328 M3S M44 103.5(8) . . ?
O783 M3T O780 101.4(12) . . ?
O783 M3T O404 150.9(12) . . ?
O780 M3T O404 87.6(9) . . ?
O783 M3T O393 87.3(9) . . ?
O780 M3T O393 149.3(11) . . ?
O404 M3T O393 72.2(5) . . ?
O783 M3T O480 93.2(10) . . ?
O780 M3T O480 19.3(8) . . ?
O404 M3T O480 86.4(6) . . ?
O393 M3T O480 132.7(8) . . ?
O783 M3T O483 20.2(7) . . ?
O780 M3T O483 96.3(10) . . ?
O404 M3T O483 132.3(8) . . ?
O393 M3T O483 81.8(6) . . ?
O480 M3T O483 82.9(7) . . ?
O783 M3T Mo35 126.3(9) . . ?
O780 M3T Mo35 126.2(9) . . ?
O404 M3T Mo35 38.6(3) . . ?
O393 M3T Mo35 39.1(3) . . ?
O480 M3T Mo35 123.1(6) . . ?
O483 M3T Mo35 119.4(6) . . ?
O825 M3U O432 95.2(9) . . ?
O825 M3U O395 98.7(9) . . ?
O432 M3U O395 143.8(5) . . ?
O825 M3U O380 161.8(10) . . ?
O432 M3U O380 81.9(4) . . ?
O395 M3U O380 74.6(4) . . ?
O825 M3U C81 106.8(11) . . ?
O432 M3U C81 140.6(8) . . ?
O395 M3U C81 65.2(8) . . ?
O380 M3U C81 86.0(9) . . ?
O799 M3W O756 92.8(10) . . ?
O799 M3W O421 91.5(8) . . ?
O756 M3W O421 129.6(8) . . ?
O799 M3W O370 155.4(10) . . ?
O756 M3W O370 78.8(6) . . ?
O421 M3W O370 76.9(4) . . ?
O799 M3W C31 105.1(9) . . ?
O756 M3W C31 150.6(8) . . ?
O421 M3W C31 74.0(6) . . ?
O370 M3W C31 92.7(6) . . ?
O523 M3X O413 97.4(5) . . ?
O523 M3X O387 92.4(5) . . ?
O413 M3X O387 145.4(5) . . ?
O523 M3X O303 146.0(5) . . ?
O413 M3X O303 78.8(3) . . ?
O387 M3X O303 74.7(3) . . ?
O523 M3X C91 127.2(6) . . ?
O413 M3X C91 78.7(5) . . ?
O387 M3X C91 120.4(6) . . ?
O303 M3X C91 85.5(5) . . ?
O523 M3X O398 76.0(5) . . ?
O413 M3X O398 75.3(4) . . ?
O387 M3X O398 75.1(4) . . ?
O303 M3X O398 70.3(3) . . ?
C91 M3X O398 147.2(5) . . ?
O342 M39 O288 95.3(5) . . ?
O342 M39 O148 91.0(5) . 2_667 ?
O288 M39 O148 152.1(7) . 2_667 ?
O342 M39 O360 152.5(6) . . ?
O288 M39 O360 82.3(5) . . ?
O148 M39 O360 79.7(4) 2_667 . ?
O342 M39 O416 79.4(5) . . ?
O288 M39 O416 80.0(5) . . ?
O148 M39 O416 74.5(4) 2_667 . ?
O360 M39 O416 73.2(4) . . ?
O342 M39 C101 116.0(6) . . ?
O288 M39 C101 123.6(6) . . ?
O148 M39 C101 76.7(4) 2_667 . ?
O360 M39 C101 87.2(4) . . ?
O416 M39 C101 147.5(5) . . ?
O538 M40 O813 96.0(8) . . ?
O538 M40 O533 98.5(7) . . ?
O813 M40 O533 162.4(8) . . ?
O538 M40 O836 97.5(10) . . ?
O813 M40 O836 76.2(11) . . ?
O533 M40 O836 92.2(9) . . ?
O538 M40 O453 178.2(9) . . ?
O813 M40 O453 84.8(6) . . ?
O533 M40 O453 80.9(4) . . ?
O836 M40 O453 84.3(9) . . ?
O538 M40 O537 95.9(8) . . ?
O813 M40 O537 101.2(9) . . ?
O533 M40 O537 87.1(7) . . ?
O836 M40 O537 166.6(9) . . ?
O453 M40 O537 82.3(7) . . ?
O815 M41 O467 93.5(9) . . ?
O815 M41 O270 95.8(9) . . ?
O467 M41 O270 141.6(6) . . ?
O467 M41 O215 79.8(4) . 2_667 ?
O270 M41 O215 78.3(4) . 2_667 ?
O472 M43 O470 96.5(9) 2_576 . ?
O472 M43 O455 84.5(6) 2_576 . ?
O470 M43 O455 134.8(9) . . ?
O472 M43 O431 138.7(10) 2_576 . ?
O470 M43 O431 78.6(6) . . ?
O455 M43 O431 71.9(4) . . ?
O472 M43 C21 145.6(11) 2_576 . ?
O470 M43 C21 111.9(9) . . ?
O455 M43 C21 88.6(8) . . ?
O431 M43 C21 68.8(8) . . ?
C11 M44 O784 120(2) . . ?
C11 M44 O483 151(2) . . ?
O784 M44 O483 85.9(18) . . ?
C11 M44 O383 80.3(14) . . ?
O784 M44 O383 80.2(15) . . ?
O483 M44 O383 119(2) . . ?
C11 M44 O783 160(2) . . ?
O784 M44 O783 79.3(17) . . ?
O483 M44 O783 15.2(7) . . ?
O383 M44 O783 104.6(17) . . ?
C11 M44 M3S 43.8(10) . . ?
O784 M44 M3S 84.1(14) . . ?
O483 M44 M3S 164(2) . . ?
O383 M44 M3S 46.6(7) . . ?
O783 M44 M3S 149.3(17) . . ?
O405 M46 O444 145.1(7) . . ?
O405 M46 O527 78.1(5) . . ?
O444 M46 O527 73.8(5) . . ?
O405 M46 O318 78.6(5) . . ?
O444 M46 O318 73.9(5) . . ?
O527 M46 O318 73.0(5) . . ?
O516 M47 O521 124.9(9) . . ?
O516 M47 O374 98.5(8) . . ?
O521 M47 O374 97.6(7) . . ?
O516 M47 O444 101.3(7) . . ?
O521 M47 O444 96.4(7) . . ?
O374 M47 O444 142.8(6) . . ?
O516 M47 O343 82.5(7) . . ?
O521 M47 O343 152.7(7) . . ?
O374 M47 O343 77.3(4) . . ?
O444 M47 O343 74.4(4) . . ?
O516 M47 O517 155.5(8) . . ?
O521 M47 O517 79.6(7) . . ?
O374 M47 O517 75.5(5) . . ?
O444 M47 O517 73.4(5) . . ?
O343 M47 O517 73.1(4) . . ?
O516 M47 C71 24.2(6) . . ?
O521 M47 C71 125.8(8) . . ?
O374 M47 C71 119.8(7) . . ?
O444 M47 C71 77.2(6) . . ?
O343 M47 C71 78.0(6) . . ?
O517 M47 C71 143.2(7) . . ?
O476 M48 O473 91.0(7) . . ?
O476 M48 O439 86.3(8) . . ?
O473 M48 O439 143.8(9) . . ?
O476 M48 O468 139.8(9) . . ?
O473 M48 O468 80.6(5) . . ?
O439 M48 O468 78.4(6) . . ?
O476 M48 C61 117.1(10) . . ?
O473 M48 C61 143.7(10) . . ?
O439 M48 C61 65.4(9) . . ?
O468 M48 C61 90.0(10) . . ?
O475 M60 O532 129.4(13) . . ?
O475 M60 O480 104.9(13) . . ?
O532 M60 O480 91.9(8) . . ?
O475 M60 O439 98.8(11) . . ?
O532 M60 O439 89.4(9) . . ?
O480 M60 O439 147.9(13) . . ?
O475 M60 O780 122.3(14) . . ?
O532 M60 O780 85.5(10) . . ?
O480 M60 O780 18.9(7) . . ?
O439 M60 O780 129.9(14) . . ?
O475 M60 O479 94.3(11) . . ?
O532 M60 O479 136.0(13) . . ?
O480 M60 O479 80.0(5) . . ?
O439 M60 O479 77.0(6) . . ?
O780 M60 O479 72.9(8) . . ?
O475 M60 C61 34.0(10) . . ?
O532 M60 C61 123.7(10) . . ?
O480 M60 C61 136.4(12) . . ?
O439 M60 C61 64.9(9) . . ?
O780 M60 C61 149.6(12) . . ?
O479 M60 C61 88.0(10) . . ?
O534 M61 O452 113.2(14) . . ?
O534 M61 O533 106.6(13) . . ?
O452 M61 O533 105.6(12) . . ?
O534 M61 O392 91.6(10) . . ?
O452 M61 O392 94.8(12) . . ?
O533 M61 O392 143.9(12) . . ?
O534 M61 O535 84.4(10) . . ?
O452 M61 O535 158.1(11) . . ?
O533 M61 O535 80.1(10) . . ?
O392 M61 O535 70.8(7) . . ?
O534 M61 O356 153.9(12) . . ?
O452 M61 O356 89.1(8) . . ?
O533 M61 O356 78.4(8) . . ?
O392 M61 O356 72.4(6) . . ?
O535 M61 O356 71.0(6) . . ?
Mo56 O1 Mo51 121.9(2) . . ?
Mo51 O3 Mo4A 138.2(3) . . ?
Mo51 O3 Mo4Q 110.0(2) . . ?
Mo4A O3 Mo4Q 109.6(2) . . ?
Mo4P O4 Mo54 140.8(3) . . ?
Mo4P O4 Mo4H 102.5(2) . . ?
Mo54 O4 Mo4H 102.6(2) . . ?
Mo4P O4 Mo4T 102.88(19) . . ?
Mo54 O4 Mo4T 103.56(19) . . ?
Mo4H O4 Mo4T 96.57(18) . . ?
Mo4B O5 Mo53 121.9(2) . 2_667 ?
Mo4S O6 Mo4G 102.9(2) . . ?
Mo4S O6 Mo58 107.4(2) . . ?
Mo4G O6 Mo58 88.36(15) . . ?
Mo59 O7 Mo4C 137.6(3) . . ?
Mo59 O7 Mo4T 109.6(2) . . ?
Mo4C O7 Mo4T 111.0(2) . . ?
Mo4T O8 Mo4C 103.1(2) . . ?
Mo4T O8 Mo54 107.7(2) . . ?
Mo4C O8 Mo54 88.81(15) . . ?
Mo55 O9 Mo51 158.0(3) . . ?
Mo58 O10 Mo4G 124.2(3) . . ?
Mo54 O11 Mo53 157.8(3) . . ?
Mo57 O12 Mo4O 108.5(2) . . ?
Mo57 O12 Mo1D 141.8(3) . . ?
Mo4O O12 Mo1D 108.1(2) . . ?
Mo4B O13 Mo52 108.5(2) . . ?
Mo4B O13 Mo4F 143.6(3) . 2_567 ?
Mo52 O13 Mo4F 107.7(2) . 2_567 ?
Mo4I O14 Mo4J 110.8(2) . . ?
Mo4I O14 Mo1S 108.9(2) . . ?
Mo4J O14 Mo1S 140.1(3) . . ?
Mo4M O15 Mo4D 122.8(3) . . ?
Mo4B O16 Mo4C 158.0(3) . 2_667 ?
Mo4T O17 Mo59 103.3(2) . . ?
Mo4T O17 Mo4P 107.5(2) . . ?
Mo59 O17 Mo4P 88.72(17) . . ?
Mo12 O19 Mo17 142.2(3) . . ?
Mo12 O19 Mo1G 102.6(2) . . ?
Mo17 O19 Mo1G 102.3(2) . . ?
Mo12 O19 Mo19 102.6(2) . . ?
Mo17 O19 Mo19 102.7(2) . . ?
Mo1G O19 Mo19 95.8(2) . . ?
Mo4S O20 Mo52 116.2(2) . . ?
Mo4Q O21 Mo4A 103.6(2) . . ?
Mo4Q O21 Mo57 108.2(2) . . ?
Mo4A O21 Mo57 88.53(16) . . ?
Mo1W O22 Mo1V 141.3(3) . . ?
Mo1W O22 Mo30 102.8(2) . . ?
Mo1V O22 Mo30 103.2(3) . . ?
Mo1W O22 Mo2Q 102.5(2) . . ?
Mo1V O22 Mo2Q 102.8(2) . . ?
Mo30 O22 Mo2Q 96.1(2) . . ?
Mo4R O23 Mo55 140.6(3) . . ?
Mo4R O23 Mo4I 103.3(2) . . ?
Mo55 O23 Mo4I 103.1(2) . . ?
Mo4R O23 Mo1B 102.9(2) . . ?
Mo55 O23 Mo1B 103.0(2) . . ?
Mo4I O23 Mo1B 95.64(19) . . ?
Mo4U O24 Mo4M 140.9(3) . . ?
Mo4U O24 Mo1F 102.7(2) . . ?
Mo4M O24 Mo1F 103.1(2) . . ?
Mo4U O24 Mo1Q 103.6(2) . . ?
Mo4M O24 Mo1Q 102.3(2) . . ?
Mo1F O24 Mo1Q 96.25(19) . . ?
Mo4W O26 Mo15 148.9(3) . . ?
Mo4O O27 Mo1H 110.5(2) . . ?
Mo4O O27 Mo31 109.3(3) . . ?
Mo1H O27 Mo31 134.1(3) . . ?
Mo4B O29 Mo58 141.0(2) . . ?
Mo4B O29 Mo52 102.9(2) . . ?
Mo58 O29 Mo52 102.1(2) . . ?
Mo4B O29 Mo4S 102.73(19) . . ?
Mo58 O29 Mo4S 103.9(2) . . ?
Mo52 O29 Mo4S 95.88(18) . . ?
Mo4U O31 Mo4N 123.4(3) . . ?
Mo1B O32 Mo4L 103.2(2) . . ?
Mo1B O32 Mo4R 108.5(2) . . ?
Mo4L O32 Mo4R 89.28(18) . . ?
Mo52 O33 Mo2J 108.7(2) . . ?
Mo52 O33 Mo4K 112.0(2) . . ?
Mo2J O33 Mo4K 138.9(3) . . ?
Mo4P O34 Mo4H 109.2(2) . . ?
Mo4P O34 Mo1C 143.2(3) . . ?
Mo4H O34 Mo1C 107.6(2) . . ?
Mo12 O35 Mo15 123.1(3) . . ?
Mo57 O36 Mo56 140.2(2) . . ?
Mo57 O36 Mo4O 103.2(2) . . ?
Mo56 O36 Mo4O 103.6(2) . . ?
Mo57 O36 Mo4Q 103.6(2) . . ?
Mo56 O36 Mo4Q 102.28(18) . . ?
Mo4O O36 Mo4Q 95.89(17) . . ?
Mo54 O37 Mo4C 123.1(3) . . ?
Mo4X O38 Mo4A 157.4(3) . . ?
Mo1J O40 Mo2B 124.3(3) . . ?
Mo19 O41 Mo4Z 102.8(2) . . ?
Mo19 O41 Mo17 107.0(2) . . ?
Mo4Z O41 Mo17 88.72(17) . . ?
Mo54 O42 Mo4H 108.7(2) . . ?
Mo54 O42 Mo4E 141.7(3) . . ?
Mo4H O42 Mo4E 108.1(2) . . ?
Mo19 O43 Mo15 103.5(2) . . ?
Mo19 O43 Mo12 108.3(2) . . ?
Mo15 O43 Mo12 88.99(18) . . ?
Mo4H O44 Mo4E 110.7(2) . . ?
Mo4H O44 Mo28 109.2(2) . . ?
Mo4E O44 Mo28 139.9(3) . . ?
Mo1I O46 Mo13 141.1(3) 2_576 . ?
Mo1I O46 Mo1N 103.5(3) 2_576 . ?
Mo13 O46 Mo1N 103.0(2) . . ?
Mo1I O46 Mo2K 102.5(2) 2_576 2_576 ?
Mo13 O46 Mo2K 102.6(2) . 2_576 ?
Mo1N O46 Mo2K 95.76(19) . 2_576 ?
Mo1K O47 Mo18 103.2(2) . . ?
Mo1K O47 Mo4X 108.1(2) . . ?
Mo18 O47 Mo4X 89.08(17) . . ?
Mo4V O49 Mo1E 123.4(3) . . ?
Mo56 O50 Mo10 158.8(3) . . ?
Mo1I O52 Mo20 123.3(3) . . ?
Mo19 O53 Mo1G 116.5(3) . . ?
Mo17 O54 Mo59 156.8(3) . . ?
Mo4L O55 Mo10 139.4(3) . . ?
Mo4L O55 Mo1B 109.8(2) . . ?
Mo10 O55 Mo1B 108.7(2) . . ?
Mo17 O57 Mo4Z 123.5(3) . . ?
Mo1K O59 Mo1E 103.3(2) . . ?
Mo1K O59 Mo4V 107.9(2) . . ?
Mo1E O59 Mo4V 88.58(17) . . ?
Mo22 O62 Mo2O 109.1(3) . . ?
Mo22 O62 Mo32 142.6(3) . . ?
Mo2O O62 Mo32 107.8(3) . . ?
Mo18 O63 Mo1E 137.3(3) . . ?
Mo18 O63 Mo1K 110.5(2) . . ?
Mo1E O63 Mo1K 109.9(2) . . ?
Mo13 O65 Mo16 157.9(3) . . ?
Mo4T O66 Mo4H 117.3(2) . . ?
Mo1Q O67 Mo4N 102.9(2) . . ?
Mo1Q O67 Mo4U 107.6(2) . . ?
Mo4N O67 Mo4U 88.56(17) . . ?
Mo55 O68 Mo4I 108.9(2) . . ?
Mo55 O68 Mo4J 140.9(2) . . ?
Mo4I O68 Mo4J 108.5(2) . . ?
Mo1B O69 Mo4I 116.6(3) . . ?
Mo2J O72 Mo2J 180.0 2_567 . ?
Mo57 O74 Mo4A 123.3(3) . . ?
Mo4G O76 Mo53 137.9(2) 2_667 . ?
Mo4G O76 Mo4S 111.0(2) 2_667 2_667 ?
Mo53 O76 Mo4S 109.1(2) . 2_667 ?
Mo11 O77 Mo1J 142.4(3) . . ?
Mo11 O77 Mo1L 103.0(2) . . ?
Mo1J O77 Mo1L 102.6(2) . . ?
Mo11 O77 Mo2I 102.1(2) . . ?
Mo1J O77 Mo2I 102.5(2) . . ?
Mo1L O77 Mo2I 95.4(2) . . ?
Mo55 O78 Mo10 123.0(3) . . ?
Mo58 O79 Mo52 108.5(2) . . ?
Mo58 O79 Mo4K 142.7(3) . . ?
Mo52 O79 Mo4K 108.3(2) . . ?
Mo4Q O80 Mo51 103.2(2) . . ?
Mo4Q O80 Mo56 108.9(2) . . ?
Mo51 O80 Mo56 89.65(16) . . ?
Mo4P O81 Mo59 123.3(3) . . ?
Mo4X O82 Mo4V 141.3(3) . . ?
Mo4X O82 Mo1A 103.7(2) . . ?
Mo4V O82 Mo1A 103.2(2) . . ?
Mo4X O82 Mo1K 102.8(2) . . ?
Mo4V O82 Mo1K 101.76(19) . . ?
Mo1A O82 Mo1K 95.62(19) . . ?
Mo26 O83 Mo1X 137.3(3) . . ?
Mo26 O83 Mo2C 109.8(3) . . ?
Mo1X O83 Mo2C 110.9(2) . . ?
Mo4Z O84 Mo15 137.4(3) . . ?
Mo4Z O84 Mo19 111.5(2) . . ?
Mo15 O84 Mo19 109.8(2) . . ?
Mo2Q O85 Mo23 103.0(2) . . ?
Mo2Q O85 Mo1W 107.6(3) . . ?
Mo23 O85 Mo1W 88.4(2) . . ?
Mo4Q O86 Mo4O 117.1(2) . . ?
Mo1A O89 Mo2X 110.3(3) . . ?
Mo1A O89 Mo1M 110.9(2) . . ?
Mo2X O89 Mo1M 136.5(3) . . ?
Mo4M O90 Mo4G 157.3(3) . . ?
Mo4H O91 Mo28 110.3(3) . . ?
Mo4H O91 Mo1C 110.8(3) . . ?
Mo28 O91 Mo1C 133.1(3) . . ?
Mo4X O92 Mo18 123.2(3) . . ?
Mo37 O93 Mo2O 116.9(3) . . ?
Mo1P O95 Mo4A 149.7(3) . . ?
Mo29 O96 Mo4G 149.9(3) . . ?
Mo1H O97 Mo10 148.0(3) . . ?
Mo4P O98 Mo4Z 156.9(3) . . ?
Mo4J O100 Mo51 146.8(3) . . ?
Mo2W O101 Mo25 103.2(3) . . ?
Mo2W O101 Mo27 107.5(2) . . ?
Mo25 O101 Mo27 88.59(18) . . ?
Mo11 O102 Mo14 158.5(3) . . ?
Mo56 O104 Mo4O 110.1(2) . . ?
Mo56 O104 Mo1H 141.4(3) . . ?
Mo4O O104 Mo1H 107.1(2) . . ?
Mo2H O105 Mo14 123.0(3) . . ?
Mo4R O106 Mo4I 109.3(2) . . ?
Mo4R O106 Mo4W 142.3(3) . . ?
Mo4I O106 Mo4W 107.9(2) . . ?
Mo2I O107 Mo1Z 104.0(2) . . ?
Mo2I O107 Mo11 108.4(2) . . ?
Mo1Z O107 Mo11 89.35(19) . . ?
Mo1L O108 Mo1O 110.5(3) . . ?
Mo1L O108 Mo2R 109.0(2) . . ?
Mo1O O108 Mo2R 135.5(3) . . ?
Mo1B O109 Mo10 103.4(2) . . ?
Mo1B O109 Mo55 108.5(2) . . ?
Mo10 O109 Mo55 88.72(17) . . ?
Mo2V O112 Mo2O 109.7(3) . . ?
Mo2V O112 Mo2P 142.3(3) . . ?
Mo2O O112 Mo2P 107.8(3) . . ?
Mo1Q O114 Mo4D 103.3(2) . . ?
Mo1Q O114 Mo4M 107.6(2) . . ?
Mo4D O114 Mo4M 88.82(16) . . ?
Mo2K O116 Mo20 103.0(3) . . ?
Mo2K O116 Mo1I 107.7(2) . . ?
Mo20 O116 Mo1I 88.56(18) . . ?
Mo36 O117 Mo20 148.4(4) . . ?
Mo52 O119 Mo2J 108.5(2) . . ?
Mo52 O119 Mo4F 111.8(2) . 2_567 ?
Mo2J O119 Mo4F 139.0(2) . 2_567 ?
Mo2F O120 Mo24 123.4(3) . . ?
Mo4Y O122 Mo59 150.0(3) . . ?
Mo21 O123 Mo4L 148.3(3) . . ?
Mo4S O125 Mo53 103.5(2) . 2_667 ?
Mo4S O125 Mo4B 108.3(2) . . ?
Mo53 O125 Mo4B 89.15(16) 2_667 . ?
Mo57 O126 Mo18 158.0(3) . . ?
Mo4R O127 Mo15 157.6(3) . . ?
Mo4I O131 Mo1S 110.1(2) . . ?
Mo4I O131 Mo4W 110.6(3) . . ?
Mo1S O131 Mo4W 134.8(3) . . ?
Mo4E O132 Mo53 147.9(3) . . ?
Mo1K O135 Mo1A 116.4(3) . . ?
Mo4V O136 Mo4N 158.4(3) . . ?
Mo2F O137 Mo2H 141.0(3) . . ?
Mo2F O137 Mo35 103.2(2) . . ?
Mo2H O137 Mo35 103.4(2) . . ?
Mo2F O137 Mo2Z 102.7(2) . . ?
Mo2H O137 Mo2Z 102.5(2) . . ?
Mo35 O137 Mo2Z 95.5(2) . . ?
Mo16 O138 Mo23 137.4(3) . . ?
Mo16 O138 Mo2Q 110.1(3) . . ?
Mo23 O138 Mo2Q 110.2(3) . . ?
Mo1G O139 Mo2S 110.0(2) . . ?
Mo1G O139 Mo4Y 110.6(2) . . ?
Mo2S O139 Mo4Y 134.5(3) . . ?
Mo11 O141 Mo1Z 121.7(3) . . ?
Mo2H O142 Mo1Z 158.3(4) . . ?
Mo4F O144 Mo4C 148.0(3) . 1_455 ?
Mo2Z O146 Mo24 102.8(2) . . ?
Mo2Z O146 Mo2F 107.5(2) . . ?
Mo24 O146 Mo2F 88.0(2) . . ?
Mo2O O147 Mo3K 109.6(3) . . ?
Mo2O O147 Mo2P 110.4(3) . . ?
Mo3K O147 Mo2P 135.9(4) . . ?
Mo39 O148 Mo1R 137.5(4) 2_667 . ?
Mo39 O148 M39 20.0(3) 2_667 2_667 ?
Mo1R O148 M39 123.5(5) . 2_667 ?
Mo1N O153 Mo38 109.2(3) . 2_576 ?
Mo1N O153 Mo1U 109.8(3) . . ?
Mo38 O153 Mo1U 136.2(3) 2_576 . ?
Mo4D O155 Mo4N 137.4(3) . . ?
Mo4D O155 Mo1Q 110.1(2) . . ?
Mo4N O155 Mo1Q 110.1(2) . . ?
Mo4K O157 Mo4D 147.8(3) . . ?
Mo2A O160 Mo2M 141.4(3) . . ?
Mo2A O160 Mo2D 103.0(2) . . ?
Mo2M O160 Mo2D 102.7(3) . . ?
Mo2A O160 Mo2C 103.2(2) . . ?
Mo2M O160 Mo2C 102.1(2) . . ?
Mo2D O160 Mo2C 96.3(2) . . ?
Mo1D O161 Mo18 146.7(3) . . ?
Mo1G O163 Mo2S 109.8(2) . . ?
Mo1G O163 Mo21 110.8(3) . . ?
Mo2S O163 Mo21 136.9(3) . . ?
Mo12 O164 Mo1G 109.6(2) . . ?
Mo12 O164 Mo21 141.4(3) . . ?
Mo1G O164 Mo21 108.2(2) . . ?
Mo4X O167 Mo1A 109.4(2) . . ?
Mo4X O167 Mo1P 141.7(3) . . ?
Mo1A O167 Mo1P 108.1(2) . . ?
Mo58 O168 Mo4D 157.6(3) . . ?
Mo1J O169 Mo1L 109.8(3) . . ?
Mo1J O169 Mo2N 141.1(3) . . ?
Mo1L O169 Mo2N 108.6(2) . . ?
Mo2M O171 Mo26 122.7(3) . . ?
Mo4V O172 Mo1A 109.0(2) . . ?
Mo4V O172 Mo1M 142.1(3) . . ?
Mo1A O172 Mo1M 108.3(2) . . ?
Mo22 O173 Mo23 158.0(4) . . ?
Mo4R O176 Mo4L 123.1(3) . . ?
Mo2U O177 Mo34 135.9(3) . . ?
Mo2U O177 Mo37 111.4(3) . . ?
Mo34 O177 Mo37 110.2(3) . . ?
Mo2Q O178 Mo16 103.5(2) . . ?
Mo2Q O178 Mo1V 108.5(3) . . ?
Mo16 O178 Mo1V 89.23(18) . . ?
Mo2K O179 Mo1N 118.1(3) . 2_576 ?
Mo2Y O180 Mo25 149.3(4) . . ?
Mo4U O181 Mo1F 108.9(3) . . ?
Mo4U O181 Mo2L 142.1(3) . . ?
Mo1F O181 Mo2L 108.2(3) . . ?
Mo1C O183 Mo4Z 149.9(3) . . ?
Mo25 O184 Mo2T 136.6(3) . . ?
Mo25 O184 Mo2W 111.2(3) . . ?
Mo2T O184 Mo2W 110.4(2) . . ?
Mo2J O185 Mo3N 159.2(3) . . ?
Mo2F O186 Mo34 158.1(4) . . ?
Mo4U O189 Mo1E 158.1(3) . . ?
Mo2Z O191 Mo14 103.3(2) . . ?
Mo2Z O191 Mo2H 108.1(2) . . ?
Mo14 O191 Mo2H 89.1(2) . . ?
Mo1R O192 Mo4K 168.0(4) . 2_567 ?
Mo1J O193 Mo26 157.7(3) . . ?
Mo4E O194 Mo3I 152.0(3) . . ?
Mo4E O194 M3I 154.8(5) . . ?
Mo2P O195 Mo24 149.8(3) . . ?
Mo12 O196 Mo4L 157.2(3) . . ?
Mo1I O198 Mo1N 109.4(3) . 2_576 ?
Mo1I O198 Mo2Y 141.8(3) . . ?
Mo1N O198 Mo2Y 108.5(2) 2_576 . ?
Mo4F O199 Mo1R 155.9(3) . 2_567 ?
Mo2J O200 Mo1R 158.8(3) . . ?
Mo2I O203 Mo1L 117.3(3) . . ?
Mo1Y O204 Mo2B 149.3(4) . . ?
Mo11 O206 Mo1L 108.9(2) . . ?
Mo11 O206 Mo1O 141.4(3) . . ?
Mo1L O206 Mo1O 108.6(3) . . ?
Mo2V O207 Mo34 123.6(3) . . ?
Mo3N O208 Mo4F 176.1(4) . . ?
Mo33 O211 Mo1X 149.0(3) . . ?
Mo13 O212 Mo1N 109.2(2) . . ?
Mo13 O212 Mo1U 141.0(3) . . ?
Mo1N O212 Mo1U 108.1(2) . . ?
Mo1U O213 Mo3O 152.7(4) . . ?
Mo29 O215 Mo41 156.2(4) . 2_667 ?
Mo29 O215 M41 143.6(5) . 2_667 ?
Mo41 O215 M41 24.3(2) 2_667 2_667 ?
Mo2C O217 Mo1X 103.5(2) . . ?
Mo2C O217 Mo2A 107.4(3) . . ?
Mo1X O217 Mo2A 88.81(19) . . ?
Mo1M O221 Mo4N 149.1(3) . . ?
Mo2Q O222 Mo30 116.8(3) . . ?
Mo2A O223 Mo2D 108.9(3) . . ?
Mo2A O223 Mo3A 141.8(3) . . ?
Mo2D O223 Mo3A 108.8(3) . . ?
Mo2C O224 Mo26 103.3(2) . . ?
Mo2C O224 Mo2M 108.1(2) . . ?
Mo26 O224 Mo2M 89.39(18) . . ?
Mo37 O225 Mo2U 102.8(3) . . ?
Mo37 O225 Mo22 107.4(3) . . ?
Mo2U O225 Mo22 88.5(2) . . ?
Mo1Z O227 Mo2B 137.2(3) . . ?
Mo1Z O227 Mo2I 110.1(2) . . ?
Mo2B O227 Mo2I 110.9(3) . . ?
Mo2N O230 Mo26 148.4(4) . . ?
Mo1F O231 Mo3E 109.5(3) . . ?
Mo1F O231 Mo29 110.5(3) . . ?
Mo3E O231 Mo29 136.8(3) . . ?
Mo22 O232 Mo2U 123.3(4) . . ?
Mo2K O235 Mo1T 103.2(2) . . ?
Mo2K O235 Mo13 108.7(3) . 2_576 ?
Mo1T O235 Mo13 89.09(18) . 2_576 ?
Mo1F O236 Mo3E 109.9(3) . . ?
Mo1F O236 Mo2L 110.7(3) . . ?
Mo3E O236 Mo2L 137.3(3) . . ?
Mo2I O238 Mo2B 103.1(3) . . ?
Mo2I O238 Mo1J 107.4(2) . . ?
Mo2B O238 Mo1J 88.14(18) . . ?
Mo1W O239 Mo30 108.7(3) . . ?
Mo1W O239 Mo3F 142.0(3) . . ?
Mo30 O239 Mo3F 108.4(3) . . ?
Mo27 O242 Mo25 123.2(3) . . ?
Mo30 O244 Mo3P 109.6(3) . . ?
Mo30 O244 Mo3B 111.0(3) . 2_576 ?
Mo3P O244 Mo3B 134.9(4) . 2_576 ?
Mo1O O245 Mo3G 153.6(4) . . ?
Mo4J O246 Mo3M 153.1(3) . . ?
Mo13 O248 Mo1T 121.8(3) . 2_576 ?
Mo2C O249 Mo2D 116.2(3) . . ?
Mo1L O250 Mo2R 109.7(3) . . ?
Mo1L O250 Mo2N 111.0(3) . . ?
Mo2R O250 Mo2N 133.8(3) . . ?
Mo2A O251 Mo1X 122.8(3) . . ?
Mo1I O252 Mo25 158.2(3) . . ?
Mo1W O253 Mo2U 157.9(4) . . ?
Mo27 O256 Mo2G 141.4(3) . . ?
Mo27 O256 Mo2E 102.9(3) . . ?
Mo2G O256 Mo2E 102.7(2) . . ?
Mo27 O256 Mo2W 102.9(2) . . ?
Mo2G O256 Mo2W 102.4(2) . . ?
Mo2E O256 Mo2W 96.2(2) . . ?
Mo1T O259 Mo20 136.8(3) . . ?
Mo1T O259 Mo2K 110.8(3) . . ?
Mo20 O259 Mo2K 110.5(3) . . ?
Mo1V O261 Mo1T 158.5(3) . 2_576 ?
Mo4O O262 Mo31 109.5(3) . . ?
Mo4O O262 Mo1D 110.7(2) . . ?
Mo31 O262 Mo1D 139.1(3) . . ?
Mo22 O263 Mo2V 141.3(3) . . ?
Mo22 O263 Mo2O 103.0(3) . . ?
Mo2V O263 Mo2O 102.8(2) . . ?
Mo22 O263 Mo37 102.6(2) . . ?
Mo2V O263 Mo37 102.9(2) . . ?
Mo2O O263 Mo37 96.0(2) . . ?
Mo37 O266 Mo34 103.3(2) . . ?
Mo37 O266 Mo2V 108.0(2) . . ?
Mo34 O266 Mo2V 89.1(2) . . ?
Mo2H O268 Mo35 109.9(3) . . ?
Mo2H O268 Mo3C 141.0(3) . . ?
Mo35 O268 Mo3C 108.2(3) . . ?
Mo4M O269 Mo1F 109.3(2) . . ?
Mo4M O269 Mo29 142.0(3) . . ?
Mo1F O269 Mo29 108.3(3) . . ?
Mo41 O270 Mo3I 142.6(5) . . ?
M41 O270 M3I 110.0(7) . . ?
Mo17 O272 Mo1G 109.1(2) . . ?
Mo17 O272 Mo4Y 143.1(3) . . ?
Mo1G O272 Mo4Y 107.7(2) . . ?
Mo1P O273 Mo3Q 153.1(4) . . ?
Mo2R O274 M3L 150.7(7) . . ?
Mo2R O274 Mo3L 158.1(4) . . ?
Mo2G O275 Mo2E 108.8(3) . . ?
Mo2G O275 Mo33 142.8(3) . . ?
Mo2E O275 Mo33 108.1(3) . . ?
Mo32 O276 Mo23 149.8(4) . . ?
Mo27 O277 Mo20 158.2(3) . . ?
Mo1Q O278 Mo1F 117.0(3) . . ?
Mo2W O279 Mo2T 102.9(2) . . ?
Mo2W O279 Mo2G 107.6(3) . . ?
Mo2T O279 Mo2G 88.62(19) . . ?
Mo2E O280 Mo3H 109.8(3) . . ?
Mo2E O280 Mo36 110.5(3) . . ?
Mo3H O280 Mo36 135.2(3) . . ?
Mo2S O288 M39 151.8(6) . . ?
Mo2S O288 Mo39 160.0(4) . . ?
Mo24 O289 Mo14 136.9(3) . . ?
Mo24 O289 Mo2Z 110.9(3) . . ?
Mo14 O289 Mo2Z 110.1(2) . . ?
Mo2V O291 Mo24 158.4(4) . . ?
Mo2L O297 Mo1E 149.5(3) . . ?
Mo27 O302 Mo2E 108.9(3) . . ?
Mo27 O302 Mo36 142.1(3) . . ?
Mo2E O302 Mo36 108.6(3) . . ?
Mo1M O303 Mo3X 154.5(4) . . ?
Mo1M O303 M3X 151.8(4) . . ?
Mo1W O304 Mo23 123.3(3) . . ?
Mo3B O305 Mo1T 148.9(4) . . ?
Mo2R O307 Mo3G 157.7(4) . . ?
Mo1A O311 Mo1P 111.3(3) . . ?
Mo1A O311 Mo2X 108.9(3) . . ?
Mo1P O311 Mo2X 137.9(3) . . ?
Mo2Z O314 Mo35 116.9(3) . . ?
Mo2M O315 Mo2D 109.4(3) . . ?
Mo2M O315 Mo1Y 142.3(3) . . ?
Mo2D O315 Mo1Y 108.1(3) . . ?
Mo1C O318 Mo46 154.4(4) . . ?
Mo1C O318 M46 148.3(5) . . ?
Mo3Q O321 Mo3M 141.5(4) . . ?
Mo2G O322 Mo2T 122.8(3) . . ?
Mo3C O323 Mo1Z 149.3(3) . . ?
Mo2F O324 Mo35 109.2(3) . . ?
Mo2F O324 Mo3J 141.7(3) . . ?
Mo35 O324 Mo3J 108.2(3) . . ?
Mo1V O325 Mo16 121.6(3) . . ?
Mo1Y O328 Mo3S 155.8(4) . . ?
Mo1Y O328 M3S 136.1(5) . . ?
Mo2E O330 Mo3H 110.7(3) . . ?
Mo2E O330 Mo33 110.1(3) . . ?
Mo3H O330 Mo33 137.1(3) . . ?
Mo1U O333 Mo16 148.8(3) . . ?
Mo1O O334 Mo14 149.2(3) . . ?
Mo2D O338 Mo3A 110.7(3) . . ?
Mo2D O338 Mo3D 109.1(3) . . ?
Mo3A O338 Mo3D 136.3(3) . . ?
Mo3F O339 Mo2U 149.5(3) . . ?
Mo1N O341 Mo38 110.1(3) . 2_576 ?
Mo1N O341 Mo2Y 110.0(3) . 2_576 ?
Mo38 O341 Mo2Y 133.5(3) 2_576 2_576 ?
Mo4W O343 Mo47 150.8(4) . . ?
Mo4W O343 M47 153.7(4) . . ?
Mo4K O345 Mo3N 153.5(4) . . ?
Mo32 O346 Mo3Z 147.6(4) . . ?
Mo2M O347 Mo2B 158.3(3) . . ?
C101 O351 Mo1R 128.3(7) 2_667 . ?
Mo2G O355 Mo1X 157.7(3) . . ?
Mo1D O356 Mo61 153.3(5) . . ?
Mo1D O356 M61 153.8(7) . . ?
Mo2D O357 Mo3D 110.0(3) . . ?
Mo2D O357 Mo1Y 110.8(3) . . ?
Mo3D O357 Mo1Y 134.4(3) . . ?
Mo21 O358 M3R 149.5(6) . . ?
Mo21 O358 Mo3R 155.9(4) . . ?
Mo3A O359 Mo2T 149.7(3) . . ?
Mo4Y O360 Mo39 154.4(3) . . ?
Mo4Y O360 M39 146.7(4) . . ?
Mo2W O361 Mo2E 116.5(3) . . ?
Mo1V O362 Mo30 109.7(3) . . ?
Mo1V O362 Mo3B 140.9(3) . 2_576 ?
Mo30 O362 Mo3B 108.8(3) . 2_576 ?
Mo2A O363 Mo2T 157.5(4) . . ?
Mo28 O364 M3I 154.1(7) . . ?
Mo28 O364 Mo3I 159.1(4) . . ?
Mo2O O366 Mo3K 109.5(3) . . ?
Mo2O O366 Mo32 110.6(3) . . ?
Mo3K O366 Mo32 136.0(4) . . ?
Mo38 O369 Mo3V 157.3(4) . . ?
Mo33 O370 Mo3W 155.5(4) . . ?
Mo33 O370 M3W 144.2(5) . . ?
Mo1S O374 M47 152.3(6) . . ?
Mo1S O374 Mo47 157.2(5) . . ?
Mo38 O375 Mo3O 158.3(4) . 2_576 ?
Mo36 O377 Mo3Y 156.1(4) . . ?
Mo2N O378 M3L 151.1(6) . . ?
Mo2N O378 Mo3L 154.6(4) . . ?
Mo1H O380 Mo3U 156.3(4) . . ?
Mo1H O380 M3U 147.0(5) . . ?
Mo3S O383 Mo44 139.5(5) . . ?
M3S O383 M44 83.8(11) . . ?
Mo30 O384 Mo3P 110.1(3) . . ?
Mo30 O384 Mo3F 109.9(3) . . ?
Mo3P O384 Mo3F 136.8(3) . . ?
Mo2X O387 Mo3X 158.9(5) . . ?
Mo2X O387 M3X 162.0(6) . . ?
Mo31 O392 Mo61 154.3(5) . . ?
Mo31 O392 M61 155.2(6) . . ?
Mo35 O393 M3T 101.5(5) . . ?
Mo35 O393 Mo3T 109.4(3) . . ?
Mo35 O393 Mo3C 109.9(3) . . ?
M3T O393 Mo3C 147.5(5) . . ?
Mo3T O393 Mo3C 136.3(4) . . ?
Mo3U O395 Mo3R 140.8(5) . . ?
M3R O395 M3U 106.9(7) . . ?
Mo3D O396 M3S 136.8(7) . . ?
Mo3D O396 Mo3S 158.6(4) . . ?
Mo2Y O399 Mo3V 153.5(4) . . ?
M3T O404 Mo35 103.6(4) . . ?
Mo35 O404 Mo3T 109.7(3) . . ?
M3T O404 Mo3J 144.4(5) . . ?
Mo35 O404 Mo3J 110.5(3) . . ?
Mo3T O404 Mo3J 136.0(4) . . ?
Mo28 O405 M46 142.6(6) . . ?
Mo28 O405 Mo46 153.7(4) . . ?
C91 O406 Mo3N 122.7(10) . . ?
Mo2S O409 Mo3R 159.2(4) . . ?
Mo2S O409 M3R 141.7(6) . . ?
C101 O410 Mo39 129.3(8) . . ?
Mo3N O413 Mo3X 137.4(5) . . ?
Mo3N O413 M3X 120.1(5) . . ?
Mo2P O414 Mo42 152.8(4) . . ?
Mo3A O415 Mo45 154.9(4) . . ?
Mo3G O419 Mo42 140.0(5) . . ?
Mo3W O421 Mo3L 140.4(5) . . ?
M3L O421 M3W 108.0(7) . . ?
C31 O423 Mo3L 118.6(10) . . ?
Mo3C O425 Mo44 149.2(6) . . ?
C51 O429 Mo3G 112.1(17) . . ?
Mo3Y O431 Mo43 140.3(5) . . ?
Mo3Y O431 M43 124.3(6) . . ?
Mo31 O432 M3U 140.3(6) . . ?
Mo31 O432 Mo3U 154.4(4) . . ?
C21 O436 Mo43 121.2(15) . . ?
M60 O439 M48 114.1(10) . . ?
Mo3V O442 Mo45 135.9(5) . . ?
Mo46 O444 Mo47 139.2(5) . . ?
M47 O444 M46 102.0(6) . . ?
Mo3J O446 Mo34 148.5(4) . . ?
Mo1S O447 Mo3M 158.3(5) . . ?
Mo3Z O448 Mo3O 139.1(5) . . ?
Mo3H O449 Mo3Y 158.0(6) . . ?
C11 O450 Mo3S 123.5(12) . . ?
Mo2L O453 M40 151.5(5) . . ?
Mo2L O453 Mo40 159.5(5) . . ?
Mo3B O455 Mo43 153.7(5) . . ?
Mo3B O455 M43 144.5(6) . . ?
Mo3H O456 Mo3W 155.6(7) . . ?
C11 O457 Mo44 123.2(13) . . ?
C81 O458 Mo3R 101.8(14) . . ?
Mo2X O459 Mo3Q 157.6(5) . . ?
Mo3E O467 Mo41 160.0(6) 2_667 . ?
Mo3E O467 M41 143.1(6) 2_667 . ?
Mo3F O468 Mo48 156.7(4) . . ?
Mo3F O468 M48 144.0(6) . . ?
M43 O472 Mo3P 149.1(9) 2_576 . ?
Mo3P O472 Mo43 157.1(7) . 2_576 ?
Mo3P O473 M48 145.8(7) . . ?
Mo3P O473 Mo48 160.1(6) . . ?
C61 O474 Mo48 109.9(17) . . ?
M60 O475 C61 116.4(19) . . ?
C61 O475 Mo60 110.4(17) . . ?
Mo3J O479 Mo60 154.9(5) . . ?
Mo3J O479 M60 148.0(6) . . ?
O780 O480 M60 96(3) . . ?
Mo3T O480 Mo60 149.3(8) . . ?
O780 O480 M3T 62(2) . . ?
M60 O480 M3T 151.1(9) . . ?
O783 O483 M44 125(2) . . ?
Mo3T O483 Mo44 149.4(6) . . ?
O783 O483 M3T 49.4(17) . . ?
M44 O483 M3T 160.4(12) . . ?
Mo3D O489 Mo45 158.0(5) . . ?
C1 O492 Mo45 127.1(11) . . ?
C21 O495 Mo3Y 125.3(16) . . ?
C31 O501 Mo3W 121.8(11) . . ?
Mo3K O504 Mo42 157.3(6) . . ?
Mo3K O505 Mo3Z 150.6(6) . . ?
Mo3E O513 Mo40 159.0(8) . . ?
C71 O516 M47 127.1(12) . . ?
C71 O516 Mo47 123.1(11) . . ?
C81 O518 Mo3U 108.3(13) . . ?
C51 O519 Mo42 112.0(15) . . ?
C71 O520 Mo46 125.8(11) . . ?
C91 O524 Mo3X 125.8(11) . . ?
C1 O529 Mo3V 125.3(10) . . ?
Mo40 O533 Mo61 137.4(8) . . ?
M61 O533 M40 136.5(9) . . ?
Mo60 O739 Mo48 121.3(10) . . ?
Mo3H O756 M3W 126.5(12) . . ?
O480 O780 M3T 99(3) . . ?
O480 O780 M60 65(2) . . ?
M3T O780 M60 155.3(16) . . ?
O483 O783 M3T 110(2) . . ?
O483 O783 M44 39.8(17) . . ?
M3T O783 M44 144.7(16) . . ?
Mo3E O813 M40 151.2(12) . . ?
O529 C1 O492 127.4(14) . . ?
O529 C1 C2 110.0(14) . . ?
O492 C1 C2 122.4(15) . . ?
N0 C2 C3 118(2) . . ?
N0 C2 C1 123(2) . . ?
C3 C2 C1 114.5(17) . . ?
O457 C11 O450 131.6(18) . . ?
O457 C11 C12 118.3(19) . . ?
O450 C11 C12 108.6(17) . . ?
C12 C11 M44 132(2) . . ?
C12 C11 M3S 125.6(15) . . ?
M44 C11 M3S 101.6(14) . . ?
N1 C12 C13 120(2) . . ?
N1 C12 C11 126(2) . . ?
C13 C12 C11 114(2) . . ?
O495 C21 O436 122(2) . . ?
O495 C21 C22 125(3) . . ?
O436 C21 C22 114(2) . . ?
O495 C21 M43 108.6(15) . . ?
C22 C21 M43 126(2) . . ?
N2 C22 C23 126(3) . . ?
N2 C22 C21 116(3) . . ?
C23 C22 C21 114(2) . . ?
O501 C31 O423 131.5(15) . . ?
O501 C31 C32 114.5(16) . . ?
O423 C31 C32 112.4(15) . . ?
C32 C31 M3W 133.7(13) . . ?
C32 C31 M3L 131.3(14) . . ?
M3W C31 M3L 89.6(7) . . ?
N3 C32 C33 113.0(19) . . ?
N3 C32 C31 122.7(19) . . ?
C33 C32 C31 124.2(18) . . ?
O429 C51 C52 116(3) . . ?
O429 C51 O519 142(2) . . ?
C52 C51 O519 101(2) . . ?
N5 C52 C53 121(3) . . ?
N5 C52 C51 115(3) . . ?
C53 C52 C51 124(3) . . ?
O474 C61 O475 133(3) . . ?
O474 C61 C62 113(2) . . ?
O475 C61 C62 108(2) . . ?
O475 C61 M48 119.0(18) . . ?
C62 C61 M48 133.4(16) . . ?
O475 C61 M60 29.7(10) . . ?
C62 C61 M60 130.8(16) . . ?
M48 C61 M60 93.3(11) . . ?
N6 C62 C63 122(3) . . ?
N6 C62 C61 120(2) . . ?
C63 C62 C61 116(2) . . ?
O516 C71 O520 123.6(15) . . ?
O516 C71 C72 118.2(16) . . ?
O520 C71 C72 117.8(16) . . ?
O516 C71 M47 28.7(7) . . ?
C72 C71 M47 138.3(14) . . ?
N7 C72 C71 110.7(19) . . ?
N7 C72 C73 117(2) . . ?
C71 C72 C73 111.3(19) . . ?
C82 C81 O518 112.2(17) . . ?
C82 C81 O458 107.0(16) . . ?
O518 C81 O458 130(2) . . ?
C82 C81 M3R 128.4(14) . . ?
C82 C81 M3U 134.2(13) . . ?
M3R C81 M3U 95.5(11) . . ?
N8 C82 C83 119(2) . . ?
N8 C82 C81 122(2) . . ?
C83 C82 C81 119(2) . . ?
O406 C91 O524 125.1(14) . . ?
O406 C91 C92 126.3(16) . . ?
O524 C91 C92 107.8(15) . . ?
O406 C91 M3X 102.7(9) . . ?
C92 C91 M3X 130.6(13) . . ?
N9 C92 C91 106.7(16) . . ?
N9 C92 C93 112(2) . . ?
C91 C92 C93 114(2) . . ?
O410 C101 O351 125.6(10) . 2_667 ?
O410 C101 C102 112.1(10) . . ?
O351 C101 C102 122.2(10) 2_667 . ?
O351 C101 M39 105.1(7) 2_667 . ?
C102 C101 M39 131.3(8) . . ?
N10 C102 C103 118.4(15) . . ?
N10 C102 C101 113.7(13) . . ?
C103 C102 C101 112.8(12) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1A O162 1.675(6) . ?
Mo1A O311 1.985(5) . ?
Mo1A O89 1.987(5) . ?
Mo1A O167 2.011(5) . ?
Mo1A O172 2.013(5) . ?
Mo1A O82 2.101(5) . ?
Mo1A O135 2.236(6) . ?
Mo1B O75 1.674(6) . ?
Mo1B O69 1.765(5) . ?
Mo1B O109 1.940(5) . ?
Mo1B O32 1.956(5) . ?
Mo1B O55 2.109(5) . ?
Mo1B O23 2.492(5) . ?
Mo1C O70 1.675(7) . ?
Mo1C O318 1.732(7) . ?
Mo1C O183 1.839(6) . ?
Mo1C O91 2.050(6) . ?
Mo1C O34 2.125(5) . ?
Mo1C O258 2.320(7) . ?
Mo1D O154 1.673(5) . ?
Mo1D O356 1.730(6) . ?
Mo1D O161 1.840(6) . ?
Mo1D O262 2.058(6) . ?
Mo1D O12 2.107(5) . ?
Mo1D O298 2.336(6) . ?
Mo1E O94 1.676(6) . ?
Mo1E O189 1.902(6) . ?
Mo1E O49 1.926(6) . ?
Mo1E O297 1.968(6) . ?
Mo1E O63 2.003(5) . ?
Mo1E O59 2.339(5) . ?
Mo1F O115 1.674(6) . ?
Mo1F O231 1.988(6) . ?
Mo1F O236 1.997(7) . ?
Mo1F O269 2.009(5) . ?
Mo1F O181 2.009(5) . ?
Mo1F O24 2.104(5) . ?
Mo1F O278 2.241(5) . ?
Mo1G O284 1.694(6) . ?
Mo1G O139 1.987(5) . ?
Mo1G O163 1.989(6) . ?
Mo1G O164 2.008(5) . ?
Mo1G O272 2.012(5) . ?
Mo1G O19 2.112(5) . ?
Mo1G O53 2.222(6) . ?
Mo1H O309 1.695(6) . ?
Mo1H O380 1.731(6) . ?
Mo1H O97 1.833(6) . ?
Mo1H O27 2.055(6) . ?
Mo1H O104 2.105(5) . ?
Mo1H O353 2.330(6) . ?
Mo1I O216 1.672(5) . ?
Mo1I O252 1.848(6) . ?
Mo1I O52 1.865(6) . ?
Mo1I O198 1.994(5) . ?
Mo1I O46 2.070(6) 2_576 ?
Mo1I O116 2.451(5) . ?
Mo1J O103 1.669(6) . ?
Mo1J O40 1.850(6) . ?
Mo1J O193 1.854(5) . ?
Mo1J O169 1.991(6) . ?
Mo1J O77 2.082(5) . ?
Mo1J O238 2.456(5) . ?
Mo1K O51 1.691(6) . ?
Mo1K O135 1.774(5) . ?
Mo1K O59 1.938(5) . ?
Mo1K O47 1.966(5) . ?
Mo1K O63 2.104(5) . ?
Mo1K O82 2.496(5) . ?
Mo1L O151 1.677(5) . ?
Mo1L O250 1.980(6) . ?
Mo1L O108 1.995(5) . ?
Mo1L O169 2.005(5) . ?
Mo1L O206 2.015(5) . ?
Mo1L O77 2.109(6) . ?
Mo1L O203 2.222(5) . ?
Mo1M O129 1.684(6) . ?
Mo1M O303 1.739(6) . ?
Mo1M O221 1.830(5) . ?
Mo1M O89 2.067(5) . ?
Mo1M O172 2.106(5) . ?
Mo1M O354 2.327(7) . ?
Mo1N O209 1.674(5) . ?
Mo1N O341 1.983(6) . ?
Mo1N O153 2.001(5) . ?
Mo1N O198 2.013(6) 2_576 ?
Mo1N O212 2.015(6) . ?
Mo1N O46 2.097(5) . ?
Mo1N O179 2.214(6) 2_576 ?
Mo1O O365 1.697(6) . ?
Mo1O O245 1.738(6) . ?
Mo1O O334 1.844(6) . ?
Mo1O O108 2.064(6) . ?
Mo1O O206 2.091(5) . ?
Mo1O O88 2.325(5) . ?
Mo1P O229 1.719(6) . ?
Mo1P O273 1.745(5) . ?
Mo1P O95 1.810(5) . ?
Mo1P O311 2.049(6) . ?
Mo1P O167 2.101(5) . ?
Mo1P O219 2.322(6) . ?
Mo1Q O190 1.680(5) . ?
Mo1Q O278 1.758(6) . ?
Mo1Q O114 1.947(5) . ?
Mo1Q O67 1.974(5) . ?
Mo1Q O155 2.109(5) . ?
Mo1Q O24 2.477(5) . ?
Mo1R O220 1.692(6) . ?
Mo1R O192 1.710(6) . ?
Mo1R O148 1.907(6) . ?
Mo1R O200 2.000(6) . ?
Mo1R O351 2.193(7) . ?
Mo1R O199 2.245(5) 2_567 ?
Mo1S O374 1.754(7) . ?
Mo1S O428 1.756(9) . ?
Mo1S O447 1.774(8) . ?
Mo1S O131 2.052(6) . ?
Mo1S O14 2.068(5) . ?
Mo1S O422 2.283(9) . ?
Mo1T O403 1.674(6) . ?
Mo1T O261 1.905(6) 2_576 ?
Mo1T O248 1.949(6) 2_576 ?
Mo1T O305 1.970(6) . ?
Mo1T O259 1.996(6) . ?
Mo1T O235 2.319(6) . ?
Mo1U O286 1.692(6) . ?
Mo1U O213 1.755(6) . ?
Mo1U O333 1.829(6) . ?
Mo1U O153 2.078(6) . ?
Mo1U O212 2.106(5) . ?
Mo1U O312 2.319(6) . ?
Mo1V O218 1.670(7) . ?
Mo1V O261 1.845(6) . ?
Mo1V O325 1.863(5) . ?
Mo1V O362 1.997(6) . ?
Mo1V O22 2.074(6) . ?
Mo1V O178 2.426(6) . ?
Mo1W O201 1.665(6) . ?
Mo1W O253 1.842(6) . ?
Mo1W O304 1.854(6) . ?
Mo1W O239 1.990(6) . ?
Mo1W O22 2.072(6) . ?
Mo1W O85 2.453(6) . ?
Mo1X O287 1.674(6) . ?
Mo1X O355 1.908(6) . ?
Mo1X O251 1.958(7) . ?
Mo1X O211 1.962(6) . ?
Mo1X O83 2.001(6) . ?
Mo1X O217 2.330(6) . ?
Mo1Y O331 1.697(7) . ?
Mo1Y O328 1.754(7) . ?
Mo1Y O204 1.833(6) . ?
Mo1Y O357 2.059(6) . ?
Mo1Y O315 2.115(6) . ?
Mo1Y O394 2.330(7) . ?
Mo1Z O226 1.674(6) . ?
Mo1Z O142 1.914(6) . ?
Mo1Z O141 1.947(6) . ?
Mo1Z O323 1.955(6) . ?
Mo1Z O227 1.997(6) . ?
Mo1Z O107 2.310(6) . ?
Mo2A O267 1.672(6) . ?
Mo2A O363 1.844(6) . ?
Mo2A O251 1.847(6) . ?
Mo2A O223 2.001(6) . ?
Mo2A O160 2.069(6) . ?
Mo2A O217 2.444(6) . ?
Mo2B O257 1.666(6) . ?
Mo2B O347 1.910(6) . ?
Mo2B O40 1.927(6) . ?
Mo2B O204 1.964(6) . ?
Mo2B O227 2.002(5) . ?
Mo2B O238 2.343(6) . ?
Mo2C O271 1.671(6) . ?
Mo2C O249 1.774(6) . ?
Mo2C O224 1.956(6) . ?
Mo2C O217 1.974(6) . ?
Mo2C O83 2.109(5) . ?
Mo2C O160 2.478(6) . ?
Mo2D O348 1.672(6) . ?
Mo2D O357 1.994(6) . ?
Mo2D O338 1.995(6) . ?
Mo2D O223 2.003(6) . ?
Mo2D O315 2.005(6) . ?
Mo2D O160 2.095(6) . ?
Mo2D O249 2.239(6) . ?
Mo2E O111 1.683(6) . ?
Mo2E O280 1.979(6) . ?
Mo2E O330 1.989(6) . ?
Mo2E O302 2.010(6) . ?
Mo2E O275 2.019(6) . ?
Mo2E O256 2.093(6) . ?
Mo2E O361 2.221(6) . ?
Mo2F O337 1.666(7) . ?
Mo2F O186 1.830(6) . ?
Mo2F O120 1.853(6) . ?
Mo2F O324 1.989(6) . ?
Mo2F O137 2.066(6) . ?
Mo2F O146 2.463(6) . ?
Mo2G O296 1.672(6) . ?
Mo2G O355 1.846(6) . ?
Mo2G O322 1.861(6) . ?
Mo2G O275 1.987(6) . ?
Mo2G O256 2.077(6) . ?
Mo2G O279 2.435(6) . ?
Mo2H O285 1.677(7) . ?
Mo2H O142 1.834(5) . ?
Mo2H O105 1.856(6) . ?
Mo2H O268 1.986(6) . ?
Mo2H O137 2.071(5) . ?
Mo2H O191 2.428(6) . ?
Mo2I O350 1.682(6) . ?
Mo2I O203 1.762(6) . ?
Mo2I O107 1.946(6) . ?
Mo2I O238 1.964(5) . ?
Mo2I O227 2.103(6) . ?
Mo2I O77 2.491(5) . ?
Mo2J O185 1.737(5) . ?
Mo2J O200 1.756(5) . ?
Mo2J O214 1.984(6) . ?
Mo2J O33 2.027(5) . ?
Mo2J O119 2.042(5) . ?
Mo2J O72 2.0617(11) . ?
Mo2K O349 1.682(6) . ?
Mo2K O179 1.759(6) . ?
Mo2K O116 1.957(6) . ?
Mo2K O235 1.959(6) . ?
Mo2K O259 2.086(6) . ?
Mo2K O46 2.494(5) 2_576 ?
Mo2L O390 1.708(7) . ?
Mo2L O453 1.725(8) . ?
Mo2L O297 1.825(6) . ?
Mo2L O236 2.055(6) . ?
Mo2L O181 2.105(6) . ?
Mo2L O381 2.324(8) . ?
Mo2M O281 1.668(6) . ?
Mo2M O347 1.840(6) . ?
Mo2M O171 1.853(7) . ?
Mo2M O315 1.989(6) . ?
Mo2M O160 2.078(6) . ?
Mo2M O224 2.416(6) . ?
Mo2N O295 1.692(7) . ?
Mo2N O378 1.747(7) . ?
Mo2N O230 1.832(6) . ?
Mo2N O250 2.066(5) . ?
Mo2N O169 2.098(6) . ?
Mo2N O332 2.302(7) . ?
Mo2O O352 1.678(6) . ?
Mo2O O366 1.981(7) . ?
Mo2O O147 1.996(6) . ?
Mo2O O112 2.009(5) . ?
Mo2O O62 2.021(5) . ?
Mo2O O263 2.096(6) . ?
Mo2O O93 2.222(6) . ?
Mo2P O264 1.700(7) . ?
Mo2P O414 1.746(7) . ?
Mo2P O195 1.818(6) . ?
Mo2P O147 2.071(6) . ?
Mo2P O112 2.124(6) . ?
Mo2P O329 2.316(8) . ?
Mo2Q O283 1.679(6) . ?
Mo2Q O222 1.774(6) . ?
Mo2Q O85 1.944(6) . ?
Mo2Q O178 1.958(6) . ?
Mo2Q O138 2.093(5) . ?
Mo2Q O22 2.482(6) . ?
Mo2R O400 1.701(8) . ?
Mo2R O307 1.789(6) . ?
Mo2R O274 1.797(7) . ?
Mo2R O250 2.062(5) . ?
Mo2R O108 2.065(6) . ?
Mo2R O368 2.342(7) . ?
Mo2S O379 1.733(8) . ?
Mo2S O409 1.772(6) . ?
Mo2S O288 1.772(6) . ?
Mo2S O139 2.047(5) . ?
Mo2S O163 2.052(6) . ?
Mo2S O292 2.314(10) . ?
Mo2T O165 1.663(6) . ?
Mo2T O363 1.912(6) . ?
Mo2T O322 1.935(7) . ?
Mo2T O359 1.968(6) . ?
Mo2T O184 2.005(6) . ?
Mo2T O279 2.334(6) . ?
Mo2U O306 1.659(8) . ?
Mo2U O253 1.915(6) . ?
Mo2U O232 1.930(7) . ?
Mo2U O339 1.959(7) . ?
Mo2U O177 1.995(5) . ?
Mo2U O225 2.352(6) . ?
Mo2V O320 1.666(6) . ?
Mo2V O291 1.831(5) . ?
Mo2V O207 1.848(7) . ?
Mo2V O112 1.973(7) . ?
Mo2V O263 2.071(6) . ?
Mo2V O266 2.433(6) . ?
Mo2W O265 1.678(6) . ?
Mo2W O361 1.775(6) . ?
Mo2W O279 1.957(6) . ?
Mo2W O101 1.959(6) . ?
Mo2W O184 2.092(6) . ?
Mo2W O256 2.471(6) . ?
Mo2X O387 1.742(7) . ?
Mo2X O459 1.766(7) . ?
Mo2X O373 1.831(10) . ?
Mo2X O89 2.038(5) . ?
Mo2X O311 2.076(6) . ?
Mo2X O434 2.150(10) . ?
Mo2Y O300 1.704(7) . ?
Mo2Y O399 1.742(7) . ?
Mo2Y O180 1.831(6) . ?
Mo2Y O341 2.084(6) 2_576 ?
Mo2Y O198 2.094(6) . ?
Mo2Y O344 2.307(8) . ?
Mo2Z O233 1.663(6) . ?
Mo2Z O314 1.774(6) . ?
Mo2Z O146 1.951(6) . ?
Mo2Z O191 1.967(5) . ?
Mo2Z O289 2.091(6) . ?
Mo2Z O137 2.494(6) . ?
Mo3A O310 1.703(7) . ?
Mo3A O415 1.737(7) . ?
Mo3A O359 1.825(6) . ?
Mo3A O338 2.056(7) . ?
Mo3A O223 2.095(6) . ?
Mo3A O427 2.343(8) . ?
Mo3B O388 1.721(8) . ?
Mo3B O455 1.747(7) . ?
Mo3B O305 1.829(6) . ?
Mo3B O244 2.066(7) 2_576 ?
Mo3B O362 2.099(6) 2_576 ?
Mo3B O408 2.301(8) . ?
Mo3C O326 1.705(7) . ?
Mo3C O425 1.760(10) . ?
Mo3C O725 1.77(2) . ?
Mo3C O323 1.840(6) . ?
Mo3C O393 2.067(6) . ?
Mo3C O268 2.104(6) . ?
Mo3C O440 2.306(9) . ?
Mo3D O488 1.731(11) . ?
Mo3D O396 1.768(8) . ?
Mo3D O489 1.778(9) . ?
Mo3D O357 2.037(6) . ?
Mo3D O338 2.058(7) . ?
Mo3D O465 2.284(10) . ?
Mo3E O512 1.733(11) . ?
Mo3E O813 1.75(2) . ?
Mo3E O513 1.780(13) . ?
Mo3E O467 1.794(9) 2_667 ?
Mo3E O236 2.036(6) . ?
Mo3E O231 2.053(6) . ?
Mo3E O511 2.245(12) . ?
Mo3F O255 1.711(7) . ?
Mo3F O468 1.747(7) . ?
Mo3F O339 1.838(7) . ?
Mo3F O384 2.087(7) . ?
Mo3F O239 2.094(5) . ?
Mo3F O371 2.330(9) . ?
Mo3G O401 1.662(8) . ?
Mo3G O391 1.714(8) . ?
Mo3G O419 1.881(7) . ?
Mo3G O307 2.002(6) . ?
Mo3G O245 2.217(7) . ?
Mo3G O429 2.278(10) . ?
Mo3H O445 1.692(10) . ?
Mo3H O449 1.755(10) . ?
Mo3H O456 1.784(11) . ?
Mo3H O756 1.89(2) . ?
Mo3H O330 2.026(7) . ?
Mo3H O280 2.057(6) . ?
Mo3H O498 2.268(13) . ?
Mo3I O402 1.695(8) . ?
Mo3I O418 1.721(10) . ?
Mo3I O270 1.891(8) . ?
Mo3I O364 1.968(7) . ?
Mo3I O411 2.131(11) . ?
Mo3I O194 2.223(6) . ?
Mo3J O336 1.712(7) . ?
Mo3J O479 1.765(9) . ?
Mo3J O446 1.825(7) . ?
Mo3J O404 2.062(6) . ?
Mo3J O324 2.108(6) . ?
Mo3J O386 2.316(9) . ?
Mo3K O430 1.758(11) . ?
Mo3K O504 1.772(9) . ?
Mo3K O505 1.773(9) . ?
Mo3K O147 2.033(7) . ?
Mo3K O366 2.051(7) . ?
Mo3K O397 2.230(11) . ?
Mo3L O426 1.660(10) . ?
Mo3L O461 1.676(9) . ?
Mo3L O421 1.896(7) . ?
Mo3L O274 2.019(7) . ?
Mo3L O378 2.205(7) . ?
Mo3L O423 2.241(11) . ?
Mo3M O469 1.696(11) . ?
Mo3M O438 1.819(9) . ?
Mo3M O321 1.884(6) . ?
Mo3M O175 1.942(11) . ?
Mo3M O447 1.994(8) . ?
Mo3M O246 2.200(5) . ?
Mo3N O208 1.681(6) . ?
Mo3N O420 1.709(8) . ?
Mo3N O413 1.898(8) . ?
Mo3N O185 2.005(5) . ?
Mo3N O406 2.200(10) . ?
Mo3N O345 2.282(6) . ?
Mo3O O463 1.687(8) . ?
Mo3O O441 1.711(10) . ?
Mo3O O448 1.904(8) . ?
Mo3O O375 1.987(7) 2_576 ?
Mo3O O213 2.219(6) . ?
Mo3O O385 2.292(11) . ?
Mo3P O471 1.750(13) . ?
Mo3P O473 1.763(10) . ?
Mo3P O472 1.775(11) . ?
Mo3P O384 2.034(7) . ?
Mo3P O244 2.059(6) . ?
Mo3P O462 2.249(11) . ?
Mo3Q O466 1.717(11) . ?
Mo3Q O321 1.883(7) . ?
Mo3Q O510 1.964(14) . ?
Mo3Q O509 1.986(12) . ?
Mo3Q O459 1.988(7) . ?
Mo3Q O273 2.165(6) . ?
Mo3R O743 1.668(19) . ?
Mo3R O514 1.747(12) . ?
Mo3R O395 1.890(7) . ?
Mo3R O409 2.020(6) . ?
Mo3R O358 2.180(7) . ?
Mo3R O458 2.250(15) . ?
Mo3S O487 1.651(10) . ?
Mo3S O786 1.707(19) . ?
Mo3S O383 1.863(7) . ?
Mo3S O396 2.040(8) . ?
Mo3S O328 2.190(6) . ?
Mo3S O450 2.316(16) . ?
Mo3T O480 1.748(12) . ?
Mo3T O483 1.797(10) . ?
Mo3T O481 1.879(11) . ?
Mo3T O404 2.057(7) . ?
Mo3T O393 2.061(6) . ?
Mo3T O482 2.192(11) . ?
Mo3U O525 1.672(13) . ?
Mo3U O460 1.809(11) . ?
Mo3U O395 1.868(8) . ?
Mo3U O432 2.026(7) . ?
Mo3U O518 2.074(13) . ?
Mo3U O380 2.158(6) . ?
Mo3V O494 1.679(11) . ?
Mo3V O493 1.711(11) . ?
Mo3V O442 1.898(9) . ?
Mo3V O369 2.003(8) . ?
Mo3V O399 2.208(7) . ?
Mo3V O529 2.218(11) . ?
Mo3W O499 1.656(14) . ?
Mo3W O500 1.745(12) . ?
Mo3W O421 1.879(7) . ?
Mo3W O456 2.017(12) . ?
Mo3W O501 2.176(14) . ?
Mo3W O370 2.180(7) . ?
Mo3X O523 1.691(11) . ?
Mo3X O398 1.779(9) . ?
Mo3X O413 1.905(8) . ?
Mo3X O387 2.033(8) . ?
Mo3X O524 2.127(14) . ?
Mo3X O303 2.236(6) . ?
Mo3Y O496 1.658(13) . ?
Mo3Y O412 1.860(11) . ?
Mo3Y O431 1.867(9) . ?
Mo3Y O449 2.016(10) . ?
Mo3Y O495 2.039(15) . ?
Mo3Y O377 2.188(7) . ?
Mo3Z O454 1.716(11) . ?
Mo3Z O506 1.870(14) . ?
Mo3Z O448 1.874(8) . ?
Mo3Z O505 1.951(9) . ?
Mo3Z O424 2.103(11) . ?
Mo3Z O346 2.197(8) . ?
Mo4A O237 1.671(5) . ?
Mo4A O38 1.910(5) . ?
Mo4A O74 1.953(5) . ?
Mo4A O95 1.969(5) . ?
Mo4A O3 2.007(5) . ?
Mo4A O21 2.330(5) . ?
Mo4B O58 1.686(5) . ?
Mo4B O16 1.835(5) . ?
Mo4B O5 1.865(5) . ?
Mo4B O13 1.986(5) . ?
Mo4B O29 2.072(5) . ?
Mo4B O125 2.428(5) . ?
Mo4C O73 1.661(6) . ?
Mo4C O16 1.911(5) 2_667 ?
Mo4C O37 1.945(5) . ?
Mo4C O144 1.976(5) 1_655 ?
Mo4C O7 2.008(5) . ?
Mo4C O8 2.334(5) . ?
Mo4D O61 1.668(5) . ?
Mo4D O168 1.920(5) . ?
Mo4D O15 1.944(5) . ?
Mo4D O157 1.977(5) . ?
Mo4D O155 1.987(5) . ?
Mo4D O114 2.326(5) . ?
Mo4E O124 1.687(5) . ?
Mo4E O194 1.750(6) . ?
Mo4E O132 1.835(5) . ?
Mo4E O44 2.047(5) . ?
Mo4E O42 2.089(5) . ?
Mo4E O243 2.376(5) . ?
Mo4F O110 1.678(6) . ?
Mo4F O199 1.735(5) . ?
Mo4F O144 1.840(5) . ?
Mo4F O119 2.045(5) 2_567 ?
Mo4F O13 2.108(5) 2_567 ?
Mo4F O208 2.369(6) . ?
Mo4G O45 1.667(5) . ?
Mo4G O90 1.924(5) . ?
Mo4G O10 1.931(5) . ?
Mo4G O96 1.956(6) . ?
Mo4G O76 1.995(5) 2_667 ?
Mo4G O6 2.340(5) . ?
Mo4H O113 1.685(5) . ?
Mo4H O44 1.987(6) . ?
Mo4H O91 1.993(5) . ?
Mo4H O34 1.998(5) . ?
Mo4H O42 2.009(5) . ?
Mo4H O4 2.094(5) . ?
Mo4H O66 2.220(5) . ?
Mo4I O240 1.686(5) . ?
Mo4I O131 1.977(5) . ?
Mo4I O14 1.991(6) . ?
Mo4I O68 2.003(5) . ?
Mo4I O106 2.010(5) . ?
Mo4I O23 2.093(5) . ?
Mo4I O69 2.230(5) . ?
Mo4J O121 1.694(5) . ?
Mo4J O246 1.750(5) . ?
Mo4J O100 1.836(5) . ?
Mo4J O14 2.051(5) . ?
Mo4J O68 2.095(5) . ?
Mo4J O64 2.358(5) . ?
Mo4K O170 1.677(7) . ?
Mo4K O345 1.739(6) . ?
Mo4K O157 1.843(5) . ?
Mo4K O33 2.041(5) . ?
Mo4K O79 2.120(5) . ?
Mo4K O192 2.358(6) 2_567 ?
Mo4L O254 1.668(6) . ?
Mo4L O196 1.916(5) . ?
Mo4L O176 1.943(5) . ?
Mo4L O123 1.962(6) . ?
Mo4L O55 1.990(5) . ?
Mo4L O32 2.315(5) . ?
Mo4M O143 1.672(5) . ?
Mo4M O90 1.839(5) . ?
Mo4M O15 1.852(5) . ?
Mo4M O269 1.999(5) . ?
Mo4M O24 2.069(5) . ?
Mo4M O114 2.436(5) . ?
Mo4N O182 1.670(6) . ?
Mo4N O136 1.912(5) . ?
Mo4N O31 1.940(5) . ?
Mo4N O221 1.971(5) . ?
Mo4N O155 2.013(5) . ?
Mo4N O67 2.337(5) . ?
Mo4O O188 1.665(5) . ?
Mo4O O27 1.983(5) . ?
Mo4O O262 2.002(5) . ?
Mo4O O12 2.019(5) . ?
Mo4O O104 2.020(5) . ?
Mo4O O36 2.099(5) . ?
Mo4O O86 2.232(5) . ?
Mo4P O145 1.670(5) . ?
Mo4P O98 1.849(5) . ?
Mo4P O81 1.871(5) . ?
Mo4P O34 1.986(5) . ?
Mo4P O4 2.070(5) . ?
Mo4P O17 2.460(5) . ?
Mo4Q O28 1.683(5) . ?
Mo4Q O86 1.767(5) . ?
Mo4Q O21 1.930(5) . ?
Mo4Q O80 1.965(5) . ?
Mo4Q O3 2.098(5) . ?
Mo4Q O36 2.493(5) . ?
Mo4R O25 1.683(5) . ?
Mo4R O127 1.848(5) . ?
Mo4R O176 1.854(6) . ?
Mo4R O106 1.989(5) . ?
Mo4R O23 2.065(5) . ?
Mo4R O32 2.435(5) . ?
Mo4S O87 1.678(5) . ?
Mo4S O20 1.771(4) . ?
Mo4S O125 1.946(5) . ?
Mo4S O6 1.969(5) . ?
Mo4S O76 2.103(5) 2_667 ?
Mo4S O29 2.470(5) . ?
Mo4T O56 1.673(5) . ?
Mo4T O66 1.769(5) . ?
Mo4T O17 1.933(5) . ?
Mo4T O8 1.981(5) . ?
Mo4T O7 2.100(5) . ?
Mo4T O4 2.467(5) . ?
Mo4U O247 1.678(5) . ?
Mo4U O189 1.850(5) . ?
Mo4U O31 1.856(6) . ?
Mo4U O181 1.994(6) . ?
Mo4U O24 2.067(5) . ?
Mo4U O67 2.449(5) . ?
Mo4V O202 1.684(5) . ?
Mo4V O136 1.839(5) . ?
Mo4V O49 1.863(6) . ?
Mo4V O172 1.998(5) . ?
Mo4V O82 2.066(5) . ?
Mo4V O59 2.437(5) . ?
Mo4W O210 1.688(6) . ?
Mo4W O343 1.734(6) . ?
Mo4W O26 1.840(5) . ?
Mo4W O131 2.073(5) . ?
Mo4W O106 2.108(5) . ?
Mo4W O159 2.317(7) . ?
Mo4X O149 1.678(5) . ?
Mo4X O38 1.852(5) . ?
Mo4X O92 1.862(5) . ?
Mo4X O167 1.996(5) . ?
Mo4X O82 2.057(5) . ?
Mo4X O47 2.431(5) . ?
Mo4Y O134 1.683(6) . ?
Mo4Y O360 1.741(6) . ?
Mo4Y O122 1.837(5) . ?
Mo4Y O139 2.063(5) . ?
Mo4Y O272 2.112(5) . ?
Mo4Y O197 2.329(7) . ?
Mo4Z O228 1.655(6) . ?
Mo4Z O98 1.910(5) . ?
Mo4Z O57 1.934(6) . ?
Mo4Z O183 1.955(6) . ?
Mo4Z O84 1.994(5) . ?
Mo4Z O41 2.352(5) . ?
Mo10 O156 1.671(6) . ?
Mo10 O50 1.917(5) . ?
Mo10 O78 1.936(5) . ?
Mo10 O97 1.962(5) . ?
Mo10 O55 2.009(5) . ?
Mo10 O109 2.313(5) . ?
Mo11 O71 1.689(5) . ?
Mo11 O102 1.832(5) . ?
Mo11 O141 1.864(6) . ?
Mo11 O206 2.002(6) . ?
Mo11 O77 2.068(5) . ?
Mo11 O107 2.423(5) . ?
Mo12 O293 1.676(6) . ?
Mo12 O196 1.847(5) . ?
Mo12 O35 1.855(6) . ?
Mo12 O164 1.987(5) . ?
Mo12 O19 2.073(5) . ?
Mo12 O43 2.430(6) . ?
Mo13 O205 1.678(5) . ?
Mo13 O65 1.851(6) . ?
Mo13 O248 1.862(6) . ?
Mo13 O212 1.987(5) . ?
Mo13 O46 2.073(6) . ?
Mo13 O235 2.426(5) 2_576 ?
Mo14 O133 1.678(6) . ?
Mo14 O102 1.914(5) . ?
Mo14 O105 1.927(6) . ?
Mo14 O334 1.954(6) . ?
Mo14 O289 2.005(5) . ?
Mo14 O191 2.308(5) . ?
Mo15 O174 1.659(6) . ?
Mo15 O127 1.907(5) . ?
Mo15 O35 1.940(6) . ?
Mo15 O26 1.963(6) . ?
Mo15 O84 1.999(5) . ?
Mo15 O43 2.331(5) . ?
Mo16 O130 1.681(6) . ?
Mo16 O65 1.900(5) . ?
Mo16 O325 1.946(6) . ?
Mo16 O333 1.974(6) . ?
Mo16 O138 1.999(6) . ?
Mo16 O178 2.307(5) . ?
Mo17 O150 1.653(6) . ?
Mo17 O54 1.856(5) . ?
Mo17 O57 1.865(6) . ?
Mo17 O272 1.990(5) . ?
Mo17 O19 2.074(5) . ?
Mo17 O41 2.436(5) . ?
Mo18 O241 1.678(5) . ?
Mo18 O126 1.919(5) . ?
Mo18 O92 1.930(6) . ?
Mo18 O161 1.977(6) . ?
Mo18 O63 1.995(5) . ?
Mo18 O47 2.322(5) . ?
Mo19 O60 1.671(6) . ?
Mo19 O53 1.775(5) . ?
Mo19 O43 1.939(5) . ?
Mo19 O41 1.975(5) . ?
Mo19 O84 2.108(5) . ?
Mo19 O19 2.468(6) . ?
Mo20 O313 1.676(6) . ?
Mo20 O277 1.909(6) . ?
Mo20 O52 1.933(6) . ?
Mo20 O117 1.987(6) . ?
Mo20 O259 2.009(6) . ?
Mo20 O116 2.334(6) . ?
Mo21 O260 1.712(6) . ?
Mo21 O358 1.746(7) . ?
Mo21 O123 1.837(5) . ?
Mo21 O163 2.058(5) . ?
Mo21 O164 2.102(5) . ?
Mo21 O382 2.313(8) . ?
Mo22 O282 1.676(7) . ?
Mo22 O173 1.847(6) . ?
Mo22 O232 1.865(7) . ?
Mo22 O62 1.980(7) . ?
Mo22 O263 2.069(5) . ?
Mo22 O225 2.432(6) . ?
Mo23 O294 1.669(6) . ?
Mo23 O173 1.906(6) . ?
Mo23 O304 1.940(6) . ?
Mo23 O276 1.978(6) . ?
Mo23 O138 2.001(6) . ?
Mo23 O85 2.335(6) . ?
Mo24 O128 1.683(6) . ?
Mo24 O291 1.920(6) . ?
Mo24 O120 1.942(6) . ?
Mo24 O195 1.968(7) . ?
Mo24 O289 1.996(5) . ?
Mo24 O146 2.346(6) . ?
Mo25 O234 1.681(6) . ?
Mo25 O252 1.908(6) . ?
Mo25 O242 1.934(6) . ?
Mo25 O180 1.962(6) . ?
Mo25 O184 1.995(6) . ?
Mo25 O101 2.335(6) . ?
Mo26 O158 1.673(6) . ?
Mo26 O193 1.902(6) . ?
Mo26 O171 1.945(6) . ?
Mo26 O230 1.970(6) . ?
Mo26 O83 2.000(6) . ?
Mo26 O224 2.324(5) . ?
Mo27 O166 1.685(6) . ?
Mo27 O277 1.846(6) . ?
Mo27 O242 1.865(6) . ?
Mo27 O302 2.000(6) . ?
Mo27 O256 2.077(6) . ?
Mo27 O101 2.449(6) . ?
Mo28 O340 1.665(8) . ?
Mo28 O405 1.766(7) . ?
Mo28 O364 1.800(7) . ?
Mo28 O91 2.038(6) . ?
Mo28 O44 2.069(5) . ?
Mo28 O290 2.375(7) . ?
Mo29 O152 1.710(6) . ?
Mo29 O215 1.731(7) . ?
Mo29 O96 1.816(6) . ?
Mo29 O231 2.061(6) . ?
Mo29 O269 2.096(5) . ?
Mo29 O299 2.342(7) . ?
Mo30 O376 1.677(7) . ?
Mo30 O244 1.980(7) . ?
Mo30 O384 1.992(6) . ?
Mo30 O362 2.002(6) . ?
Mo30 O239 2.022(6) . ?
Mo30 O22 2.098(6) . ?
Mo30 O222 2.227(6) . ?
Mo31 O372 1.757(8) . ?
Mo31 O392 1.773(7) . ?
Mo31 O432 1.775(7) . ?
Mo31 O262 2.053(5) . ?
Mo31 O27 2.077(6) . ?
Mo31 O407 2.290(7) . ?
Mo32 O118 1.699(7) . ?
Mo32 O346 1.746(8) . ?
Mo32 O276 1.816(5) . ?
Mo32 O366 2.073(6) . ?
Mo32 O62 2.103(7) . ?
Mo32 O417 2.340(8) . ?
Mo33 O316 1.694(7) . ?
Mo33 O370 1.745(6) . ?
Mo33 O211 1.832(6) . ?
Mo33 O330 2.074(7) . ?
Mo33 O275 2.095(5) . ?
Mo33 O335 2.354(8) . ?
Mo34 O389 1.667(8) . ?
Mo34 O186 1.922(6) . ?
Mo34 O207 1.940(7) . ?
Mo34 O446 1.975(7) . ?
Mo34 O177 2.006(6) . ?
Mo34 O266 2.327(6) . ?
Mo35 O317 1.662(8) . ?
Mo35 O404 1.998(6) . ?
Mo35 O393 2.002(7) . ?
Mo35 O268 2.007(5) . ?
Mo35 O324 2.010(6) . ?
Mo35 O137 2.093(6) . ?
Mo35 O314 2.214(7) . ?
Mo35 M3T 3.109(11) . ?
Mo36 O308 1.704(7) . ?
Mo36 O377 1.738(7) . ?
Mo36 O117 1.819(6) . ?
Mo36 O280 2.067(6) . ?
Mo36 O302 2.085(6) . ?
Mo36 O367 2.337(8) . ?
Mo37 O327 1.657(7) . ?
Mo37 O93 1.768(7) . ?
Mo37 O266 1.959(6) . ?
Mo37 O225 1.967(5) . ?
Mo37 O177 2.101(6) . ?
Mo37 O263 2.477(6) . ?
Mo38 O433 1.714(8) . ?
Mo38 O375 1.784(7) . ?
Mo38 O369 1.789(8) . ?
Mo38 O341 2.044(6) 2_576 ?
Mo38 O153 2.049(6) 2_576 ?
Mo38 O319 2.299(7) . ?
Mo39 O416 1.688(8) . ?
Mo39 O342 1.697(7) . ?
Mo39 O148 1.894(6) 2_667 ?
Mo39 O288 2.019(6) . ?
Mo39 O410 2.220(9) . ?
Mo39 O360 2.226(6) . ?
Mo40 O533 1.671(16) . ?
Mo40 O538 1.682(9) . ?
Mo40 O537 1.792(9) . ?
Mo40 O536 1.827(10) . ?
Mo40 O513 2.29(2) . ?
Mo40 O453 2.409(15) . ?
Mo41 O515 1.667(14) . ?
Mo41 O502 1.776(14) . ?
Mo41 O270 1.876(8) . ?
Mo41 O467 1.964(9) . ?
Mo41 O215 2.192(7) 2_667 ?
Mo41 O503 2.194(16) . ?
Mo42 O464 1.716(12) . ?
Mo42 O419 1.893(6) . ?
Mo42 O504 1.939(9) . ?
Mo42 O519 1.964(14) . ?
Mo42 O508 2.008(13) . ?
Mo42 O414 2.159(8) . ?
Mo43 O470 1.690(13) . ?
Mo43 O437 1.708(12) . ?
Mo43 O431 1.901(9) . ?
Mo43 O472 2.023(11) 2_576 ?
Mo43 O455 2.188(7) . ?
Mo43 O436 2.281(14) . ?
Mo44 O530 1.650(10) . ?
Mo44 O484 1.671(12) . ?
Mo44 O383 1.900(7) . ?
Mo44 O483 2.008(9) . ?
Mo44 O425 2.199(10) . ?
Mo44 O457 2.263(15) . ?
Mo45 O490 1.677(11) . ?
Mo45 O528 1.692(12) . ?
Mo45 O442 1.909(9) . ?
Mo45 O489 2.000(9) . ?
Mo45 O415 2.188(8) . ?
Mo45 O492 2.213(13) . ?
Mo46 O527 1.676(11) . ?
Mo46 O526 1.744(12) . ?
Mo46 O444 1.884(9) . ?
Mo46 O405 2.064(7) . ?
Mo46 O318 2.228(7) . ?
Mo46 O520 2.240(12) . ?
Mo47 O517 1.687(12) . ?
Mo47 O521 1.691(12) . ?
Mo47 O444 1.897(9) . ?
Mo47 O374 2.039(7) . ?
Mo47 O343 2.245(7) . ?
Mo47 O516 2.260(12) . ?
Mo48 O541 1.676(15) . ?
Mo48 O476 1.700(15) . ?
Mo48 O473 2.015(10) . ?
Mo48 O739 2.073(18) . ?
Mo48 O468 2.165(7) . ?
Mo48 O474 2.19(2) . ?
Mo51 O30 1.670(5) . ?
Mo51 O9 1.901(5) . ?
Mo51 O1 1.943(5) . ?
Mo51 O100 1.978(5) . ?
Mo51 O3 1.996(5) . ?
Mo51 O80 2.306(5) . ?
Mo52 O140 1.684(5) . ?
Mo52 O119 1.986(5) . ?
Mo52 O33 1.997(5) . ?
Mo52 O79 2.010(5) . ?
Mo52 O13 2.024(5) . ?
Mo52 O29 2.092(5) . ?
Mo52 O20 2.221(5) . ?
Mo53 O18 1.685(5) . ?
Mo53 O11 1.911(5) . ?
Mo53 O5 1.938(5) 2_667 ?
Mo53 O132 1.974(5) . ?
Mo53 O76 2.008(5) . ?
Mo53 O125 2.308(5) 2_667 ?
Mo54 O2 1.673(5) . ?
Mo54 O11 1.835(5) . ?
Mo54 O37 1.854(5) . ?
Mo54 O42 2.002(5) . ?
Mo54 O4 2.081(5) . ?
Mo54 O8 2.440(5) . ?
Mo55 O99 1.681(5) . ?
Mo55 O9 1.843(5) . ?
Mo55 O78 1.858(5) . ?
Mo55 O68 2.003(5) . ?
Mo55 O23 2.069(5) . ?
Mo55 O109 2.455(5) . ?
Mo56 O48 1.683(5) . ?
Mo56 O50 1.835(5) . ?
Mo56 O1 1.864(5) . ?
Mo56 O104 1.989(5) . ?
Mo56 O36 2.082(5) . ?
Mo56 O80 2.414(5) . ?
Mo57 O187 1.673(5) . ?
Mo57 O126 1.835(5) . ?
Mo57 O74 1.854(5) . ?
Mo57 O12 1.984(5) . ?
Mo57 O36 2.045(5) . ?
Mo57 O21 2.468(5) . ?
Mo58 O39 1.665(5) . ?
Mo58 O168 1.826(5) . ?
Mo58 O10 1.861(5) . ?
Mo58 O79 1.982(5) . ?
Mo58 O29 2.074(5) . ?
Mo58 O6 2.467(5) . ?
Mo59 O301 1.680(5) . ?
Mo59 O54 1.903(5) . ?
Mo59 O81 1.935(5) . ?
Mo59 O122 1.959(5) . ?
Mo59 O7 2.000(5) . ?
Mo59 O17 2.328(5) . ?
Mo60 O531 1.644(18) . ?
Mo60 O532 1.705(13) . ?
Mo60 O739 2.012(18) . ?
Mo60 O480 2.086(12) . ?
Mo60 O479 2.134(9) . ?
Mo60 O475 2.25(2) . ?
Mo61 O534 1.763(8) . ?
Mo61 O452 1.766(14) . ?
Mo61 O533 1.882(15) . ?
Mo61 O392 2.006(12) . ?
Mo61 O535 2.008(15) . ?
Mo61 O356 2.180(9) . ?
M3I O402 1.867(16) . ?
M3I O364 1.920(14) . ?
M3I O270 2.043(15) . ?
M3I O194 2.227(13) . ?
M3L O461 1.794(19) . ?
M3L O274 1.831(17) . ?
M3L O421 2.101(17) . ?
M3L O378 2.151(19) . ?
M3L O426 2.368(19) . ?
M3L C31 2.52(2) . ?
M3R O443 1.982(18) . ?
M3R O409 2.084(14) . ?
M3R O395 2.089(15) . ?
M3R C81 2.12(3) . ?
M3R O358 2.153(15) . ?
M3S O486 1.83(2) . ?
M3S O396 1.931(16) . ?
M3S C11 2.24(2) . ?
M3S O383 2.320(16) . ?
M3S O328 2.349(14) . ?
M3S M44 3.17(4) . ?
M3T O783 1.77(2) . ?
M3T O780 1.87(3) . ?
M3T O404 1.958(13) . ?
M3T O393 2.011(13) . ?
M3T O480 2.094(17) . ?
M3T O483 2.186(18) . ?
M3U O825 1.73(2) . ?
M3U O432 1.931(12) . ?
M3U O395 2.104(13) . ?
M3U O380 2.253(11) . ?
M3U C81 2.42(2) . ?
M3W O799 1.76(2) . ?
M3W O756 2.06(2) . ?
M3W O421 2.151(12) . ?
M3W O370 2.218(11) . ?
M3W C31 2.359(19) . ?
M3X O523 1.689(12) . ?
M3X O413 1.971(11) . ?
M3X O387 2.085(10) . ?
M3X O303 2.393(9) . ?
M3X C91 2.489(18) . ?
M3X O398 2.510(11) . ?
M39 O342 1.749(12) . ?
M39 O288 1.880(11) . ?
M39 O148 2.082(11) 2_667 ?
M39 O360 2.254(12) . ?
M39 O416 2.383(12) . ?
M39 C101 2.586(15) . ?
M40 O538 1.754(13) . ?
M40 O813 1.92(2) . ?
M40 O533 1.952(12) . ?
M40 O836 2.04(3) . ?
M40 O453 2.171(9) . ?
M40 O537 2.178(16) . ?
M41 O815 1.79(2) . ?
M41 O467 1.976(12) . ?
M41 O270 2.002(12) . ?
M41 O215 2.223(10) 2_667 ?
M43 O472 1.725(17) 2_576 ?
M43 O470 1.904(18) . ?
M43 O455 2.247(13) . ?
M43 O431 2.363(16) . ?
M43 C21 2.57(3) . ?
M44 C11 1.84(4) . ?
M44 O784 1.96(5) . ?
M44 O483 1.97(4) . ?
M44 O383 2.43(4) . ?
M44 O783 2.52(5) . ?
M46 O405 1.935(14) . ?
M46 O444 2.131(15) . ?
M46 O527 2.398(15) . ?
M46 O318 2.407(13) . ?
M47 O516 1.538(15) . ?
M47 O521 1.593(16) . ?
M47 O374 2.017(13) . ?
M47 O444 2.057(14) . ?
M47 O343 2.396(12) . ?
M47 O517 2.465(15) . ?
M47 C71 2.56(2) . ?
M48 O476 1.847(18) . ?
M48 O473 1.938(14) . ?
M48 O439 1.999(18) . ?
M48 O468 2.224(13) . ?
M48 C61 2.29(3) . ?
M60 O475 1.28(3) . ?
M60 O532 1.79(2) . ?
M60 O480 1.957(14) . ?
M60 O439 1.997(18) . ?
M60 O780 2.15(3) . ?
M60 O479 2.310(14) . ?
M60 C61 2.32(3) . ?
M61 O534 1.62(2) . ?
M61 O452 1.63(2) . ?
M61 O533 1.82(3) . ?
M61 O392 2.20(2) . ?
M61 O535 2.20(2) . ?
M61 O356 2.397(18) . ?
O351 C101 1.297(13) 2_667 ?
O406 C91 1.34(2) . ?
O410 C101 1.264(14) . ?
O423 C31 1.32(2) . ?
O429 C51 1.38(4) . ?
O436 C21 1.43(3) . ?
O450 C11 1.28(2) . ?
O457 C11 1.11(2) . ?
O458 C81 1.576(18) . ?
O474 C61 1.45(2) . ?
O475 C61 1.45(2) . ?
O480 O780 0.70(2) . ?
O483 O783 0.80(2) . ?
O492 C1 1.268(19) . ?
O495 C21 1.36(3) . ?
O501 C31 1.31(2) . ?
O516 C71 1.31(2) . ?
O518 C81 1.569(18) . ?
O519 C51 1.54(4) . ?
O520 C71 1.33(2) . ?
O524 C91 1.35(2) . ?
O529 C1 1.234(18) . ?
C1 C2 1.490(10) . ?
C2 N0 1.433(10) . ?
C2 C3 1.476(10) . ?
C11 C12 1.500(10) . ?
C12 N1 1.442(10) . ?
C12 C13 1.495(10) . ?
C21 C22 1.513(10) . ?
C22 N2 1.449(10) . ?
C22 C23 1.501(10) . ?
C31 C32 1.494(10) . ?
C32 N3 1.429(10) . ?
C32 C33 1.487(10) . ?
C51 C52 1.500(10) . ?
C52 N5 1.438(10) . ?
C52 C53 1.493(10) . ?
C61 C62 1.508(10) . ?
C62 N6 1.442(10) . ?
C62 C63 1.488(10) . ?
C71 C72 1.507(10) . ?
C72 N7 1.460(10) . ?
C72 C73 1.510(10) . ?
C81 C82 1.507(10) . ?
C82 N8 1.425(10) . ?
C82 C83 1.488(10) . ?
C91 C92 1.493(10) . ?
C92 N9 1.427(10) . ?
C92 C93 1.506(10) . ?
C101 C102 1.500(9) . ?
C102 N10 1.461(10) . ?
C102 C103 1.468(9) . ?
